CLUSTER MODEL INTERRELATION WITH MODERN PHYSICAL CONCEPTS No part of this digital document may be reproduced, stored in...

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

CLUSTER MODEL INTERRELATION WITH MODERN PHYSICAL CONCEPTS No part of this digital document may be reproduced, stored in a retrieval system or transmitted in any form or by any means. The publisher has taken reasonable care in the preparation of this digital document, but makes no expressed or implied warranty of any kind and assumes no responsibility for any errors or omissions. No liability is assumed for incidental or consequential damages in connection with or arising out of information contained herein. This digital document is sold with the clear understanding that the publisher is not engaged in rendering legal, medical or any other professional services.

CLUSTER MODEL INTERRELATION WITH MODERN PHYSICAL CONCEPTS

G. V. KOZLOV AND

G. E. ZAIKOV

Nova Science Publishers, Inc. New York

Copyright © 2009 by Nova Science Publishers, Inc.

All rights reserved. No part of this book may be reproduced, stored in a retrieval system or transmitted in any form or by any means: electronic, electrostatic, magnetic, tape, mechanical photocopying, recording or otherwise without the written permission of the Publisher. For permission to use material from this book please contact us: Telephone 631-231-7269; Fax 631-231-8175 Web Site: http://www.novapublishers.com NOTICE TO THE READER The Publisher has taken reasonable care in the preparation of this book, but makes no expressed or implied warranty of any kind and assumes no responsibility for any errors or omissions. No liability is assumed for incidental or consequential damages in connection with or arising out of information contained in this book. The Publisher shall not be liable for any special, consequential, or exemplary damages resulting, in whole or in part, from the readers’ use of, or reliance upon, this material. Independent verification should be sought for any data, advice or recommendations contained in this book. In addition, no responsibility is assumed by the publisher for any injury and/or damage to persons or property arising from any methods, products, instructions, ideas or otherwise contained in this publication. This publication is designed to provide accurate and authoritative information with regard to the subject matter covered herein. It is sold with the clear understanding that the Publisher is not engaged in rendering legal or any other professional services. If legal or any other expert assistance is required, the services of a competent person should be sought. FROM A DECLARATION OF PARTICIPANTS JOINTLY ADOPTED BY A COMMITTEE OF THE AMERICAN BAR ASSOCIATION AND A COMMITTEE OF PUBLISHERS. LIBRARY OF CONGRESS CATALOGING-IN-PUBLICATION DATA Kozlov, G. V. Cluster model interrelation with modern physical concepts / G.V. Kozlov & G.E. Zaikov. p. cm. Includes index. ISBN 978-1-60741-684-5 (E-Book) 1. Polymers--Structure. I. Zaikov, Gennadii Efremovich. II. Title. QC173.4.P65K69 2009 547'.7--dc22 2008047189

Published by Nova Science Publishers, Inc. + New York

CONTENTS

Chapter 1

Fractality of the Polymer Structure and the Cluster Model 1

Chapter 2

Clusters as Dissipative Structures

13

Chapter 3

Cluster and Fluctuation Free Volume Models

35

Chapter 4

The Cluster Model and the Anharmonicity Concept

41

Chapter 5

Cluster Structure as a Percolation System

47

Chapter 6

Cluster model as the Model of Irreversible Aggregation

63

References

87

Index

97

Chapter 1

FRACTALITY OF THE POLYMER STRUCTURE AND THE CLUSTER MODEL During recent 20 years methods of fractal analysis were widely spread in theoretical physics [1] and general material science [2], in physicochemistry of polymers [3 – 8], in particular. This tendency is explained by a broad spreading of fractal objects in the nature. There are two basic factors determining interrelation between the local order and fractal origin of the polymer solid phase: thermodynamic non-equilibrium and dimensional periodicity of the structure. A simple relation between the non-

~ im

equilibrium index, which is the Gibbs function variation, ΔG , at polymer selfassembly (the cluster structure formation), and a relative part of clusters, ϕcl, as follows:

~ ΔG im ~ ϕcl.

(1)

Figure 1 shows graphical presentation of this relation for amorphous glassy

~ im

= 0 [10, 11], the relation (1) PC and PAr polymers. Since at Т = Тg(Tm) ΔG indicates necessary complete decomposition of the cluster system (ϕcl = 0) at these temperatures or transition to thermodynamically equilibrium structure. As for interrelation between fractality and thermodynamic non-equilibrium, Hornbogen [12] has indicated that exactly thermodynamically non-equilibrium processes form fractal structures. The classic example of this regularity fulfillment is represented by fracture surfaces of solids: many experimental researches have indicated their fractality independently of thermodynamic conditions of the solid

2

G. V. Kozlov and G. E. Zaikov

itself [12]. This is stipulated by thermodynamic non-equilibrium of the degradation process [13]. This very fact does also determine experimentally proved fractality of the polymer structure [14 – 16]. Similar to every real (physical) fractal, fractal properties of the polymer structure are limited by definite linear scales. For example, in works [14, 17] these scales are limited by several angstroms (the lower limit) to several ten angstroms (the upper limit). The lower limit is associated with the finite size of structural elements and the upper limit with irregular approaching the limit of the fractal dimensionality of the structure, df [18]. The above-mentioned scales are in good keeping with the border dimensions of the cluster structure: the lower with the static segment length, lst, and the upper with the distance between clusters, Rcl [19]. In these scales, fractality of the polymer structure assumes dependence of density, ρ, on scale, L, of the following shape (Figure 2) [1]: d f −d

ρ~L

,

(2)

where d is dimensionality of the Euclidean space, to which the fractal is inserted.

Figure 1. Dependence of the relative cluster part, ϕcl, on the absolute value of specific Gibbs function for non-equilibrium phase transition

ΔG im

for PC (1) and PAr (2) [8]

Fractality of the Polymer Structure and the Cluster Model

3

Figure 2. Dependence of density ρ on linear scale L for a solid in double logarithmic coordinates. Fractal behavior is observed in the Lmin-Lmax range [18]

Figure 3. Schematic presentation of the cluster structure of the polymer amorphous state [5]

Figure 3 presents schematic image of the cluster structure of the polymer amorphous state. Clearly within the borders of the above-mentioned dimensional periodicity data in Figures 2 and 3 correspond to one another, i.e. the cluster model suggests ρ decrease with removing from the cluster center. At the same time, the Flory “felt” model [20] does not fit this criterion (for it ρ = const). Since fractality of the polymer structure was proved in experiments [14 – 16], it is

4

G. V. Kozlov and G. E. Zaikov

obvious that the cluster model conforms to the structure of real solid polymers, whereas the “felt” model does not correspond to it. Obviously the reverse dependence for final ρ is also true: ρ variation in definite limits necessarily suggests structure periodicity. However, one should remember that fractal analysis gives just general mathematical description of polymers, i.e. it does not identify structural units (elements), from which any real polymer is formed. Physical description of thermodynamically non-equilibrium polymer structure in the framework of the local order ideas gives the cluster model of the polymer amorphous state structure that quantitatively identify its elements. Since these models consider the polymer structure somewhat from two sides, they are excellent completing one another [21]. It is common knowledge [22] that structures displaying fractal behavior on small length scale and being homogeneous on large length scale are named homogeneous fractals. These fractals are percolation clusters at the percolation threshold [1]. As shown below, the cluster structure represents the percolation system and, due to the above-said, the homogeneous fractal. To put it differently, the presence of the local order in the condensed phase of polymers determines fractality of their structures. Fractal dimensionality, df, of the percolation system can be expressed by the equation as follows [22]:

df =d−

βp νp

,

(3)

where βp and νp are critical indices in the percolation theory. Table 1. Percolation cluster characteristics [5] Parameter

βp νp βp/νp df

Experimentally determined indices EP-1 EP-2 0.54 0.58 1.20 1.15 0.45 0.504 2.55 2.50

Theoretical “configuration” indices [22] 0.40 0.88 0.455 2.545

Fractality of the Polymer Structure and the Cluster Model

5

As a consequence, the condition βp ≠ 0 that follows from Table 1 does also determine fractality of the polymer structure. Obviously this condition and, consequently, fractality of the polymer structure determined temperature dependence of ϕcl, e.g. thermofluctuation origin of the local order. To put it differently, the structure fractality and the local order “frozen” below Tg (ϕcl = const) represent mutually exclusive notions. The above-considered statements allow binding the fractal dimension, df, and local order characteristics (ϕcl or υcl) by an analytical relation. The following equation binds df value to the Poisson coefficient ν [18]: df = (d – 1)(1 + ν);

(4)

in its turn, ν value is associated with νcl. Equation (4) allows obtaining of the interconnection between df and ϕcl or νcl as follows:

⎛ ϕ df = 1.5(d – 1) – 3.22(d – 1)×10 ⎜⎜ cl ⎝ SC ∞ -10

12

⎞ ⎟⎟ ⎠

,

(5)

or df = 1.5(d – 1) – 3.22(d – 1)×10-10(l0νcl)1/2.

(6)

These expressions, most frequently used for the case d = 3, are reduced to the simple form as follows [4]:

⎛ ϕ df = 3 – 6.44×10 ⎜⎜ cl ⎝ SC ∞ -10

12

⎞ ⎟⎟ ⎠

,

(7)

or df = 3 – 6.44×10-10(l0νcl)1/2.

(8)

Turning back to correlation (5.1), note that its substitution into equation (5) or (7) allows obtaining of the following expression (for d = 3) [9]:

6

G. V. Kozlov and G. E. Zaikov

(

~ ΔG im ~ C ∞ S 3 − d f

)2 .

(9) ~ im

The Gibbs specific function of supermolecular structure formation, ΔG , is given for non-equilibrium “overcooled liquid – solid” phase transition [11]. As

~ im

follows from the relation (9), ΔG = 0 at df = 3, e.g. at df = d and transition to the Euclidean behavior. To put it differently, fractal structures are induced by nonequilibrium processes only, as it has been assumed before [12]. One more noteworthy analogy can be traced between glassy polymers and homogeneous fractals. It is known [23] that the mentioned polymers do not fit the Prigozhine-Defye criterion that means that to be described they require more than one order parameter. Concerning Euclidean objects (spaces), they possess translational symmetry and, consequently, require one parameter to be described, namely, the Euclidean dimensionality d [24]. Fractal objects (spaces) possess dilatation symmetry and, therefore, require three dimensionalities for characterization: the Hausdorff df, spectral ds, and d. Even if in the latter case d is assumed constant and equal 3, correct description of the fractal requires, at least, two dimensionalities: df and ds. Even this qualitative comparison proves fractality of the glassy polymer structure. General ideas for the benefit of the local order existence in polymers were considered based on the Ramsey theorem [18, 21]. By analogy, it can be proved that any structure consisting of N elements (N > BN(i)) represents an aggregate of a finite number k ≤ j of self-similar structures enclosed in one another, the Hausdorff dimensionality of which, in general, can be different. This means that any structure consisting of quite large number of elements, independently of its physical origin, represents a multifractal (fractal, in particular) and is characterized by a spectrum of Regnier dimensionalities dq, q = 0, 1, 2, … [18]. It has been shown [25] that the tendency of condensed systems to self-organization in the scale-invariant multifractal forms originate from the fundamental thermodynamic principles of open systems, and dq is determined by the competition of short- and long-range interatomic correlations, which determine volumetric compressibility and shear rigidity of solids, respectively. As mentioned above, the cluster model and the fractal analysis are complement approaches and their combined application discloses new possibilities for simulation of the polymer structure. This point is considered on the example of forecasting parameters of polymer network cluster structure [26]. It is known [27 – 29] that computer simulation of the processes has induced a conclusion that in the gel-formation point cross-linked backbones of these

Fractality of the Polymer Structure and the Cluster Model

7

polymers represent fractal structures, cross-linking frequency increase inducing an increase of the fractal dimensionality of such backbone. However, from positions of practice the cross-linking frequency is not suitable enough, though at the present time polymer networks are preferably characterized using the value νnw [30]. Nevertheless, it has been shown [31] that at constant νnw for one and the same polymer network, different properties (for example, different Tg) can be obtained. This is explained by the change of supermolecular (cluster) structure of polymer network during physical aging, namely, by increase of the local order degree [31]. In its turn, the local order degree determines df value (equations (5) – (8)). Thus there occurs a possibility of forecasting structural characteristics (and as a consequence properties) of polymer networks in the glassy state basing on chemical cross-linking degree in the gel formation point. One of possible alternatives of solving this problem was discussed [32] on the example of typical representatives of the polymer network class – epoxy polymers of amine (EP-1) and anhydride (EP-2) cross-linking type, as well as their homologues solidified under pressure of 200 MPa (EP-1-200 and EP-2-200). The relation between νnw and df of studied EPs was deduced on the basis of the model suggested in the work [33]. The essence of this model is as follows. Competing processes of crystal growth and nucleation were described in the framework of two kinetic equations [33]: dR/dt = k1cm,

(10)

dN/dt = k2cp,

(11)

where R is the crystal dimension; t is the current time; k1 and k2 are equilibrium constants; N is the number of crystals; c is the concentration of molecules at the surface; m and p are indices. The application of equations (10) and (11) to description of the local order zones (clusters) nucleation and growth in EP is based on the fact that clusters in itself represent analogues of crystallites with extended chains (CEC) [34]. The characteristic size of cluster is accepted equal the length of segments in it, i.e. the statistic segment length lst. Similar to [33], m =1, because cluster growth represents addition of a single segment with the length lst [35]; therefore, p > 1, because cluster nucleation requires occurrence of two or more segments in the nucleation point. However, application of the equation (10) to a single separate EP requires sufficient modification. Obviously, if R = lst is accepted, the equation (10) becomes meaningless, because for every studied EP lst = const and dlst/dt = 0. The latter means that clusters has not the ability to grow. That is why, denoting the

8

G. V. Kozlov and G. E. Zaikov

number of segments in a single cluster by nseg, the equation (10) will be presented as follows [32]:

dn seg dt

= k1c .

(12)

The border value of nseg is limited by nucleation of new clusters of the thermofluctuation origin. That is why [33]:

l st =

(dnseg dt ) . (dN

dt )

(13)

Obviously the part of segments of macromolecules, c, capable of forming clusters must be decreased with time during the cluster formation and, taking into account the condition lst = const for every EP, nseg must also be decreased. This fact explains the presence of unstable (possessing low nseg) clusters in the structure of the polymer amorphous state [36, 37]. This also explains selfsimilarity of the cluster structure in the scale range of its existence. Note back again the important circumstance that the system of equations (10) and (11) can be applied to the totality of studied EPs, and the system of equations (11) and (12) is applicable to any separate EP of the totality [32]. For the totality of studied EPs, one can write down the following equations [33]:

N (l st ) = (dN cl dt )t gel ,

(14)

and

l st ~

(dl st dt ) , (dN cl dt )

(15)

where Ncl is the number of clusters; tgel is the time interval of the gel formation. The relation (15) forecasts C∞ decrease with cross-linking frequency, νnw, increase and consequent lst decline. This intensifies nucleation of new clusters, i.e. Ncl increase. Assuming R = lst, m = 1 and dividing equation (10) by (11), the following correlation is obtained:

Fractality of the Polymer Structure and the Cluster Model

l st ~

dl st dt c ~ p = c1− p , dN cl dt c

9

(16)

because k1 and k2 are constants. The equation (14) combined with the expression (11) under the conditions tgel = const, k2 = const and, as before, N = Ncl, gives the following correlation: Ncl(lst) = k2tgelcp,

(17)

or with regard to k2tgel = const: Ncl(lst) ~ cp.

(18)

Equations (10) and (11) allow determination of c as follows: −1 /( p −1)

c ~ l st

,

(19)

and 1/ p

c ~ N cl .

(20)

Making equal the right parts of equations (19) and (20), it is obtained that [32]: 1/ p −1 /( p −1) N cl ~ l st

(21)

or − p /( p −1)

Ncl(lst) ~ l st

.

(22)

It has been indicated [33] that the classic nucleation theory requires р ≤ 2 and, consequently, the condition occurs as follows:

p ≥ 2. p −1

(23)

10

G. V. Kozlov and G. E. Zaikov

Moreover, there is one more restriction that states that the volume of clusters must not exceed total volume of the polymer, wherefrom one more condition follows [33]:

p ≤ 3. p −1

(24)

Thus index in the relation (22) falls within the same limits as the fractal dimensionality of the object in the three-dimensional space [34]. The accurate interrelation between p/(p – 1) and df can be obtained from comparison of the expression (22) with the ones deduced in the work [39]: −d f

Ncl(lst) ~ l st

,

(25)

therefore [32]: p/(p – 1) = df.

(26)

The value Ncl can be presented as follows [34]:

N cl =

2ν Vcl = cl . n seg F

(27)

One more important circumstance shall be mentioned. The comparison of equations (11) and (25) indicates that the maximal rate of the cluster formation is reached at p =2 or df = 2.To put it differently, it is assumed that the minimal fractal dimensionality of the polymer structure is corresponded to the maximal local order. In the framework of the cluster model [34] polymer network can be considered as a superposition of two carcasses – chemical cross-link network and physical entanglement cluster network possessing frequencies νnw and νcl, respectively. As each of these carcasses is accepted as the ideal structure (i.e. the effect of end chains is neglected), one can write down as follows [40]:

M ceff =

Mc f , 2

(28)

Fractality of the Polymer Structure and the Cluster Model

11

eff

where M c is the effective molecular mass of a chain part between chemical cross-link points; Mc is the value of the latter; f is the functionality of chemical cross-link point. With regard to equations (27) and (28), the relation (25) can be reduced to the following form [32]:

2ν nw −d ~ l st f . f

(29)

An equation linking parameters С∞ and df for d = 3 was deduced [41]. Full deduction and complete form of this equation will be given in the following Section:

⎛ df 4⎞ + ⎟. C∞ = ⎜ ⎜33−d f 3 ⎟⎠ ⎝

(

)

(30)

Combined equations (29) and (30) give the following expression [32]:

d l0 f

⎛ df 4⎞ ⎜ + ⎟ ⎜ 3(3 − d f ) 3 ⎟ ⎝ ⎠

df

= 3.75 × 10 28

f

ν nw

,

(31)

where the empirical numerical coefficient in the right part of the equation is obtained by equaling df values, calculated from equations (4) and (31), at νnw = 1027 m−3 [32]. Figure 4 compares df values, calculated by equations (4) and (31) as the function of νnw, for studied EPs under the conditions l0 = 1.25 Å [5] and f = 4. Clearly good correspondence of two selections of the fractal dimensionalities was obtained. This means that the increase of the carcass fractal dimensionality before the gel formation point [29] induces a decrease of the fractal dimensionality df of the supermolecular structure of polymer network in the glassy state. It should be noted also that knowledge of df allows the forecast of EP properties [35, 42]. Thus varying Kst or terminating the reaction at a definite stage, one can obtain polymers with required properties. However, from positions of practical significance, application of stoichiometric values Kst = 1.0 is more preferable. It gives the most stable systems [18], including polymer networks [35]. In this case, properties of

12

G. V. Kozlov and G. E. Zaikov

the final product can be varied by changing functionality of the cross-linking agent, f, or molecular characteristics of epoxy oligomer. Thus fractal analysis application allowed clearing up an interrelation between polymer network characteristics before the gel formation point (or at it) and in the glassy state. Note that this can be made for just synthesized polymer only. Further on, df will vary due to physical aging processes, unavoidable due to thermodynamically non-equilibrium origin of the polymer glassy state. Nevertheless, the methodology suggested allows forecast of properties of glassy polymer networks already at the cross-linking stage. Moreover, the model considered forecasts qualitatively previously expected effects, namely, the existence of unstable clusters [36, 37], self-similarity of the cluster structure [5, 34] and df decrease with the local ordering increase. For a brief resume, it should be noted that in the case of glassy polymers, notions of the local order and fractality are tightly connected basing on the fundamental ideas of physics. This interrelation is expressed by simple analytical equations (5) - (8). It is also shown that combined application of these complement concepts allows significant broadening and improvement of the analytical description of the polymer structure and properties. The mentioned combination will be multiply used in the future discussion.

Figure 4. Dependence of fractal dimensionality, df, of EP structure on cross-linking frequency, νnw, calculated as follows: by equation (4) for EP-1 (1), EP-2 (2), EP-1-200 (3) and EP-2-200 (4), and by equation (5.31) for all EPs [32]

Chapter 2

CLUSTERS AS DISSIPATIVE STRUCTURES Obtaining of relations between structure and properties of polymers was always the foreground task of the polymer physics. However, solution of this problem is significantly complicated by the presence of a multilevel structure in polymers – molecular, topological, supermolecular (super-segmental), etc. That is why a polymer structural model is required, which would allow association of structural parameters of the mentioned levels by quantitative relations. Obviously such relations should better be deduced on the basis of fundamental physical principles. Recent rapid development of synergism of non-equilibrium systems [43, 44] and fractal analysis allows application of these fundamental concepts to solution of the tasks mentioned, because a solid-phase polymer represents thermodynamically highly non-equilibrium system. The basic feature differing polymers from other classes of solids is their structure, composed of long chain molecules. That is why the assumption seems natural that the structural hierarchy of polymers must be based on their molecular structure. Recently, the characteristic relation С∞ [45 - 47] is more and more frequently used as the molecular parameter for description of polymer properties, hence substituting, for example, such characteristics as relation а/δ (where a in the chain “thickness” and δ is its rigidity [48]). To the point of view of Boyer and Miller [48], this is stipulated by higher uncertainty of δ compared with С∞, because the former depends upon valence angles of bonds in the macromolecule and the latter on the length of these bonds. Usually, bond lengths are determined with significantly higher accuracy than the valence angles. Not contradicting to the rightfulness of such conclusion, nevertheless, the authors assume that the reasons for broad application of С∞ parameter are much deeper and fundamental; one of the objectives of the current Section is demonstration of declared

14

G. V. Kozlov and G. E. Zaikov

fundamentality of С∞ in the framework of thermodynamics of non-equilibrium processes [43, 44]. The behavior of a deformable solid subject to mechanical impact is determined by formation (decomposition) and evolution of dissipative structures (DS) providing for the optimal mode of supplied energy dissipation [18, 25, 49]. This general statement is also true for polymers. Broad application of polymers as construction materials requires the detail study of their mechanical properties which is impossible without understanding of fundamental processes, on which their behavior under load is based. At present, it is known well that polymers possess a local order that exists in them in the form of dissipative structures (DS) [50 – 52]. However, direct application of fundamental principles of thermodynamics and statistical physics of non-equilibrium processes to the study of behavior of any class of materials is often quite difficult or even impossible without knowing particular quantitative model of the structure of this material. For such model, the cluster model of the polymer amorphous state will be used below. As shown [18, 49], the feature of DS, also formed in polymers [50 – 52], is existence of a universal hierarchy of spatial scales (structural levels), which is reflected in the hierarchy of linear sizes of the structure. For example, even in elastically isotropic bodies, at least, three independent length scales do exist: lp, lε, and le, bound with one another by the following relations [49]: lp = aM; lε = aMΛ0; le = lεΛ1,

(32)

where aM is the linear size; Λ0 and Λ1 are self-similarity coefficients. At personification of these length scales related to polymers the atomic level must be neglected, because polymer represents a solid consisting of long chain macromolecules which, in turn, are composed of various groups of atoms. That is why the minimum scale, aM, in equation (32) for polymers must be the length of the macromolecule backbone, l0, varied within the range of several angstroms [45, 53]. Then the next higher structural (segmental) level will be determined by the statistical segment length, lst. As a consequence, for this structural level, the selfsimilarity coefficient Λ0 = С∞ under the condition lp = l0 [5, 41, 54, 55]. Topological level is the consequent structural level in polymers. Its parameters are determined by characteristics of macromolecular entanglement (“hooking”) network in linear polymers and by parameters of chemical cross-link network in polymer networks. For this level, the distance between entanglements or chemical cross-link points, Rnw, is the typical linear scale, le.

Clusters as Dissipative Structures

15

As a consequence, it follows from the above discussion that if for the consequent structural levels the self-similarity coefficient value (Λ0 = С∞) is preserved, then for polymers the equation (32) can be reduced to the following form [5, 55]: 2

lp = l0; lε = lst = l0C∞; le = Rnw = l 0 C ∞ .

(33)

( ) 2

Figure 5 shows dependence Rnw C ∞ , which is linear and passes through the origin of coordinates, though it is fractioned into two straight lines. We are not to analyze the latter circumstance, though it should be mentioned that there are some obvious reasons for it, among which the following are: firstly, broad dispersion of parameters from the literature (l0, С∞, νnw) [45, 53], required for calculation; secondly, there are different approaches to interpretation of the value lε = lst [45, 2

53]. Nevertheless, proportionality of Rnw and C ∞ , shown in Figure 5, proves that C∞ is the self-similarity coefficient at DS-size scale transition from lst to Rnw.

Figure 5. Dependence of the distance between entanglements (chemical cross-link points), Rnw, on the square characteristic relation, C∞, for amorphous glassy (1) and amorphouscrystalline (2) polymers, and polymer networks (3) [5]

Figure 6 compares Rnw values, calculated from equation (33) (Rnw1 and Rnw2, respectively). Data from the Figure indicate tight quantitative conformity between Rnw1 and Rnw2 for the majority of polymers. Possible reasons for occurrence of two lines have been already discussed. Thus C∞ is regulated by the polymer topology, which can be changed by variation of νnw. For a great number of linear polymers,

16

G. V. Kozlov and G. E. Zaikov

Aharoni [53] has observed Rnw increase with the chain flexibility (C∞ increase), expressed by the following equation: Rnw = 10C∞.

(34)

For cross-linked polymers, similar equation as follows was obtained [56]: Rnw = 5C∞.

(35)

Figure 6. The relation between inter-entanglement (between chemical cross-link points) distances, Rnw1 and Rnw2 calculated from the equation (33), for amorphous glassy (1) and amorphous-crystalline (2) polymers, and polymer networks (3) [5]

One more specific length scale, which is the chain part length between entanglements or chemical cross-link points, Lc, does exist in polymers. It can be determined from the equation as follows [5]:

Lc =

F 2ν c S

.

(36)

Figure 7 shows the dependence of “transitional” chain length between 3

entanglements (cross-link points), Lc, calculated by equation (36), on C ∞ . It was also found linear and passing through the origin of coordinates. Expectedly, the straight line slope equals ~1 Å, i.e. possesses the order of magnitude of l0 [53]. This indicates that for this structural level, typical of polymers, C∞ represents the self-similarity coefficient [54, 55].

Clusters as Dissipative Structures

17

DS evolution on the example of polymer networks during their deformation will be considered below using the cluster model for the structure personification. It has been shown [21] that elastic deformation of amorphous polymers is specifically realized in clusters, and the yield stress is the function of entanglement cluster network frequency, νcl, only, i.e. the number of closely packed segments per specific polymer volume [57]. In the light of these facts the yielding can be considered as stability loss by clusters in the field of mechanical stresses. Cold flow of the polymer is considered as deformation of devitrified packless matrix, in which chemical cross-links are represented by clusters [57]. Such interpretation allows personification of structural changes proceeding at polymer deformation in the framework of the model [18, 21, 25].

Figure 7. Dependence of macromolecule segment length between entanglements (chemical cross-link points), Lc, on cubic characteristic relation,

C ∞3 , for amorphous glassy (1) and

amorphous-crystalline (2) polymers, and polymer networks (3) [5]

As mentioned above, the feature of DS formed (or existing) in deformed solid is existence of the universal hierarchy of structural levels [25]. As Balankin has suggested [18, 49], the hierarchic structure of DS is based on the fundamental property of solids, the shearing stability that determines the difference of typical spatial scales of localization zones and dissipation of energy “injected” to deformed body under external impact. Typical scale of the zones (ls), in which excessive energy is dissipated, is proportional to the shear modulus, G. Since in accordance with the above discussion, in the framework of the cluster model, these zones can be associated with the clusters, it is suitable to use their characteristic size, lst, as ls. Figure 5.8 shows relation between G and lst, which is

18

G. V. Kozlov and G. E. Zaikov

approximated by a straight line passing through the origin of coordinates. This proves correctness of lst use for ls.

Figure 8. Relation between statistical segment length, lst, and shear modulus, G, for EP-1 (1), EP-2 (2), EP-1-200 (3) and EP-2-200 (4) [5]

Concerning the next stage in the hierarchy of the structural levels, taking into account the above-mentioned interpretation of the cold flow process and equation (33), the distance between clusters, Rcl, should be taken for ls. The typical size of injected energy localization zones, le, is proportional to (В + 4/3G), where B is the uniform compression modulus [49]. The possibility of associating Rcl with le can be checked as follows. It is known [49] that the relation of DS spatial scales of DS

neighbor structural levels, Li

DS

and Li +1 , can be expressed by the following

equation:

LiDS +1 LiDS

=

l e B + 4 / 3G = = Λi , ls G

(37)

where Λi is the self-similarity coefficient. Obviously le can be obtained by multiplying (В + 4/3G)/G by ls, which equals lst. The relation between le and (В + 4/3G), shown in Figure 9, was also found linear that proves principal possibility of using parameter le as the characteristic dimension of injected energy localization zones. However, at the structural level

Clusters as Dissipative Structures

19

this assumption can be finally proved by comparison of le and Rcl. It displayed the presence of correspondence between these parameters, but also indicated systematic exceeding of Rcl over le by, approximately, 8 Å. The relation observed between le and Rcl is explained on the basis of schematically depicted cluster structure of amorphous polymers, shown in Figure 10. Obviously for obtaining le, the mentioned decrease of Rcl by 8 Å, which is approximately equal lst, means that injected energy is localized not in the whole volume of the polymer, but in the packless matrix, because cluster with the characteristic dimension lst is excluded from the consideration.

Figure 9. Correlation between characteristic dimensions of injected energy localization zones, le, and parameter (В + 4/3G). For the legend, refer to Figure 8 [5]

Figure 10. Schematic presentation of the cluster structure of amorphous polymer [5]

20

G. V. Kozlov and G. E. Zaikov

Comparison of le and Rcl – lst values, shown in Figure 11, proves this conclusion. As a consequence, structural characteristics lst and Rcl – lst estimated in the framework of the cluster model, considered as spatial scales of DS in neighboring levels, allow assessment of the self-similarity coefficient of polymer mechanical deformation, Λi, from the equation (37). The interrelation of DS scales and injected energy localization processes allow an assumption of a definite correlation between Λi and dimensionality, Df, of excessive energy localization zones in elastically deformable medium [18]. Parameter Df value can be determined from the following equation [18]:

Df =

2(1 − ν ) . 1 − 2ν

(38)

Figure 11. Correlation between characteristic size of injected energy localization zone, le, and Rcl – lst value. For the legend, refer to Figure 8. Straight line marks 1 : 1 relation [5]

Figure 12 shows comparison of Df and the self-similarity coefficient, Λi, for polymer networks. Clearly both absolute values and tendencies of changes of these parameters conform well. Analogous correlation between Rcl and Df – lst was obtained [58] for amorphous, amorphous-crystalline and oriented polymers. As a consequence, in the framework of thermodynamics of non-equilibrium processes, yielding and cold flow processes are described well; the cluster model describes structure of these materials properly. Obviously clusters are identified as DS [5, 54, 55]. Basing on the above-stated, one may suggest that Λi in the equation (37) also equals C∞. Then this equation can be reduced to the following form [5, 41]:

Clusters as Dissipative Structures

B 4 + = C∞ . G 3

21

(39)

In their turn, B and G can be expressed via Young’s modulus, E, and fractal dimensionality, df, of the polymer structure as follows [18]:

B=

E , d d −df

G=

(d − 1)E .

(

)

(40)

(41)

2d f

Figure 12. Correlation between dimensionality of injected energy localization zones, Df, and self-similarity coefficient, Λi. For the legend, refer to Figure 8. Straight line marks 1 : 1 relation [5]

Substitution of equations (40) and (41) into (39) gives quantitative correlation between the molecular parameter C∞, which characterizes statistical flexibility of the macromolecule [60] and compactness of macromolecular coil [53], and supermolecular structure characteristic df as follows [41]:

C∞ =

2f 4 + . d (d − 1) d − d f 3

(

)

(42)

22

G. V. Kozlov and G. E. Zaikov

For the Euclidean three-dimensional space (d = 3), this equation is reduced to the form (30).

Figure 13. Dependence of the polymer structure fractal dimensionality df on characteristic relation C∞. Experimental data: 1 – linear polymers (blow tests); 2 – linear polymers (d calculation by data from [59]); 3 – EP networks; 4 – ultrahigh-molecular polyethylene, produced by solid extrusion; 5 – polyarylate produced by solid extrusion at T > Tg; 6 – linear polymers (tensile tests); 7 – linear polymers (df calculation from small-angle X-ray diffraction results [15]). Continuous line presents calculation by the equation (42). The circle encloses experimental points with the highest deviation from the theoretical curve. For samples 7, experimental errors are indicated [41]

Figure 13 presents comparison of df(C∞) dependencies, calculated by the equation (42) and obtained by different methods [41] for polymers, enumerated in the Figure legend. It is indicated that almost all samples shown display good conformity between the theory and the experiment, except for samples 5, experimental points for which in Figure 13 are enclosed in the circle. All these polymers (PC, PSF, and PAr) represent heterochain polymers with similar structures and properties, possessing relatively low (close to the minimum, as shown below) C∞ values (2.2 – 2.4) [45, 53]. Samples of these polymers were produced by press molding (for blow tests) or cut from films, prepared by solution pouring on a glass support (for tensile tests). At the same time, data for PAr, prepared by solid extrusion at temperatures above Tg, conform much better with the calculation by equation (42). In this method of PAr sample preparation [61] devitrified polymer relaxes rapidly at the extrusion nozzle output that gives high νcl value and induces formation of relaxed packless matrix. A state formed is much closer to the equilibrium, than for press molded or film samples [61]. As a consequence, equations (30) and (42) give the more accurate df values, the closer

Clusters as Dissipative Structures

23

the structure of the polymeric sample approaches thermodynamically equilibrium one. To put it differently, for the current polymers, equations (30) and (42) give minimal df values [41]. Further on, variation limits for С∞, determined from the equation (42), will be appraised. As is known [1, 18], df values for bulky samples at d = 3 vary within the limits as follows: 2 ≤ df < 3. At df = 2, parameter С∞ possesses the minimal value equal 2. As observed from the literature [45, 53, 59], many polymers do not display С∞ < 2. Concerning the minimal value of С∞, at df = 3 it approaches the infinity. Actually, it has been indicated [53] that for some polymers С∞ can reach ~700, which is equivalent of the mentioned tendency in practice, if the asymptotic run of df(C∞) curve at large С∞ is considered (Figure 13). The expression binding dimensionalities Df and df is the following [18]:

D f = 1+

1 . d −df

(43)

For d = 3, it is reduced to the following form:

Df =

4−df 3−d f

.

(44)

Substitution of equation (44) into (30) gives the accurate result: С∞ = Df

(45)

that proves the empirical correlation shown in Figure 12. Two-level DS (micro- and macro-DS) are formed with the polymer network structure [62]. Micro-DS represent the local order zones (clusters), and their formation is due to high viscosity of the reaction mixture during the gel formation. This induces turbulence of viscous media and formation of oriented zones [18]. One more fundamental property of turbulent flows is fractality of the structures formed by them [18]. It is accepted that in three-dimensional turbulent flows energy dissipation mainly proceeds on a multitude with the fractional (fractal) dimensionality. However, experimental data on the rate fluctuation moments testify about impossibility of describing small-scale properties of the turbulent flow with the help of a self-similar fractal. That is why “inhomogeneous

24

G. V. Kozlov and G. E. Zaikov

fractals”, the rules of formation of which at every stage of the scale hierarchy are random in accordance with some probability distribution, are applied to description of turbulent DS. Hence, the energy transfer is described with the help of a random fragmentation model under the assumption that different stages of the process do not correlate. Therefore, the fractal volume does not possess the global invariance property in relation to similarity transformation. Nevertheless, one can calculate fractal dimensionality df determined by the relation as follows [18]: −d

N n ~ Ln f ,

(46)

where Nn is the number of active whirls at the n-th fragmentation step; βn is the part of the volume occupied by whirls of the Ln scale. Therefore:

d f = 3 + log 2 {β }.

(47)

The symbol {…} indicates averaging by ρ(β) distribution. It shall be expected that due to the above-mentioned connection between the turbulence and the order, a definite part of active whirls is finally transformed into clusters. That is why the relative part of clusters, ϕcl, must be proportional to β. Figure 14 shows the relation ϕcl(β) that proves the effect of turbulence of the local order zone formation in epoxy polymers. The dependence presented does not pass through the origin of coordinates. This means that not all active whirls are transformed into clusters, by just a definite part of them. The part of transformed whirls depends on β: the higher β is, the greater the part of such whirls is. Note also that the reverse interrelation does also exist: the presence of the local order in the structure of polymers induces deformation turbulence at the cold flow plateau [63, 64]. The amorphous solid is considered as a fractal non-equilibrium nonergodic system [65] with hierarchically subordinate levels of the structural organization of self metastable defective states. Remind that in [34] the parts of chains participating in the clusters are taken for linear defects of the structure, analogous to dislocations in metals. In this case, dependencies of the cluster ensemble realization probability on the distance l between clusters in the ultrametric space can be presented as follows [65]:

ωω (l ) ~ exp(− l l n ) ,

(48)

Clusters as Dissipative Structures

ω s (l ) ~ l − D ,

25 (49)

where ωω(l) describes low hierarchic systems; ωs(l) describes highly hierarchic systems; ln and D are positive parameters.

Figure 14. Dependence of the relative part of clusters, ϕcl, on the part of volume, β, occupied by active whirls, for sulfur-containing epoxy polymers cured by isomethyltetrahydrophthalic anhydride (1), 4,4’-diaminodiphenylmethane (2), and 4,4’diaminodiphenylsulfone (3) [62]

In this connection, two main questions occur: how good concordance between the concepts of hierarchic organization of the polymer amorphous state structure presented in [34] and [65] (equations (33) and (48), (49)) is, and what type of hierarchy structure is observed in polymers. The answer to these questions is given [66] on the example of 16 amorphous glassy and amorphous-crystalline polymers and polymer networks. Similar to the works [67, 68], it is suggested that relative part of the local order zones (clusters), ϕcl, organizing the hierarchy of the polymer amorphous state structure must be a function of ensemble realization probability for such clusters (ωω(l) or ωs(l)). To calculate probabilities ωω(l) and ωs(l) by equations (48) and (49), respectively, the following assessments were used. The value l is accepted equal Rcl and is calculated as shown in Chapter 2; ln = const = 100 Å, and this selection is stipulated by the fact that 100 Å size represents the upper linear scale of the fractal behavior of the polymer condensed state [4, 5]. Finally, index D in the equation (49) is equaled to the fractional part of the fractal dimensionality df of the polymer structure as follows:

26

G. V. Kozlov and G. E. Zaikov D = df – 2,

(50)

because the fractional part, df, characterizes the structure change (2 ≤ df < 3 [5]).

Figure 15. Dependence of the relative part of clusters, ϕcl, on low hierarchy system realization probability, ωω(l), for amorphous glassy (1) and amorphous-crystalline (2) polymers, and polymer networks (3) [66]

Figures 15 and 16 show dependencies of ϕcl on cluster ensemble realization probabilities, ωω(l) (low hierarchy systems) and ωs(l) (highly hierarchy systems), respectively. Clearly for all three classes of polymers under consideration, the correlation ϕcl(ωω(l)) is approximated by a linear dependence passing though the origin of coordinates, whereas the correlation ϕcl(ωs(l)) clearly represent the curve. Linearization of the latter correlation in the form as follows: ϕcl = f[(ωs(l))1/2], is shown in Figure 17, which indicates satisfactory linear approximation of this function by a straight line passing though the origin of coordinates. As a consequence, the dependence ϕcl(ωω(l)) is much stronger (magnitude 1) than the dependence ϕcl(ωs(l)) (magnitude 1/2). To put it differently, in the second case, the hierarchy structure is formed much less intensively than allowed by the probability ωs(l). These results assume that hierarchic organization of the polymer supermolecular (supersegmental) structure occupies the intermediate position between high and low hierarchy systems, shifted towards the latter. This situation is explained by the macromolecular origin of polymers. Segments forming the hierarchy, which participate in the clusters, are linked by strong covalent bonds to the polymeric chain that strictly limits their ability to form similar structures. Moreover, the above-mentioned data have

Clusters as Dissipative Structures

27

proved the hierarchy of supermolecular (supersegmental) structure of the amorphous state and conformity of models [34] and [65] for three main classes of polymers. Note also that the basic reason for distribution of data in Figures 15 – 17 is application of С∞ values from the literature, which can vary in significantly broad range for the same polymer [59].

Figure 16. Dependence of the relative part of clusters, ϕcl, on the high hierarchy system realization probability, ωs(l), for amorphous glassy (1) and amorphous-crystalline (2) polymers, and polymer networks (3) [66]

To complete this Section, the authors discuss the way of obtaining two fundamental conclusions in the framework of synergism and fractal analysis: dependence of the “hooking” network frequency on statistical flexibility of the chain and increase of the physical entanglement network frequency (e.g. cluster network formation) in the polymer glassy state. The idea of macromolecular entanglements’ network is one of the basic positions in the rheology of polymers [45], though attempts to apply other approaches shall also be mentioned [69]. Multiple attempts were also made to apply a model of such network, cross-link points of which are interpreted as macromolecular "hookings" [45], to description of glassy polymer properties (for example, [70, 71]). This has induced the increased interest to investigation of possible correlations between molecular characteristics of polymers and topology of macromolecular entanglement network [48, 53, 72]. Essentially, the authors of these works have come to the single point of view that macromolecular “hooking” network frequency, νnw, increases with polymer chain rigidity. However, it should be noted that parameter νnw is experimentally determined for the rubber-like state of polymers (at T > Tg);

28

G. V. Kozlov and G. E. Zaikov

it is assumed that at transition to the glassy state νnw does not change. Disadvantages of this interpretation became clear very soon. Actually, if crosslink points of such molecular hookings are considered as the points of topological chain fixation, then the assumption of equality of their frequencies in the rubbery and glassy states is very ambiguous. For example, polymer deformability decrease at transition from the rubbery to the glassy state is known well, but according to the indicated assumption this change must not happen, and for both cases, the stretch rating λ is determined from the known formula [73]:

Figure 17. Dependence of the relative part of clusters, ϕcl, on parameter [ωs(l)]1/2 for amorphous glassy (1) and amorphous-crystalline (2) polymers and polymer networks (3) [66]

λ = n1st 2 , (51) where nst is the number of statistical segments in the chain intersect between entanglements. To explain the observed change in properties at coming over Tg, a series of models has been suggested. For example, it is assumed [74] that chain sliding through entanglements, which explains λ increase with temperature, is intensified with temperature. In the models [34, 75] increase of the number of chain fixation points is assumed at transition from the rubbery to the glassy state. These fixation points are called the “sliding units” [75] or clusters [34]. In any case, they determine limitations of molecular mobility of the chain in the glassy state [42].

Clusters as Dissipative Structures

29

In the framework of deformable solid synergism, it has been shown [76] that the part of dissipating energy, η, can be estimated from the following equation: β

η = 1− Λ p ,

(52)

where Λ is the structure self-similarity coefficient; βp is the fractional part of the fractal dimensionality of the fracture surface, dp. In accordance with the above-shown, for the structure of polymers, the following equality is true: Λ = С∞, and in the case of quasi-friable destruction, dp value can be assessed as follows [18]:

dp =

10(1 + ν ) . 7 − 3ν

(53)

Fractal dimensionality, D, of the chain part between entanglements is the structural parameter characterizing molecular mobility level and, consequently, the energy dissipation level [77]. Techniques for D assessment are given in the work [5]. Good correlation between (D – 1) and η parameters was obtained for 15 amorphous and amorphous-crystalline polymers [78] (remind that 1 ≤ D ≤ 2 and 0 ≤ η ≤ 1). Physical basis for this correlation is obvious. As mentioned above, D parameter characterizes molecular mobility, and intensification of the latter always induces increase of mechanical energy dissipation applied to the polymer [79]. The length of the chain segment between “hookings”, Lc, is calculated for the rubbery state that allow modification of the equation (52) as follows. For rubbers, ν is close to 0.5 (but not equals it [18]). That is why dimensionality, dp, must be calculated for viscous degradation under the condition ν ≥ 0.375 [18]. In this case, the equation for dp calculation is as follows [18]:

dp =

2(1 + 4ν ) . 1 + 2ν

(54)

As ν ≈ 0.45 is chosen for rubbers [80], calculation by the equation (54) gives dp ≈ 2.95, i.e. in the first approximation one can accept β ≈ 1 in equation (52). Then under the above-mentioned conditions (η = D – 1 and Λ = С∞) modified equation (52) is obtained:

30

G. V. Kozlov and G. E. Zaikov

D = 2−

1 . C∞

(55)

In its turn, dimensionalities D and df are interrelated by the following expression [5]:

D=

ln n st . ln 4 − d f − ln 3 − d f

(

) (

)

(56)

Combined equations (54) – (56) allow calculation of nst for rubbers practically by known C∞ values only, because ν (or df and dр) values are fixed. The equation for Lc assessment is deduced as follows [78]: Lc = nstlst = nstl0C∞.

(57)

Table 2. Values of characteristic relations С∞, backbone real bond lengths l0, e

t

experimental Lc and theoretical Lc lengths of the chain intersects between macromolecular “hookings” for some polymers [78] Polymer Poly-n-dodecylmethacrylate Poly-n-octylmethacrylate Polystyrene Polyvinylacetate Poly-n-butylmethacrylate Poly(methyl methacrylate) Polyethylene Polyvinylchloride Polytetrafluoroethylene Polyamide-6 Polypropylenoxide Polyethylenoxide Poly(ethyleneterephthalate) Poly(ester terephthalate) Polycarbonate

C∞ [45,53] 13.4 10.0 10.0 9.4 9.1 8.6 6.8 6.7 6.3 5.3 5.1 4.2 4.2 3.3 2.4

l0 [45,53], Å Lec , nm [81] Ltc , nm 1.54 1.54 1.54 1.54 1.54 1.54 1.54 1.54 1.54 1.49 1.49 1.49 1.25 1.25 1.25

226 177 104 88 130 97 56 31 41 46 60 45 21 28 29

208 149 149 136 131 92 88 87 80 61 58 43 36 30 17

Clusters as Dissipative Structures

31

Table 2 shows parameters l0 and C∞ required for calculation and accepted in

( )

accordance with [45, 53], Lc Lec values from the literature (in accordance with

( )

[81]), and Lc Ltc values calculated by the method above. The Table indicates good conformity between theoretical and experimental results.

Figure 18. Dependence of theoretical lengths of the chain intersect between entanglements

Ltc

on characteristic relation C∞ for polymers listed in Table 2 [78]

Figure 18 shows correlation Ltc (C∞) for polymers, mentioned in Table 2. Good linear correlation obtained proves already known principle of entanglement network frequency increase with statistical chain rigidity [45]. At Ltc = 0, the dependence Ltc (C∞) is extrapolated to С∞ ≈ 2 that corresponds to tetrahedral valence angle θ (≈ 70.5°) in the chain model with fixed valence angles [60]. However, this value of С∞ cannot be considered the border one. As follows from the equation (55), С∞ = 1 at the border value D = 1 [5]. In the mentioned model of the chain with fixed valence angles С∞ is determined as follows [60]:

C∞ =

1 + cos θ . 1 − cos θ

(58)

32

G. V. Kozlov and G. E. Zaikov

Obviously at С∞ = 1, cosθ = 0 and θ = 90°. Thus the fractal analysis assumes С∞ falling within the range of 1 – 2 and arbitrary sharp valence angles. It is known [80, 82] that transition from the rubbery to the glassy state is accompanied by the Poisson coefficient decrease, which value below Tg depends on the test temperature. This means decrease of df in accordance with the equation (4) and nst (i.e. decrease of Lc) in accordance with the equation (56) in the glassy state rather than in the rubbery state even at invariable D. This effect is intensified by the appropriate decrease of D that follows even from the well known fact as follows: the decrease of molecular mobility in the polymer glassy state [59], and is proved experimentally [5]. Thus the fractal analysis suggested enables forecast of the topological chain fixation point number increase at T < Tg, suggested before [75, 83].

Figure 19. Dependencies of

Lec Lcl

(1) and

Ltc 0 Ltc

(2) (see text for details) on the

test temperature for PC [78]

Quantitatively, this forecast can be checked by temperature dependence of two relations. The first of them is the relation of chain intersect lengths between e

“hookings” Lc (the rubbery state) [81] and between clusters Lcl (the glassy state) t

[83]. The second one is the relation between lengths, Lc , obtained by the abovet

mentioned method at ν = 0.45 ( Lc 0 , the rubbery state) and at ν values. The first

Clusters as Dissipative Structures

(

33

) gives results, obtained within the framework of the cluster model [83]; the second one (L 0 L ) - in the framework of the fractal analysis. e

relation Lc Lcl

t c

t c

Figure 19 shows temperature dependencies of both relations for PC, for which t

good conformity was observed. Values of Lc were calculated at randomly chosen D = 1.75, but any other choice in the above-mentioned interval will not change symbate type of dependencies, shown in Figure 19, but just slightly deviate their quantitative conformity. Thus in the framework of the fractal analysis the increase of macromolecular “hookings” network frequency with statistical chain rigidity was proved. In contrast with previous studies, the fractal analysis forecasts increase of the number of topological fixation points of macromolecules in the glassy state rather than in the rubbery one. The cluster model of the polymer amorphous state structure gives correct quantitative description of this effect [78].

Chapter 3

CLUSTER AND FLUCTUATION FREE VOLUME MODELS The fluctuation free volume model is widely spread in descriptions of the physical meaning of liquids and glasses [84 – 86]. Hence, the physical meaning of the model parameters is yet mainly unclear [87, 88]. Moreover, difficulties appear in the free volume theory concerning explanation of the temperature dependence of kinetic properties, in particular, viscosity at fixed volume of the system. The relative part of the fluctuation free volume, ff, is determined, for instance, by data in the glass transition zone [85, 86]. If ff is known, one can calculate the formation energy of the minimal free volume microcavity, εh, by the formula as follows [86]:

εh = kTgln(1/ff).

(59)

Let us now turn to comparison of the cluster model with the fluctuation free volume for solid polymers [83, 89]. Obviously in accordance with the cluster model the fluctuation free volume is accumulated in the packless matrix. In terms of the free volume theory, detachment of a kinetic unit (an atom or a group of atoms) from a cluster means formation of a random microcavity, and addition of a kinetic unit to a cluster means its “implosion” (annihilation). As a consequence, random change of the free volume with temperature can be realized in principle at a constant volume of the system due to microcavity exchange between clusters and the packless matrix. This approach to the mechanism of generation and migration of random microcavities overcomes the above-mentioned difficulty in

36

G. V. Kozlov and G. E. Zaikov

explanation of the temperature dependence of viscosity at fixed volume of the system [89]. νcl, and cluster functionality, F, with temperature increase for amorphous glassy polymers [90]. Analysis of these data induces a conclusion that the number of clusters per specific volume of the polymer remains practically unchanged with temperature increase, but the number of segments in each cluster decreases. However, at T = Tg in the glass transition zone clusters are completely decomposed (νcl = 0), and excessive fluctuation free volume reaches the critical value. Thus from these positions, devitrification of a glassy polymer is caused by cluster decomposition (i.e. annihilation of the local order). Therefore, energy of the cluster formation or decomposition, Ucl, must possess the magnitude of the average energy of kinetic unit (statistical segment) heat motion at the glass transition temperature: Ucl ≅ (i/2)kTg, where i is the number of degrees of freedom of the kinetic unit. If one takes into consideration that a segment consists of many atoms, then in the first approximation i must equal the number of degrees of freedom in a multiatomic molecule, i = 6 [89].

Figure 20. Correlation between the segment interaction energy in the cluster, Ucl, and kTg value for the polymer solid phase at T = 293 K: 1 – HDPE, 2 – PP, 3 – PA-6, 4 – PETP, 5 – PVC, 6 – PHE, 7 – PTPE, 8 – PC, 9 – PSP, 10 – PAr [89]

Expectedly, the energy of segment detachment from the cluster was found proportional to the glass transition temperature of polymers (Figure 20). It is noteworthy that the slope of Ucl(kTg) line is practically coincident with i/2 value and the coefficient of proportionality between energy of the minimal random microcavity formation (see equation (59)): Ucl = 3.3 kTg and εh = 3.5 kTg. It is

Cluster and Fluctuation Free Volume Models

37

taken into account here that common value of ff for glassy polymers equals 0.025 and ln(1/ff) = 3.5. As a consequence, the energy of random microcavity formation is practically coincident with the energy of segments’ interaction in the cluster (εh = Ucl). From this point of view, generation and implosion of a random microcavity in amorphous polymers are stipulated by dissociation and segment association into a cluster, respectively. Microcavity formation energy equals the work for collinear segments detachment from one another in the cluster by breaking intermolecular bonds between them, and the magnitude of the microcavity minimum size (≈ 4 – 5 Å [89]) equals the border elastic deformation of the intermolecular bond between segments. Ucl decrease with temperature due to the presence of temperature dependencies of G and ν [91]. It can be shown that for glassy polymers, ff increases (though slowly) with temperature [92] that induces the corresponded decrease of εh. However, it should be noted that temperature dependencies of energies εh and Ucl are very weak. Apparently, this is explained by the fact that parameters εh and Ucl represent characteristics of the short-range (local) order of glasses, weakly responding to temperature variation (anyway, at T < Tg′ [90]).

Figure 21. Dependence of the relative fluctuation free volume, ff, on volumetric part of the packless matrix, ϕp.m., for linear amorphous polymers: PC (1) and PAr (2) [93]

Besides the above-considered correspondence between the cluster model and the kinetic theory of the fluctuation free volume, application of the former one allowed obtaining of a series of new ideas on the interconnection between structure and free volume [93]. For example, Figure 21 shows dependencies of the relative random volume, ff, on the volumetric part of packless matrix, ϕp.m., for

38

G. V. Kozlov and G. E. Zaikov

two linear amorphous polymers, PC and PAr. The dependencies are linear, and their extrapolation to ϕp.m. = 0 gives ff = 0. The latter means that in this case, an amorphous polymer represents a huge cluster without a fluctuation free volume. Clearly this circumstance does not exclude the presence of a configurative free volume [94]. At ϕp.m. = 1.0 ff is extrapolated to a finite value, approximately equal 0.14 and corresponded to ff at the glass transition temperature [95]. For glassy polymer networks, the type of dependencies ff(ϕp.m.) differs from the above-considered one (Figure 22). Similar to the case of linear amorphous polymers, they are approximated well by a straight line. However, the line does not pass through the origin of coordinates, but at ϕp.m. = 0 cuts an intersect ff ≈ 0.024 on the axis of ordinates. One can assume that this value of ff is associated with the presence of a network of chemical cross-link points. Thus in contrast with linear polymers, in polymer networks the relative fluctuation free volume consists of two components. One of them is constant and connected with the zones of chemical cross-link points; the second one is the linear function of ϕp.m. and is determined by supersegmental (cluster) structure. Various components of ff determine different properties of epoxy polymers: variable part of ff regulates elasticity and local plasticity, and total value of ff regulates properties in the zone of macroscopic flow behavior [96].

Figure 22. Dependence of the relative fluctuation free volume, ff, on volumetric part of the packless matrix, ϕp.m., for epoxy polymers: EP-1 (1), EP-2 (2), EP-1-200 (3), and EP-2-200 (4) [93]

Thus correlations obtained using the cluster model of the polymer amorphous state structure allow an observation that the fluctuation free volume, and the type

Cluster and Fluctuation Free Volume Models

39

of its variation with respect to structural factors are significantly determined by the type of polymer structure [93].

Chapter 4

THE CLUSTER MODEL AND THE ANHARMONICITY CONCEPT In recent 20 years, increased interest to the Grüneisen parameter, γ, is observed in physics of liquids and glasses. This parameter participates in the equation of state and represents the anharmonicity index of quasi-lattice oscillations and nonlinearity of interatomic interaction forces [59, 97]. The Grüneisen parameter was successfully applied to analysis of the cluster formation event and orientation of molecules in liquids [98 – 100]. Since a liquid and the glassy state are structurally indistinguishable [101], of interest is the Grüneisen parameter application to studies the local order in glassy polymers. In the framework of the cluster model temperature dependence of γ for amorphous polymer was interpreted [83]. Knopoff and Shapiro [98] have indicated that for water and mercury, γ decrease with the specific volume increase can be assigned to the change of the average number of molecules in the cluster, N. They have suggested a semiquantitative one-dimensional model, which enables description of γ dependence on volume. It is assumed that γ represents the sum of two components [98]:

γ = γD +ξ

∂ ln N ∂ ln V

,

(60)

T

where γD is the component of γ corresponded to the Debye heat capacity theory; ξ is a factor dependent on N.

42

G. V. Kozlov and G. E. Zaikov

The equation (60) describes γ variation with pressure, P, but due to equivalence of P and T variables in the equation of state it can be used for assessment of the temperature dependence of γ under constant pressure. In this case, index T in the equation (60) is replaced by P. The Debye component γD in the Grüneisen parameter can be assessed as follows [98]:

γ = −ξ

∂ ln ω D ∂ ln V

,

(61)

P

where ωD = πω0 is the Debye frequency of polymeric chain oscillations; ω0 is determined as follows:

ω0 =

U . M

(62)

Here M is the mass of oscillating kinetic unit of the chain; U is the potential energy of interaction between two kinetic units, accepted equal Ucl in the framework of the cluster model. Temperature dependence of the specific volume, V, is calculated by the following equation [100]:

(V~

13

)

−1 =

αT , 3(1 + αT )

(63)

~

where V = V/V* is the reduced specific volume; V* is the characteristic specific volume; α is the volumetric coefficient of heat expansion, temperature dependence of which is determined as follows [83]:

⎛α 2 ⎞ ⎛ ∂α ⎞ ⎟. ⎜ ⎟ = (7 + 4αT )⎜⎜ ⎟ ∂ T 3 ⎝ ⎠P ⎝ ⎠

(64)

Accepting α value at T = 293 K [83] and characteristic volume as the reverse density, ρ, one can obtain correlation lnωD(lnV), shown in Figure 23 for PAr and PSF. Clearly the correlation between ωD and V in double logarithmic coordinates

The Cluster Model and the Anharmonicity Concept

43

is well approximated by a linear correlation. In accordance with the equation (61), this means that γD constancy in the considered temperature interval (293 – 453 K for PAr and 293 – 433 K for PSF). Absolute values of γD can be estimated from the slope of lines in Figure 23, which are independent of V* selection: these values (γD = 12 for PAr and γD = 13.75 for PSF) are close to the ones previously obtained for polymers of this type [102].

Figure 23. Variation of the Debye frequency, ωD, with the specific volume, V, present in double logarithmic coordinates for PAr (1) and PSF (2) [83]

Figure 24. Correlation between the average number of segments in the cluster, nseg, and the specific volume, V, present in double logarithmic coordinates for PAr (1) and PSF (2) [83]

Thus for the case of temperature independence of the segments’ number in the cluster, the above-shown results indicate obligatory fulfillment of the following condition (equation (60)) [83]:

γ = γD = const.

(65)

44

G. V. Kozlov and G. E. Zaikov

Indicated in the above discussion was γ decrease with temperature [59]. It is assumed that dN ≠ 0, whence the necessity of assessment of the second term in the equation (60) follows. As indicated in Chapter 2, N = nseg = F/2. Figure 24 shows dependence lnnseg(lnV) for PAr and PSF; both dependencies are described by single linear relation that gives an opportunity to assess the relation ∂lnnseg/∂lnV ≈ 6.5. For large nseg, parameter ξ in equation (60) at temperatures above the Debye point is approximated by the following series expansion [98]:

ξ = 0.6942 +

0.03780 + ... . n seg

(66)

Figures 25 and 26 show temperature dependencies of γ, calculated by equation (60) for PAr and PSF, respectively.

Figure 25. Temperature dependence of the Grüneisen parameter γ for PAr: the Debye component γD (1), calculations by equations (60) (2), (67) (3), and (68) (4) [83]

Figure 26. Temperature dependence of the Grüneisen parameter γ for PSF: the Debye component γD (1), calculations by equations (60) (2), (67) (3), and (68) (4) [83]

The Cluster Model and the Anharmonicity Concept

45

The value of γ can also be calculated by two independent methods as follows. The first method uses simple relation for temperature dependence of the elasticity modulus, E [103]: Е = Е0(1 - γαТ),

(67)

where Е0 is the value of E extrapolated to 0 K. The second method is based on application of the Sharma equation [100]:

(

)

⎛ 1 ⎞ 1 ~1 3 ⎟ − 5V − 2 . ⎝ 2αT ⎠ 3

γ = 1+ ⎜

(68)

The values of γ calculated for PAr and PSF by equations (67) and (68) are also shown in Figures 25 and 26, respectively. Clearly calculation results by three equations mentioned display high coincidence. Previously, γ decrease with temperature was attributed to accompanying the elasticity modulus decrease; in its turn, the latter was attributed to decrease of the cluster network frequency, e.g. nseg decrease [57]. Thus the above-shown results conform to previously suggested explanation of the effect observed. Equations (60), (67) and (68) give adequate description of γ(Т) dependence by both the general tendency and absolute values. In its turn, this proves correctness of the cluster model and suitability of application of the anharmonicity concept to description of the local orientation of the polymer amorphous state structure [83].

Chapter 5

CLUSTER STRUCTURE AS A PERCOLATION SYSTEM Percolation models are widely used for description of many physical problems [22], including polymers [104 – 108]. These models are differed by simplicity and demonstrativeness [22], and their application to description of the structure and properties of polymers allows the use of the well-developed mathematical apparatus of the percolation theory. The cluster structure formation at Tg sharply changes properties of amorphous polymers attributing their rigidity typical of solids [90]. That is why one may suggest Tg representing the percolation threshold on the temperature scale in this case, at which an infinite cluster (in the sample borders) is formed. Relating to description of polymers, the “carcass coherency” concept [109, 110], suggested 35 years ago, can be accepted to be the predecessor of percolation models. This concept assumes that the existence of carcass coherency of macromolecules in polymers is the necessary condition of their rigidity and strength. It also gives a relation for assessing probability of the carcass bond formation, ηх. The most probable candidate for the carcass role in linear amorphous and amorphous-crystalline polymers is the network of macromolecular entanglements. As mentioned above, two basic concepts of the structure of such network do exist now: the “hooking” network and the cluster network. The contribution of these networks to the carcass coherency of amorphous and amorphous-crystalline polymer and, consequently, their mechanical properties were determined [111]. If the cluster network of macromolecular entanglements is accepted to be such carcass, it is natural to assume equality of the probability of this “carcass”

48

G. V. Kozlov and G. E. Zaikov

formation, ηх, to the relative part of clusters, ϕcl. The value of ηх can be assessed as follows [109]:

ηx =

S , ac E

(69)

where S is the cross-section of the macromolecule; ac is the analogue to Young’s modulus for elastic stretch of macromolecules; E is the elasticity modulus, determined experimentally. The value of ac can be assessed in accordance with recommendations in the ref. [109], which gives the following results [11]: 2.22×10−1 N for LDPE; 4.5×10−10 N for HDPE; 7.5×10−10 N for PC and PAr. Figure 27 shows comparison of ϕcl and ηх for PC and PAr. Clearly a linear correlation between them is observed, but ηх values regularly exceed appropriate ϕcl values. At ϕcl = 0 ηх is extrapolated to ηх0 ≈ 0.18 that assumes existence of two carcasses in amorphous PC and PAr. Moreover, frequency of one of these carcasses (the cluster one) is the function of temperature, whereas the second carcass (macromolecular hookings) possesses constant frequency. Macromolecular hookings’ carcass frequency, ηх0, is assessed from the following equation [109]:

ηx0 = nx0S.

(70)

Then the molecular mass, Mx0, of the chain segment between neighbor hookings can be calculated. For PC and PAr, Мх0 ≈ 1,610 g/mol. Values of this parameter shown in the literature are as follows: 1,780 – 2,250 g/mol [45] and 1,400 – 2,426 g/mol [112], which correlate well with the assessment. Thus for amorphous glassy PC and PAr polymers, the cluster network of macromolecular entanglements represents the "carcass", and contribution of the macromolecular “hooking” network is rather low (especially at low temperatures) and constant [111]. Figure 28 shows the same comparison of ϕcl and ηх for LDPE and HDPE. Similar to two amorphous polymers (Figure 27), linear correlation between ϕcl and ηх is observed. However, for LDPE and HDPE linear approximation passes through the origin of coordinates, i.e. ϕcl ≈ ηх. This fact is explained by the devitrified state of the polyethylenes’ amorphous phase in the temperature interval studied; thus the elasticity modulus of the phase (and, respectively, ηх) is very low

Cluster Structure as a Percolation System

49

(~2.1 MPa [45]). That is why ηх0 value is much lower than inaccuracy of the graphical correlation ηх(ϕcl).

Figure 27. Dependence of the coherency carcass formation probability, ηх, on the relative part of clusters, ϕcl, for PC (1) and PAr (2) [111]

Figure 28. Dependence of the probability of coherence carcass formation, ηх, on the relative part of clusters, ϕcl, for LDPE (1) and HDPE (2) [111]

Thus the above results allow the statement that the macromolecular entanglement cluster network represents the “carcass” for amorphous and amorphous-crystalline polymers. As a consequence, this very network causes the main impact on mechanical properties of solid polymers (especially amorphous ones [57]). Contribution of the macromolecular hooking network is independent of temperature and is sufficient in the glassy state of polymer only. Estimation performed by the equation (69) has indicated that the presence of the macromolecular hooking network only in PC and PAr would give, approximately, three-fold lower elasticity modulus compared with the experimentally observed one, and polyethylenes would completely lose rigidity [111, 113].

50

G. V. Kozlov and G. E. Zaikov

It is known [22] that at approach of percolation threshold, хс, critical behavior of the infinite cluster cardinality, Р∞ (the probability of cross-link point belonging to the current cluster), is described by the scaling relation as follows:

P∞ ~ ( x − xc )β n .

(71)

In the framework of the cluster model, ϕcl is the obvious selection for Р∞, and the glass transition temperature, as mentioned above, is accepted for хс [67, 68]. In this case, the test temperature, T, is accepted as the current probability, X, and the relation (71) can be reduced to as follows [67]:

ϕ cl ~ (Tg − T )β n = (ΔT )β n ,

(72)

where changing over Tg and T is caused by the inequality Tg > T. Figure 29 shows dependence ϕcl(ΔТ) in double logarithmic coordinates, corresponded to correlation (72). The graph of this dependence is linear that enables calculation of βn ≈ 0.46.

Figure 29. Dependence of the relative part of clusters, ϕcl, on temperature difference (Tg – T), presented in double logarithmic coordinates for PMMA (1), PC (2), and PAr (3) [67]

This value is close to theoretical “classical” one βn = 0.40 for a threedimensional percolation cluster [22]. The graph in Figure 29 is plotted for the temperature range Tg – (Tg – 80 K), because correlation (71) is true under the condition х → хс [22] (or Т → Тg). Thus the amorphous polymer structure represents a percolation cluster, which can be described by general laws of the

Cluster Structure as a Percolation System

51

percolation theory [67]. The same result was obtained for glassy polymer networks [68] and amorphous-crystalline polymers [114]. For example, in the framework of these general laws, the number of cross-link points, S, in a finite cluster, which can be the local order zone consisting of F/2 closely packed segments (where F is the cluster functionality [90]), depends upon dimensionless deviation of concentration, τ, from its critical value (τ = (х – хс)/хс [22]) at τ → 0 as follows:

S~τ

−γ n

.

(73)

As mentioned above, the number of cross-link points, S, in the local order zone (classified as the cluster [34, 90]) equals F/2, and for τ parameter (Тg – Т)/Тg should be accepted. Figure 30 shows dependencies of F/2 on (Тg – Т)/Тg in double logarithmic coordinates for epoxy-polymers. The dependencies were found linear that allowed estimation of the index in correlation (73) as 1.28 for EP-1 and 2.28 for EP-2. For amorphous glassy polymers the following values of γn were obtained: ~1.45 for PMMA, ~1.36 for PC, and ~1.14 for PAr. All calculated values of γn satisfactorily correlate with its theoretical value (= 1.84) for a threedimensional cluster [22].

Figure 30. Dependencies of the number of cross-link points (segments) in a finite cluster, F/2, on dimensionless temperature deviation, τ = (Тg – Т)/Тg, presented in double logarithmic coordinates for EP-1 (1) and EP-2 (2) [68]

As a consequence, the results obtained [67, 68, 114] indicate that at temperature Tg (Tmelt) a structure of statistical segments is formed in amorphous (amorphous-crystalline) polymers representing a percolation cluster and being

52

G. V. Kozlov and G. E. Zaikov

described properly in the framework of the cluster model. This circumstance assumes the polymer glass transition represents the phase transition, and ϕcl value is the orientation parameter [22]. Moreover, this is one more proof for fractality of the polymer structure in the range of ~3 – 100 Å (refer to Section 1). Of special interest is the fact that critical indices of the orientation parameter, βn, obtained in refs. [67, 68, 114], though are very close to the classical percolation indices (βn = 0.37 – 0.40 [115]), but differ from them by the absolute value. The reason for such inconsistency is the percolation cluster representation as a pure geometrical structure, which is too simplified simulation of natural amorphous polymers, which possess thermodynamically non-equilibrium structure. That is why the structure of the mentioned polymers is affected by thermal interactions (remind that the cluster structure is postulated as a thermofluctuational system [34]). This means that the percolation cluster (carcass) of the polymer structure consists of elements (statistical segments) possessing molecular mobility, e.g. they oscillate around some quasi-equilibrium position. Such elements form a virtual volume, which exceeds the volume of a cluster from static elements that makes the percolation process simpler and allows formation of the percolation carcass from smaller number of elements or with higher βn value. Moreover, cluster formation is studied by the scale of relative temperatures, but not by the scale of concentrations as for the percolation cluster [22, 115]. As a consequence, thermal cluster, i.e. the cluster which equilibrium configuration is determined by both geometrical and thermal interactions [116], is more correct simulation of the polymer amorphous state. In this case, the orientation parameter ϕcl of the polymer structure is determined from the following equation [116]:

ϕ cl

⎛ Tg − T ⎞ ⎟ =⎜ ⎜ Tg ⎟ ⎝ ⎠

βT

,

(74)

where index of the orientation parameter, βТ, is not necessarily equal to the appropriate critical index, βn, in pure configuration percolation models. An attempt was made [117] to estimate variation of βТ absolute values, detect possible connection between this index and structural characteristics of polymers, and determine factors affecting βТ value. This was performed on the example of three series of epoxy polymers: amine (EP-1) and anhydride (EP-2) cross-linking type, and EP-1 after natural aging under atmospheric conditions during 3 years (EP-3) [18].

Cluster Structure as a Percolation System

53

It has been shown [119] that universality of critical indices of the percolation system is directly bound to the fractal dimensionality of this system. Selfsimilarity of the percolation system assumes the presence of a series of subsets possessing the order n (n = 1, 2, 4, …), which in the case of the amorphous polymer structure are identified as follows [117]. The first subset (n = 1) is the carcass of the percolation cluster or, as shown above, cluster network of the polymer. The second subset (n = 2) represents the packless matrix, to which cluster network is buried. In this interpretation, critical indices βn, νn, and tn are given as follows (in the three-dimensional Euclidean space) [119]:

βn =

1 , df

(75)

νn =

2 , df

(76)

tn =

4 , df

(77)

where df is the fractal dimensionality of the polymer structure, determined by the equation (4). Thus βn, νn, and tn parameters represent border values for βТ pointing out the structural component of the polymer that determines its behavior. As βТ = βt, this component are clusters or, more accurately, the percolation cluster carcass identified with the cluster network. As βn < βT < νn, the polymer behavior is determined by joint influence of clusters and packless matrix. As βТ = νn, the determining structural component will be the packless matrix, and at βТ = tn the chemical cross-link network; at νn < βT < tn a joint influence of two abovementioned structural components is observed. For three series of epoxy polymers under consideration, assessments of βT parameter have indicated their possible approximation by the following values: ≈ 0.54 for EP-1, ≈ 0.55 for EP-2, and ≈ 0.38 for EP-3. Figure 31 compares ϕcl values as the function of Kst, experimental [5] and calculated by the equation (74), using the above βT values. In the framework of the thermal cluster model, experimental and calculated values conform well. The average Df value for three studied series of epoxy polymers equals 2.613. This means that according to

54

G. V. Kozlov and G. E. Zaikov

equations (75) and (76) βn ≈ 0.38 and νn ≈ 0.77. Comparison of these assessments and βT values, calculated from the equation (74), indicates that the cluster network is the basic structural factor for EP-3, and behavior of EP-1 and EP-2 is regulated by the joint effect of cluster network and packless matrix. Thus for aged epoxy polymers (EP-3) only indices of the orientation parameter of percolation and thermal clusters coincide. For the case under consideration, this indicates insufficiency of thermal interaction for the polymer structure and that its equilibrium configuration is determined by geometrical interactions only. It has been shown [118] that during heat aging the structure of epoxy polymer EP-3 reaches its quasi-equilibrium state, characterized by the balance between the tendency to local order increase, the index of which is ϕcl, and entropic chain straining. Hence chain intersects between clusters are stretched, and their fractal dimensionality D approaches 1. This indicates [5, 77] full suppression of molecular mobility of these parts of the chains.

Figure 31. Dependencies of the relative part of clusters, ϕcl, obtained experimentally (1 – 3) and calculated by equation (74) (4 – 6), on Kst for epoxy polymers: EP-1 (1), EP-2 (2), and EP-3 (3) [117]

For EP-1 and EP-2, D > 1 [5] and, as follows from Figure 5.31, βТ > βn. Consequently, it may be assumed that the condition βТ > βn is induced by nonzero molecular mobility, e.g. 1 < D ≤ 2 [5]. To check this assumption, one shall calculate D value that can be made differently, (for example, using equation (55) or (56)), but the authors in the work [117] have used a simple formula as follows [77]:

Cluster Structure as a Percolation System

2

ϕ cl

= C ∞D .

55

(78)

Figure 32 shows the dependence βТ(D) for three series of studied epoxy polymers. Expectedly, increase of D leads to βТ growth. As D = 1, βТ ≈ 0.38, i.e. the condition βТ = βn is fulfilled. The condition βТ = νn is reached at D ≈ 1.42, and extrapolation of the dependence βТ(D) shown in Figure 5.32 to D = 2 gives βТ ≈ 1.35. As known [120], D = 2 indicates a rubber-like state of polymer (df ≈ 3), characterized by complete degradation of the cluster structure [121]. In accordance with the equation (77), at df ≈ 3 tn ≈ 1.33, i.e. for rubber-like polymers the condition βТ ≈ tn and, consequently, its behavior is completely determined by the chemical cross-link network, which is the well-known fact [122]. Taking into account that for glassy epoxy polymers βn ≤ βT ≤ tn, one should assume incorrectness of the latter conclusion for them and general regulation of their behavior by the totality of three structural components: cluster network (local order zones), packless matrix and partly (at high D) chemical cross-link network (topological structure level).

Figure 32. Dependence of index βt on the fractal dimensionality D of the chain segment between clusters for EP-1 (1), EP-2 (2), and EP-3 (3). Horizontal dashed lines indicate βn (4) and νn (5) values for the percolation cluster [117]

As a consequence, the above-discussed results indicate that the structure of polymer networks can be simulated by a thermal cluster. Hence, correspondence between thermal and percolation clusters, expressed by the equality of critical indices of the orientation parameter βТ = βn, is reached for quasi-equilibrium state of the polymer structure only. Actually, βТ value is the function of molecular

56

G. V. Kozlov and G. E. Zaikov

mobility, characterized by the fractal dimensionality (D) of the chain segment between clusters [117]. Some other important points should be noted, associated with the possibility of describing the polymer structure in the framework of equation (72). For the "rigidity segment", the statistical segment with the length lst, is accepted in the cluster model. The value of lst is several times lower than the Kuhn segment length, A, which characterizes rigidity of freely joint chain [60]. Selection of A as the “rigidity segment” mostly gives ϕcl above the unit, which is physically meaningless. The following correlation binds parameters lst and A [60]: lst = Acos(θ/2),

(79)

where θ is the valence angle. Thus shorter length of the chain “rigidity segment”, lst, in the glassy state is caused by conformational restructurings typical of this state [9]. For amorphous-crystalline polymers, reduced relative part of clusters,

ϕ clr , is

used. It characterizes this parameter in relation to the entire volume of the polymer, but not its amorphous phase exclusively [123, 124]:

ϕ clr =

ϕ cl 1− K

,

(80)

where K is the crystallinity degree. Thus for amorphous-crystalline polymers, the equation (5.72) can be reduced to the form as follows [9]:

ϕ cl ~ (1 − K )(Tg − T )βT .

(81)

Figure 33 shows correlation between Df and ϕp.m. for three polymers. Clearly at ϕp.m. = 0 the value of Df does not approach its border value equal 2.0 [5], 0

namely, d f value, which is different for different polymers. Obviously, this is the minimum of Df that can be reached for current polymers. The equation (42) binding parameters Df and С∞ and gives Df values close to the minimum. Table 3 T

0

shows comparison of d f values, calculated by the equation (42), and d f (Figure 33), which indicate their good conformity. Since the equation (42) gives

Cluster Structure as a Percolation System

57

the better correspondence to the experiment, the closer the polymer structure 0

approaches thermodynamic equilibrium [41], dimensionality of d f characterizes some quasi-equilibrium state of the structure. As follows from this equation, Df = 2 can be approached for polymers possessing С∞ = 2, i.e. for chains with 0

T

tetrahedral valence angle [60]. Thus substitution of d f or d f into equation (5) or (7) can help in the local order assessment,

ϕ cl0 , maximum approachable for the

current polymer, as the function of С∞ and S, the most important characteristics of the polymer. As temperature decreases below the point, at which

ϕ cl0 is

approached, the local order remains unchanged, so this temperature T0 can be assumed to be the analogue of Т∞, at which the polymer reaches constant free volume level [125]. In its turn, this temperature can be determined from the equation (42) under the condition ϕcl =

ϕ cl0 . The values of T0 and Т∞, obtained in

this manner [125], are compared in Table 4.

Figure 33. Dependencies of the structure fractal dimensionality, df, on the relative part of packless matrix, ϕp.m., for PC (1), PMMA (2) and HDPE (3) [9]

Good conformity was obtained for all polymers, except for PC, for which calculation by the equation (42) gave physically meaningless ΔТ ≈ 670 K. The reason for this seeming non-correspondence is as follows. Previously [5], the notion of quasi-equilibrium state of the polymer structure was introduced, to which Df ≈ 2.5 is corresponded. For real polymers, the tendency of transition to thermodynamically more equilibrium state (i.e. in the state with higher local order degree, ϕcl) at a definite stage must be balanced by entropic chain straining forces.

58

G. V. Kozlov and G. E. Zaikov

To put it differently, for the majority of polymers thermodynamic balance by means of the local orientation cannot be reached. That is why Df = 2.5 instead of T

theoretical value d f should be used. Moreover, data from Figure 33 indicate that the value ϕp.m. = 1.0 (i.e. ϕcl = 0) is approached at Df = 2.92, but not at Df = 3 as suggested by the equation (5). With respect to these adjustments, calculation by the equation (42) gives T0 = 318 K for PC that properly correlates with T∞ = 323 K (Table 4).

( ) T

Table 3. Critical fractal dimensionalities of polymer structures: d f , 0

calculated by equation (42), and d f , estimated from graphs in Figure 33 [9] Polymer

(d ) T f

d 0f

2.83 2.82 2.58 2.29

2.66 2.50 2.51 2.31

Poly(methyl methacrylate) Polyethylene Epoxy polymer Polycarbonate

Table.4. Transition temperatures to “frozen” free volume (Т∞) and structure (Т0) [9] Polymer Poly(ethylene terephthalate) Polyamide-6 Polyethylene Polypropylene Polystyrene Poly(methyl methacrylate) Polyvinylchloride Polycarbonate

ϕ cl0

Т∞ , K

Т0, K

0.24 0.14 0.10 0.24 0.23 0.36 0.17 1.0 0.36

280 277 227 227 324 290 270 323

300 304 243 199 320 269 333 − 318

It is known [126] that the fluctuation glass transition theory assumes the following temperature dependence of the characteristic length of cooperatively restructured zones (CRZ), ξА:

Cluster Structure as a Percolation System

ξA ~ (T – T0)2/3,

59 (82)

where T0 is the Foegel temperature in the VLF equation. Actually, the relation (82) is the percolation one or, more exactly with respect to the above discussion, the thermal cluster model relation. ξA value is equivalent to the local order diameter, Dcl. That is why Figure 34 shows the dependence Dcl(Тg – Т) plotted in double logarithmic coordinates, corresponded to the relation (5.82) (under the condition ξА = Dcl and Т0 = Тg) for the initial PC and the one, annealed at 393 K during 6 hours [127]. Clearly in both cases dependencies of lnDcl on ln(Tg – T) were found linear, i.e. are described by the relation (82), by the slope of this dependence is lower than that for annealed PC [128]. Thus the index in the relation (82) is smaller for annealed PC compared with the initial one. It is known [127, 129] that annealing of amorphous polymers shifts their structure towards thermodynamically higher balanced state. As a consequence, data in Figure 34 allow an assumption about connection between the index in the relation (82) with the polymer structure thermodynamic state: the more unbalanced the structure is, the higher the index is [128].

Figure 34. Dependencies of the cluster diameter, Dcl, on temperature difference (Tg – T) in double logarithmic coordinates, corresponded to the relation (82), for initial (1) and annealed (2) PC [128]

For a hypothetical polymer existing in the quasi-equilibrium state, Dcl can be estimated with the help of the above-mentioned thermal cluster model, namely, by the equation (74) at βТ = 0.40. Figure 35 shows temperature dependencies of Dcl for three types of PC polymer: initial, annealed and existing in a hypothetical quasi-equilibrium state. Clearly linear correlations of Dcl(T) conforming with ref. [126] are observed for all three cases. However, the slope of linear graphs is

60

G. V. Kozlov and G. E. Zaikov

decreased with the approach of the polymer structure to thermodynamic equilibrium: from initial (0.63) to hypothetical (0.47) PC. Discussed below are data from the work [126], which indicate that though linear decrease of ξА with temperature responds to Adams and Gibbs theory [130], the slope of these dependencies is much higher than that forecasted theoretically: by three times, approximately, for PMMA and by 6 times for PS. For one of the possible reasons for this deviation (Bittrich, [126]) the nonequilibrium origin of heat fluctuations is assumed. The above-obtained results on PC allow more exact explanation of this deviation.

Figure 35. Temperature dependencies of the cluster diameter, Dcl, for PC: initial (1), annealed (2) and existing in a quasi-equilibrium state (3) [128]

Figure 36 compares of temperature dependencies of ξА in accordance with the data from [126] and Dcl, calculated for the hypothetical quasi-equilibrium state for PMMA and PS structures. Clearly the slope of Dcl(Т) dependencies is much smaller than for ξА(Т): by three times, approximately, for PMMA and by 3.5 times for PS. This approximately conforms to the deviation in slopes of theoretical and experimental ξА(Т) dependencies for the mentioned polymers, obtained in the work [126]. As a consequence, the above results indicate that the thermal cluster model correctly describe both structure of the entire amorphous polymer and its basic element (cluster) separately that might be expected due to thermofluctuation origin. Moreover, the cluster model is more general than the fluctuation glass transition theory, because it allows correct theoretical calculation of structural parameters both in thermodynamically non-equilibrium and quasi-equilibrium states, whereas Adams and Gibbs theory allows it for the latter case only [128].

Cluster Structure as a Percolation System

61

Figure 36. Temperature dependencies of CRZ characteristic length, ξА, (1, 2) and cluster diameter, Dcl, for quasi-equilibrium state (3, 4) for PMMA (1, 3) and PS (2, 4) [128]

Chapter 6

CLUSTER MODEL AS THE MODEL OF IRREVERSIBLE AGGREGATION In 1981, Witten and Sander developed the model of the particle-cluster (P-Cl) diffusion-limited aggregation (DLA) [131]. Imagine a particle present in space. Another particle making the Brownian motion appears remote from the first one. Meeting the first particle, it adheres to it, the adhesion being irreversible. Then another particle appears in the distance, diffuses and touching the primary two particles adheres to them. This process is multiply repeated. Some particles do not touch the propagating cluster during random walk, but diffuse infinitely far from it. These particles are neglected from the future consideration. Such cluster is shown in Figure 37. It was obtained using computerized Monte-Carlo method. In this method, all the totality of events is simulated in detail (the Brownian motion is given by a random number generator). Particularities of computer simulation are discussed in the work [132]. The reason for formation of branched structures (refer to Figure 37) in the P-Cl DLA model is as follows. A particle walking randomly will most probably contact cluster branches first thus increasing its size. Therefore, the probability of its penetration inside the cluster that would cause formation of a compact structure with Df = D is infinitely low. Thus cluster branches shield the internal structure of it, somewhat freezing it. As mentioned above [133], propagation of such a cluster should be considered as the phase transition between finite and infinite clusters. This formalization allows comparison of the P-Cl DLA model with others which simulate formation of an infinite system (a polymer gel). Mikin [132] has performed computerized simulation of P-Cl DLA for the case of D = 2 - 6. As

64

G. V. Kozlov and G. E. Zaikov

detected, the fractal (Hausdorff) dimensionality Df ≈ 2.5 for the Witten-Sander cluster with D = 3.

Figure 37. Two-dimensional Witten-Sander cluster composed of 11,260 particles. The adhesion coefficient (steric factor) p = 1 [132]

As indicated [8], the Witten-Sander (WS) P-Cl DLA model allows description of a great number of real physical processes and structures formed by them. Computer simulation gives an opportunity, at least, to determine the tendencies in structure variation of final aggregates under the effect of one or another factor, which is of importance for WS model application to description of the real objects. Nevertheless, under consideration of the latter computerized simulation schemes require clear physical particularization in relation to structure of the studied object. Advantages of the description of one or another process (aggregate) in the framework of P-Cl DLA model (or other aggregation models [8]) are obvious. If the cluster model of the polymer amorphous state structure can be described as WS cluster, this means their belonging to the same class of universality of physical events. Remind that the essence of the universality hypothesis is the following: if the same limiting conditions (interactions between system components) are typical of different systems, these systems belong to the same class of universality of physical events [133]. The more so this means that the polymer amorphous state structure belongs to much broader class of physical events, but not represents something isolated from other braches of physics. In

Cluster Model as the Model of Irreversible Aggregation

65

this case, it is subordinate to the general regularities of systems from the current universality class that proves theoretically the description of modern physical concepts within its framework, and the universality class is characterized by a definite selection of scaling indices [133]. It has been shown on this basis [134] that model presentations of WS clusters allow description of polymer network structures using the same scaling index, for which the fractal (Hausdorff’s) dimensionality is taken. There are many reasons (one of which is the cluster appearance, Figure 3) for association of the polymer amorphous structure in the framework of the cluster model and WS cluster. Here are three of them. The first is correspondence of the scaling index (fractal dimensionality, Df) in both models [67, 131]. The second reason is the well-known fact [135] that transition from one universality class to another is observed in the gel formation point, e.g. from cluster-cluster (Cl-Cl) to P-Cl DLA. This means that after the gel formation point the polymer represents the WS cluster. Finally, the third reason is the mechanism of local order zone formation in the cluster model. It is indicated [89] that detachment of a single segment from such zone means formation of one microcavity of fluctuation free volume, whereas addition of a segment induces “implosion” of the microcavity. In the framework of DLA model such mechanism can be identified with P-Cl aggregation that, besides Df parameter, is the basic characteristic of this class of universality [133]. Note also that the meaning of the “cluster” term in models [34] and [131] are different. In the WS model by the cluster both the local order zone (or close packing zone [136]) and chains (branches) coming out of it are meant. In the cluster model by “cluster” statistical segments only participating in the local order zone are meant. Obviously, the polymer sample structure should not be considered as WS cluster, because in such scales it represents the Euclidean object. That is why by analogy with the modified WS model [137], the polymer network structure was associated [134] with a selection of WS clusters, where every cluster is sized about 2Rcl. In accordance with the model [137] WS cluster propagation is realized on a great number of “seedings”, and Rcl parameter is bound to concentration of freely diffusing particles, c, by the following equation [137]: d −d

c = Rcl f

.

(83)

Let us discuss the physical meaning of parameter c. Figure 3 indicates that the only statistical segments of the macromolecule have the opportunity to be added

66

G. V. Kozlov and G. E. Zaikov

to the local order zone, which exist in the packless matrix. Thus c decreases with the local order, and under the condition Rcl = const this means decrease of (Df – D) or Df. Parameter c value was accepted as multiplication of the number of particles (statistical segments) per specific volume and relative part of the packless matrix. Figure 38 shows comparison of the fractal dependencies of EP e

t

structure, d f [63], and WS cluster, d f , calculated by the equation (83). The e

t

data in this Figure indicate good conformity of d f and d f values. As a consequence, modified P-Cl DLA aggregation model [137] gives good description of the polymer network structure using the expected scaling indices Df. This allows belonging of the polymer network structure to the mentioned universality class of physical systems and describes its properties in the framework of this class of relations [134]. Basically, cluster growth is induced by diffusive aggregation of particles, whereas under the stationary mode (cr = const) the following correlation is valid [138]:

c dR ~ KR , K = dr , dt R f

(84)

where t is time; cr is the rate of particle delivery to the propagation zone; R is the typical linear size of the cluster.

Figure 38. Dependencies of structure fractal dimensionalities, experimentally determined

d ef

(1, 2) and calculated by the equation (83)

Kst, for EP-1 (1, 3) and EP-2 (3, 4) [134]

d tf

, on the curing agent:oligomer relation,

Cluster Model as the Model of Irreversible Aggregation

67

If lst is accepted for R, the correlation (84) can be transformed to the following form [39]:

d ⎛⎜ l st f ⎞⎟ ⎠ ~ cr , ⎝ d −1 d T −1 l st f d

( )

(85)

where T is the cluster formation temperature. d

( ) −1

Figure 39 shows l st f T dependencies, calculated in the above-described manner, for two amorphous glassy polymers (PC and PAr). Clearly the plots show that the assumed correlation does exist, and its nonlinearity is caused by the d f −1

presence of l st term in the right part of equation (85). This means that for glassy amorphous polymers, aggregation of segments into clusters is caused by its d

( ) graphs means decrease of the

f diffusion mechanism. Curvature of l st T

−1

defect generation rate with temperature, and linearity of correlations l st (T ) , shown in Figure 40, proves this conclusion followed from consideration of the correlation (85). df

df

Figure 39. Dependencies of parameter l st [39]

on reverse temperature for PC (1) and PAr (2)

68

G. V. Kozlov and G. E. Zaikov

Power-series size distribution of objects is widely spread in the nature. Some examples of the power-series correlation between the number, N, and size, r, of defects are shown in the work [138]. General form of the correlation is as follows: N(r) ~ r-α,

(86)

where α is a constant.

d f −1

l Figure 40. Dependencies of parameter st [39]

on test temperature T for PC (1) and PAr (2)

Figure 41 shows the dependence νcl(lst) in double logarithmic coordinates for 16 polymers of different classes that corresponds to the correlation (86). This dependence is linear, which is typical fractal behavior proving the abovementioned results [39]. For the cluster WS, the following correlation characterizing variation of its density, ρWS, with the cluster radius, RWS, and fractal dimensionality, Df, is presented [136]:

⎛ RWS ⎞ ⎟ ⎝ a ⎠

ρWS = ρ c. p. ⎜

d f −d

,

(87)

where ρc.p. is the substance density in closely packed WS cluster; a is the lower border of WS cluster fractal behavior.

Cluster Model as the Model of Irreversible Aggregation

69

Figure 41. Dependence of entanglement cluster network frequency, νcl, on the length of statistical segment, lst, in double logarithmic coordinates for amorphous (1) and amorphous-crystalline (2) polymers and polymer networks (3) [39]

Let us consider equation (87) in more detail. For WS cluster, correlations Df < D and ρWS < ρc.p. (change of signs in these two inequalities by the equality sign means cluster transition to another universality class, for example, transition to the Iden cluster [133]) are determined by the condition a < RWS. At the same time, since ρWS ≠ 0 and ρc.p. ≠ 0, a cannot equal zero. Thus a compact zone (Df ≈ D) sized a does always exist in the center of WS cluster. For the polymer amorphous state structure, this compact zone is identified as the local order zone (Figure 3). This circumstance is one of the conditions of WS cluster existence [139]. Two remarks should be presented on this point. Firstly, the reason for formation of the compact zone on primary stages of WS cluster formation is easy for understanding. The fractal origin of WS cluster is determined by the screening effect of its “branches” preventing access of particles to internal cluster zones [139, 140]. However, on the primary propagation stages these “branches” are low developed, and their screening effect is also low. Secondly, the structure of polymers, as any real (physical) fractal, possesses fractal properties in a definite range of linear scales only [14]. Thus, identification of the polymer amorphous state structure as WS cluster (or, more exactly, the totality of huge amount of clusters) and the necessary existence of local order zones in the amorphous state [141]. This conclusion has been confirmed [141] by results of a value comparison in accordance with the equation (87) and sizes of the local order zones, rc.p. shown in Figure 42. For ρWS, density of the polymer packless matrix was accepted that coincides with the polymer density above Tg [93]; for ρc.p., density of crystalline zones in PC and HDPE are accepted [142, 143]. As indicated by data from Figure 42, both absolute values and tendencies of temperature variations of rc.p. and а

70

G. V. Kozlov and G. E. Zaikov

parameters display good conformity. A definite spread in a values in relation to rc.p. is induced by inaccuracy of Df assessment due to power-series dependence of a on Df (equation (87)) that causes a significant effect of the comparison accuracy. Data from Figure 42 prove the above assumption about local order zones’ necessary existence in the structure of the polymer amorphous state [141].

Figure 42. Temperature dependencies of sizes of local order zones rc.p. (1) in the model [34] and compact zones a (2) in the model [131, 139] for PC (a) and HDPE (b) [141]

As mentioned above, one of the advantages of WS model application to simulation of the polymer amorphous state structure is its thoroughly developed theoretical basis, proved by great number of computerized simulations. WS cluster growth on many “seedings” and their interaction are discussed in detail in [137]. In the framework of this model, on the example of PC and PAr, temperature variations of the structure fractal dimensionalities, Df, and the chain segment between entanglements, D, were forecasted. Two alternatives of WS cluster growth on many “seedings” (models A and B) were considered [137]. These models are thoroughly described in the works [8, 137]. Here it should be mentioned that the model A possesses two alternatives, too: with low and high −d

seeding concentrations, c0, the border between which is the concentration Rc

,

where Rc is the critical (border) radius of the WS cluster. The border value c0, calculated in this manner, was found equal 3.36×1025 and 6.40×1025 m−3 for PC and PAr polymers, respectively [144]. Let us consider physical interpretation of “seedings” for the case of the polymer amorphous state. In accordance with the model [145], an avalanche-like formation and “freezing” of local order zones proceed with temperature, T > Tg, at transition over Tg. These very local order zones are the basic structural feature of glassy polymers [34, 90]. At T > Tg macromolecular “hookings” and short-living

Cluster Model as the Model of Irreversible Aggregation

71

local order zones exclusively exist in the polymer structure [125]. As shown above, the "frozen" local order zones represent the central oriented part of the WS cluster in relation to the polymer amorphous state structure. That is why, essentially, in the case under consideration, the only candidates for the role of “seedings” are macromolecular “hookings” [144]. For the polymers under consideration, the “hooking” network frequency equals, approximately, the magnitude of 1027 m−3, more precisely, 7×1026 m−3 [112]. Thus in this case, the −d

frequency of “seedings”, c0, is greater than Rc

, and WS cluster propagation is −d f

terminated, when the amount of initial diffusing particles becomes equal Rc [137]. Analytically, this condition is expressed as follows [133]: d −d

c = Rc f

.

(88)

As before, for diffusing particles a statistical segment is accepted. In this case, c value equals [144]:

c=

1 L = , l st Sl 0 C ∞

(89)

where L is total length of macromolecules per specific polymer volume. For PC and PAr polymers, calculation of parameter Df by the equation (88) gives good conformity to experimental results [144]. As shown in Chapter 2, injection of relatively low concentrations (~ 0.01 – 1.0 wt.%) of highly disperse Fe/FeO (Z) mixture into HDPE causes significant changes in the structure and properties of HDPE + Z composites [146]. It is also indicated [146] that these effects are stipulated by formation of local order zones (clusters) by local magnetic fields of superparamagnetic domains Z. Thus Z domains represent somewhat “seedings” for amorphous phase structure formation in HDPE + Z. In its turn, this affects the structure of crystalline and interphase zones in HDPE + Z during their formation from melt. That is why the method different from the above-described one was suggested for determination of the “seedings” density, c0 [147]. Accepting in the first approximation for HDPE that Rc = 50 Å [147], the border “seeding” concentration equal ~0.8×1025 m−3 is obtained. In a natural polymer, the “seeding” density must equal the amount of clusters per specific polymer volume, Ncl, determined by the following relation: 2νcl/F [144].

72

G. V. Kozlov and G. E. Zaikov

Figure 43. Dependence of the “seeding” density, c0, on Z concentration, CZ, for HDPE + Z composites. The dashed line shows frequency of macromolecular “hooking” network for HDPE [147]

Figure 43 shows the dependence с0(Ncl) at Z concentration, CZ, for HDPE + Z composites. Dashed line in the Figure shows frequency of macromolecular “hooking” network, νh, calculated in the work [148]. Clearly the dependence с0(CZ) is of clear extreme type, corresponded to the type pf HDPE + Z composite properties variation [146]. At CZ = 0.05 wt.%, the number of “seedings” by, approximately, 2.5-fold exceeds their concentration for unmodified HDPE. For HDPE and HDPE + Z composites with CZ ≥ 0.10 wt.%, the value of νh parameter is approximately equal c0. Thus data from Figure 5.43 induce an assumption that previously detected extreme variation of HDPE + Z composite properties in CZ range of 0.01 – 0.10 wt.% is induced by the same change of the “seeding” density. In the rest cases, e.g. when Z particles do not form superparamagnetic domains, с0 = νh. Assessment of the structure change induced by c0 variation can be performed in the framework of the above-described WS model [137]. Since the minimal value of c0 (Figure 43) is, approximately, five-fold higher than the border concentration of “seedings”, the alternative of high “seedings” concentration (alternative A [137]), the basic correlation of which is equation (88), was used for assessment of structural changes [147]. Figure 44 shows comparison of fractal dimensionalities, Df, of HDPE + Z composite structure, calculated by equations (4) and (88). Clearly good correspondence by run of Df concentration dependence and absolute values of this parameter (maximal deviation does not exceed 1.5%) was obtained. The number of particles (statistical segments), nseg, in the central closely packed zone of WS cluster can be determined by the following equation [119]:

Cluster Model as the Model of Irreversible Aggregation

73

12

Rcl ⎛ n seg S ⎞ ⎟ = ⎜⎜ ⎟ 2 ⎝ πϕ cl ⎠

(90)

in accordance with equation (90) (under the condition F = 2nseg), i.e. in accordance with the cluster model of the polymer amorphous state structure and WS model, respectively. Both good qualitative and quantitative conformity is obtained again.

Figure 44. Comparison of fractal dimensionalities, df, of the structure, calculated by equations (4) (1) and (88) (2) as the function of CZ for HDPE + Z composites [147]

Figure 45. Comparison of local order zone functionality, F, calculated by equation (90) (2) as the function of Z concentration, CZ, for HDPE + Z composites [147]

As a consequence, the results have displayed [147] that besides molecular parameters S and С∞, “seeding” density, c0, is one more the important factor determining structure of the polymer amorphous state. It should be noted that the

74

G. V. Kozlov and G. E. Zaikov

crystallinity degree is the function of Df and, consequently, c0, too [123, 124]. Application of modified WS model gives an opportunity of forecasting the structure of polymers as the function of density of artificially injected “seedings” (Z in the present case) or frequency of macromolecular “hookings” [144] (chemical cross-links [134]). The energy of intermolecular interaction characterized either by molar cohesive energy, Ec, or cohesive energy density, Wc, is (besides the glass transition temperature, Tg) one of the most important characteristics of the polymer condensed state [149]. However, at present, correlations of these parameters with polymer properties are usually considered [150, 151], and there is no description of Ec (or Wc) effect on the polymer structure, though such influence is assumed quite frequently [149, 152]. Using the above-discussed models, the effect of cohesive parameters on amorphous polymer structure formation was cleared out on the example of two heterochain polyesters [153, 154]: aromatic copolyester sulfone formals (APESF) and 2,2-di-(4-oxyphenyl)propane oligoformal, phenolphthalein and isophthalic dichloranhydride (SP-OFD-10/F-1) diblock-copolyesters. Molar cohesion, Ec, can be estimated by the following equation [149]:

Tg = Tg 0

2 RTg20 n Ec

,

(91)

where Tg is the glass transition temperature of copolymer; Tg0 is the glass transition temperature of more rigid-chain component (polysulfone (PSF) for APESF and polyarylate (PAr) for SP-OFD-10/F-1); n is the part of more flexiblechain component (polyformal) in block-copolymer. However, in the framework of models applied to description of the polymer structure characteristics calculated per specific volume of the polymer are used. That is why to obtain correct correlations between cohesive characteristics and parameters of the structure, the use of density of cohesive energy, Wc, possessing “energy/volume” dimensionality (usually, MJ/m3) instead of Ec is required [155]. Figure 46 shows Wc dependencies on the composition of copolyesters, namely, on concentration of rigid blocks (PSF or PAr: CPSF and CPAr, respectively) in them. The data shown indicate that increase of rigid-chain component concentration leads to Wc increase. As a rule, such correlations are explained by formation of domains from closely packed segments in the polymer structure [149, 152]. Figure 47 shows dependencies of Tg on the formal block concentration, Cform, comparison of which with the data from Figure 46 gives

Cluster Model as the Model of Irreversible Aggregation

75

interesting results. It is known [156] that disposition of Tg dependencies with respect to composition of copolymers allows identification of their type. For example, for APESF, dependence Тg(Сform) is located above the additive glass ad

transition temperature, Tg . That is why for this polymer a tendency to regular ad

alternation of units shall be expected. For SP-OFD-10/F-1, Тg < Tg , i.e. the copolymer is inclined to formation of long sequences of the same blocks [156]. Nevertheless, for both these copolymers dependencies of Wc on composition occur beneath the appropriate additive dependence. This circumstance induces two conclusions. Firstly, in contrast with Tg dependencies on composition, the shape of analogous Wc dependence is independent of the type of copolymer. Secondly, Tg and Wc values characterize different properties of copolymers, though interdependent ones. For example, Tg is determined by rigidity of the polymer chain [157], and Wc by intensity of intermolecular interactions. In this connection, of interest is comparison of two polymers: polyamide-6 and polyvinylchloride, for which Tg are approximately equal (~323 and 343 K, respectively [155]). This is caused by approximately equal flexibility of their chains, determined by characteristic relation С∞ (6.2 and 6.7, respectively [45, 53]). However, Wc values for these polymers differ by two times (783 and 389 MJ/m3, respectively [155]).

Figure 46. Dependencies of cohesive energy density, Wc, on concentration of rigid-chain blocks, CPSF for APESF (1) and CPAr for SP-OFD-10/F-1 (2) [153]

76

G. V. Kozlov and G. E. Zaikov

Figure 47. Dependencies of the glass transition temperature, Tg, on formal block concentration, Cform, for APESF (1) and SP-OFD-10/F-1 (2) [153]

Figure 48. Correlation between cohesive energy density, Wc, and glass transition temperature, Tg, for APESF (1) and SP-OFD-10/F-1 (2) [153]

Nevertheless, correlation between Tg and cohesive characteristics are known well [158], which is explained by the above-mentioned interdependence of these parameters (refer to equation (91)). Simultaneously, the increase of the polymer chain rigidity with Tg promotes formation of closely packed domains that increases Wc (or Ec) [152]. Figure 48 shows correlation Wc(Тg) for APESF and SP-OFD-10/F-1, which is linear and reflects the above-considered interrelation. Since all data were obtained at T = 293 K, extrapolation of linear dependence Wc(Тg) to Tg = 293 K means polymer transition to devitrified state, and at this temperature Wc = 0 (anyway, in the scale of Figure 48). Broad dispersion usually observed for such correlations is caused by the fact that Тg and Wc (or Ec)

Cluster Model as the Model of Irreversible Aggregation

77

characterize different polymer properties that follows from comparison of data from Figures 46 and 47.

Figure 49. Correlation between relative part of clusters, ϕcl, and cohesive energy density, Wc, for APESF (1), SP-OFD-10/F-1 (2), PC (3), and HDPE (4) [153]

The effect of attraction and repulsion forces between particles forming WS cluster on its structure was studied [159]. It is shown that attraction force increase makes the cluster, more precisely, its external zones more packless. This aspect of amorphous polymer structure formation can also be considered in the framework of the cluster model [8]. Figure 49 shows dependence ϕcl(Wc) for APESF and SP-OFD-10/F-1. Expectedly, Wc or intermolecular attraction force intensification causes increase of the relative part of closely packed local order zones in the structure of copolymers. Data in the Figure on PC and HDPE [5] conform to ϕc(Wc) correlation, obtained for copolymers under consideration. This indicates quite high generality of the correlation [8]. Figure 50 shows dependencies of WS cluster density, ρfr (equation (2)) on the relative part of packless matrix, ρp.m., for APESF and SP-OFD-10/F-1, which indicate ρfr increase with ρp.m., i.e. ϕcl or Wc decreased (Figure 49). Thus similar to computerized simulation [159], attraction forces increase between particles (statistical segments), characterized by Wc increase, induces higher loosening (ρfr decrease) of external zones in WS clusters, identified as the packless matrix [154]. Note also that at Tg relative free volume, ff, increases with the polymer chain rigidity (or Wc, refer to Figure 48) [95]. Clearly Wc increase induces ϕcl growth (Figure 49) and ρp.m. decrease (Figure 50) and consequently, ff increase. Thus application of the WS model does also explain this feature of amorphous polymer structure [154].

78

G. V. Kozlov and G. E. Zaikov

Figure 50. Dependencies of WS cluster density, ρfr, determined by equation (2) (1, 2) and packless matrix density, ρp.m., determined by equation (92), on the relative part of packless matrix, ϕp.m., for APESF (1, 3) and SP-OFD-10/F-1 (2) [154]

Free particles are used in computerized simulation of WS clusters, whereas the principal difference of the polymer structure is linking of statistical segments forming it to the chain by strong covalent bonds. This restricts their motion. That is why ϕcl and ϕp.m. variations can be accompanied by redistribution of frequencies of these structural components only. This effect can be estimated using simple rule of mixtures:

ρ = ρclϕcl + ρp.m.ϕp.m.,

(92)

where ρ is the polymer density; ρcl and ρp.m. are densities of clusters and the packless matrix, respectively. Taking for ρ experimentally determined densities of copolyesters and assuming ρcl = 1.08ρ [142], one can estimate ρp.m. variation with ϕp.m., (under the assumption that ρfr ~ ρp.m.). Figure 50 shows the dependence ρp.m.(ϕp.m.), which can be coincident with the correlation ρfr(ϕp.m.) by simple adjustment of the scale, because ρfr values are given in relative units. Thus application of the WS model gives quite full picture of intermolecular interaction forces effect on formation of the amorphous polymer structure. The increase of Wc characterizing intensity of intermolecular attraction forces induces growth of the local order degree, ϕcl. This effect is accompanied by loosening of the packless matrix by means of segments redistribution in structural components of the amorphous polymer [154].

Cluster Model as the Model of Irreversible Aggregation

79

It has been shown [131] that autocorrelation function: c(r) = (p(r′)⋅p(r′ + r)),

(93)

where р(r′) and р(r′ + r) are probabilities of the presence of particles, from which the cluster is composed (the probability equals 1 in the presence and 0 in the absence of the particle), in points r′ and r′ + r, can be presented by the following scaling relation: с(r) ~ r−α,

(94)

for distances r greater than several steps of the lattice. In the relation (94), α is determined by the difference as follows [139]:

α = D − Df.

(95)

As a consequence, by determining the slope, α, of linear autocorrelation function, one can estimate the fractal dimensionality of the object, Df, using relations (94) and (95) [160]. Figure 51 shows schematic presentation of the autocorrelation function for the structure of amorphous polymer. Here variation of density is presented by the function of distance, r, and the origin of coordinates (r = 0) is disposed in the center of the local order zone (refer to Figures 2 and 3). In some interval from 0 to rlz (where rlz is the radius of the local order zone) parameter ρ is constant and equals density of the local order zone, which in the first approximation is accepted equal the appropriate ρcr value for crystalline polymer (particularly, for PC [160]). Then in the interval from rlz to Rcl a linear decrease of ρ to some ρmin value is assumed, assessed as follows. The average density of amorphous PC, ρа, was calculated [142], corresponded to the middle of the sloped linear part of ρ(r) dependence in Figure 51.Then basing on simple geometrical ideas, one may obtain the following [160]:

ρmin = ρа – (ρcr − ρа).

(96)

Further on, parameter α can be assessed from the following correlation [160]: (ρcr − ρmin) ~ (Rcl – rlz)−α,

(97)

80

G. V. Kozlov and G. E. Zaikov

and then Df value by equation (95) can be calculated. Figure 52 shows comparison of temperature dependencies of the fractal dimensionality values of PC structure:

( ) calculated by the equation (4) and theoretical ones within the framework of the model suggested (d ) calculated by equations (95) e

experimental values d f

t f

and (97).

Figure 51. Schematic presentation of the function ρ(r) for amorphous polymer [160]

Clearly good conformity between theoretical and experimental results is observed (deviation below 10%). However, this conformity can be improved e

using the following methodological method. To assess d f in accordance with the equation (4), ν parameter was determined from the equation (12). If in this equation the real yield stress,

σ yr , estimated as follows, is used instead of

technical one, σy, [59]:

σ yr = σy(1 + εy),

(98)

where εy is the yield deformation, somewhat lower ν value will be obtained. Data in Figure 52 indicate that the adjustment gives much better conformity between

d ef and d tf for PC. For PC also at T = 293 K Df value was determined [67] by five different methods that gave, on average, Df = 2.51. This result conforms well to Df value at T = 293 K, obtained in the framework of the WS model (Df = 2.56, Figure 53) [160].

Cluster Model as the Model of Irreversible Aggregation

81

Figure 52. Dependence of fractal dimensionality, df, of PC structure on test temperature, T. r Calculation was performed by equation (4) using σy (1) and σ y (2); by equations (95) and (97) (3) [160]

Figure 53. Dependence of steric factor, p, on cross-linking frequency, νс, for EP-2 (1) and EP-3 (2) [162]

As observed in the framework of computerized simulation of DLA clusters, the steric factor p (р ≤ 1) indicating that not all collisions of particles happen with orientation necessary for particle “adhesion” to the cluster plays the important role basically defining the aggregation mechanism and structure of the final aggregate, characterized by its fractal dimensionality, Df [159, 161]. For example, at high p approaching 1 the diffusion-limited mechanism of the aggregate propagation with relatively low values Df is realized. On this basis an attempt was made [162] to clear out the effect of cross-linking frequency, νс, on p and conditions of local order zone formation for polymer networks, EP-2 and EP-3. For WS clusters, one can write down as follows [133]:

82

G. V. Kozlov and G. E. Zaikov

p~

1 , rlz

(99)

The proportionality factor in the correlation (99) can be approximately assessed as follows. The distance between chemical cross-link points, Rc, was calculated and then the proportionality factor was determined from the correlation (99) under the condition rlz = Rc and the appropriate minimal value p = 0.1. Figure 53 shows dependence р(νс), found linear. Clearly νс increase leads to p growth, which is accompanied by Df decrease [68]. This conforms to general statements of the model [161]. There are data [163, 164] displaying that νс increase induces cluster network frequency increase, νсl, and decrease of the number of segments, nseg, in a single cluster. This means formation of a large number of small clusters, Ncl (= νcl/nseg). Figure 54 shows dependence Ncl(р) that indicates linear increase of Ncl with p (or νс, refer to Figure 53). However, dependence Ncl(р) does not pass through the origin of coordinates, and at Ncl = 0 value of p is finite and equals ~0.215. This means that at р ≤ 0.215 the cluster network is not formed or, to put it differently, polymer network does not transit to the glassy state. Figure 53 indicates that p = 0.215 corresponds to νс = 2.2×1026 m−3, and at νс below the mentioned value the cross-linkable polymer does not transit to the condensed state. The critical value

( )

ν c ν ccr can also be estimated

theoretically. The condition Ncl = 0 and, consequently, νcl = 0 is the criterion of polymer transition to the rubbery state [121]. For such state, fractal dimensionality D of a part of chain between cross-link points that characterizes molecular mobility equals 2 [120]. Moreover, for the series of epoxy polymers under consideration, the maximum of С∞ (at the minimum of νс) equals 4.8 [165]. This allows determination of maximal Df for epoxy polymers by equation (42) and then the number of segments, nseg, between chemical cross-link points by equation (56). In accordance with the relation (42) and at D = 2 and Df = 2.737, nseg = 23.3 was obtained from equation (56) and the chain length between cross-link points, Lc, was calculated by equation (57). After assessment of the total length of macromolecules, L, per specific volume of the polymer one can determine via L/Lc, whence it follows that

ν ccr

ν ccr = 2.1×1026 m−3. This theoretical value of

ν ccr conforms properly to the appropriate experimental one, graphically estimated from the data in Figure 54 (ν c = 2.2×1026 m−3). cr

Cluster Model as the Model of Irreversible Aggregation

83

Extrapolation of р(νс) curve (Figure 53) to the maximum p = 1 gives the maximum of νс

(ν ) equal ~26×10 max c

26

m−3. At this νс value the following fractal

dimensionalities shall be obtained: D = 1 and Df = 2 [5]. Under these conditions, nst = 2 from equation (56) and Lc = 12 Å from equation (57) are obtained. Then theoretical value of

ν cmax may be estimated as ~24.5×1026 m−3, which again

conforms well to the above experimental assessment. Moreover, the minimum of nst = 2 conforms completely to the analogous assessment for completely crosslinked polymers [125].

Figure 54. Dependence of the number of local order zones, Ncl, per specific volume of the polymer on steric factor, p, for EP-2 (1) and EP-3 (2) [162]

Thus the above-considered results indicate that chemical cross-link point frequency, νс, regulating conformation of the chain part between them determines the steric factor, p: the higher νс is, the greater p is. This means that νс increase forms the chain conformation favorable for statistical segments’ packing in the local order zone. Therefore, this circumstance determines formation of a large number of small clusters at high νс values [162]. In Section 5 the notion of quasi-equilibrium state of the polymer structure corresponded to the balance of tendencies to local order and entropic chain strain increase was introduced [9]. Generally, this state is characterized by Df = 2.5. It should be noted that at N → ∞ (where N is the number of particles in the cluster) this value of Df coincides with the fractal dimensionality of the WS cluster for three-dimensional space [132]. In contrast with the primary Witten-Sander model [131], in which WS cluster growth is unlimited (N → ∞), an interaction between WS clusters occurs in the modified simulation at multiple growth points [137],

84

G. V. Kozlov and G. E. Zaikov

and the condition of the process termination is obtained. That is why the conformity of quasi-equilibrium state formation conditions in cluster and WS models was considered [166]. Data from the literature for a series of amorphous and amorphous-crystalline polymers were considered [166]. For these polymers, the “seeding” density c0 = Ncl = 2νcl/F and macromolecular “hooking” network frequency, νh, were determined using Mh values from the literature [45, 53]. Figure 55 shows comparison of Ncl and νh values for 8 polymers under the strain and stress relaxation tests. Clearly quite good conformity of these parameters by both absolute values and the tendency of their variations was obtained. Quite broad dispersion is explained by corresponded deviation in Mh values from different literature sources, obtained for one and the same polymer (for example, for polyethylene Mh = 1,900 g/mol [53] and 1,390 g/mol [45], respectively). Nevertheless, Figure 55 indicates that the condition Ncl = νh allows identification of νl parameter as the “seeding” density [166].

Figure 55. Correlation between cluster density, Ncl, and macromolecular “hooking” network frequency, νh, for 8 amorphous and amorphous-crystalline polymers. The continuous line marks 1 : 1 ratio [166]

The simulation [137] assumes the presence of such parameter as the diffusion length, ξ, depended on the local environing of every “seeding”. Fractal propagation of WS cluster lasts until the condition ξ = Rc is reached [137]. Parameters ξ and Rc are bound to the concentration of free particles, c, as follows [137]: d −d + 2

ξ 2 = c −1 Rc f

.

(100)

Cluster Model as the Model of Irreversible Aggregation

85

Substituting the above condition of WS cluster termination into equation (100), the criterion (88) is obtained that gives concentration of free particles, c, at the moment of WS cluster termination, when it reaches radius Rc (hereinafter, cWS), or as in the framework of the WS model the quasi-equilibrium state is reached, because in this case, too, the structure invariance is determined by the balance of tendencies: diffusive propagation is limited by interaction of neighboring WS clusters [166]. In accordance with the relation (88) the use of dimensional Rc values induces cSW dependence on dimensionality of the length, selected for Rc. That is why for normalizing factor the lower scale of the fractal behavior (bl = 5 Å) was chosen [166], and dimensionless parameter (Rc/bl) was used in the equation (88). Selection of another bl value will change quantitative estimations of cSW insignificantly and is negligible for tendencies in their variations. In the framework of the cluster model (Figure 3), the ability to be added to the local order zone is inherent to the only segments, present in the packless matrix. As a consequence, in terms of the WS model these very segments represent free particles. That is why in the framework of the cluster model under reaching a quasi-equilibrium state, the concentration of the free particles, ccr, will equal the relative part of the packless matrix,

ϕ cr p.m. , in this state. This parameter was

calculated as follows. First, Df corresponded to the quasi-equilibrium state [41] was determined from the equation (42); sequentially, ϕcl and as (1 -

ϕ cr p.m. as (1 - ϕcl) (or

ϕ clmax ) for amorphous-crystalline polymers, equation (80)), which equals

ccr (see above) for the quasi-equilibrium state were determined from equation (7) [166]. Figure 56 gives comparison of cWS and ccr for 12 amorphous and amorphouscrystalline polymers. Clearly correspondence of these parameters indicating, in its turn, the conformity between interpretations of quasi-equilibrium states of the polymer structure in the cluster and WS models is observed. Somewhat overestimated cWS values over ccr are induced by arbitrary choice of bl value. Briefly resuming results of the present Chapter, note that the cluster model of the polymer amorphous state conforms both qualitatively and quantitatively to the modern physical concepts, which can be applied to description of the polymer structure. Applications of one or another alternative of the combined models allows significant expansion of the analytical abilities of the structure description and obtaining of principally new ideas on it.

86

G. V. Kozlov and G. E. Zaikov

Figure 56. Correlation between concentrations of free particles, cWS, and statistical segments in the packless matrix, ccr, for quasi-equilibrium states for 12 amorphous and amorphous-crystalline polymers. Dashed line marks 1 : 1 ratio [166]

REFERENCES [1] [2] [3] [4] [5] [6]

[7] [8] [9]

[10] [11] [12] [13] [14]

Feder J., Fractals, New York, Plenum Press, 1988, 254 p. Ivanova V.S., Balankin A.S., Bunin I.Zh., and Oksogoev A.A., Synergism And Fractals In The Material Science, 1994, Moscow, Nauka, 383 p. (Rus) Novokov V.U and Kozlov G.V., Uspekhi Khimii, 2000, vol. 69(4), pp. 378 393. (Rus) Novokov V.U and Kozlov G.V., Uspekhi Khimii, 2000, vol. 69(6), pp. 572 599. (Rus) Kozlov G.V. and Novikov V.U., Synergism And Fractal Analysis Of Polymer Networks, 1998, Moscow, Klassika, 112 p. (Rus) Novikov V.U. and Kozlov G.V., Analysis of Polymer Destruction In The Framework Of The Concept Of Fractals, 2001, Moscow, Izd. MGOU, 136 p. (Rus) Fractals And Local Order In Polymer Materials, Ed. G.V. Kozlov and G.E. Zaikov, 2001, New York, Nova Science Publishers. Inc., 190 p. Shogenov V.N. and Kozlov G.V., Fractal Clusters In Physicochemistry Of Polymers, 2002, Nalchik, Poligrafservis i T., 268 p. (Rus) Kozlov G.V. and Zaikov G.E., In Coll.: Fractals And Local Order In Polymer Materials, Ed. G.V. Kozlov and G.E. Zaikov, 2001, New York, Nova Science Publishers, Inc., pp. 55 - 64. Gladyishev G.P. and Gladyishev D.P., On Physicochemical Theory Of Bilogical Evolution (Preprint), 1993, Moscpw, Olimp, 24 p. (Rus) Gladyishev G.P. and Gladyishev D.P., Zh. Fiz. Khim., 1994, vol. 68(5), pp. 790 - 792. (Rus) Hornbogen E., Int. Mater. Rev., 1989, vol. 34(6), pp. 277 - 296. Bessendorf M.H., Int. J. Eng. Sci., 1987, vol. 25(6), pp. 667 - 672. Zemlyanov M.G., Malinovsky V.K., Novikov V.N., Parshin P.P., and Sokolov A.P., Zh. Eksper. Teor. Fiz., 1992, vol. 101(1), pp. 284 - 293. (Rus)

88

G. V. Kozlov and G. E. Zaikov

[15] Kozlov G.V., Ozden S., Krysov V.A., and Zaikov G.E., In Coll.: Fractals And Local Order In Polymeric Materials, Ed. G.V. Kozlov and G.E. Zaikov, 2001, New York, Nova Science Publishers, Inc., pp. 83 - 88. [16] Kozlov G.V., Ozden S., and Dolbin I.V., Russian Polymer News, 2002, vol. 7(2), pp. 35 - 38. [17] Bagryansky V.A., Malinovsky V.K., Novikov V.N., Pushchaeva L.M., and Sokolov A.P., Fizika Tverdogo Tela, 1988, vol. 30(8), pp. 2360 – 2366. (Rus) [18] Balankin A.S., Synergism of Deformable Body, 1991, Moscow, MO SSSR, 404 p. (Rus) [19] Kozlov G.V., Belousov V.N., and Mikitaev A.K., High Pressure Physics and Technology, 1998, vol. 8(1), pp. 64 - 70. (Rus) [20] Flory P.J., Brit. Polymer J., 1976, vol. 8(1), pp. 1 - 10. [21] Balankin A.S., Bugrimov A.L., Kozlov G.V., Mikitaev A.K., and Sanditov D.S., Doklady AN, 1992, vol. 326(3), pp. 463 - 466. (Rus) [22] Sokolov I.M., Uspekhi Fizicheskikh Nauk, 1986, vol. 150(2), pp. 221 - 256. (Rus) [23] Song H.-H. and Roe R.-J., Macromolecules, 1987, vol. 20(11), pp. 2723 2732. [24] Rammal R. and Toulouse G., J. Physiq. Lettr., 1983, vol. 44(1), pp. L13 L22. [25] Balankin A.S., Pis’ma V ZhTF, 1991, vol. 17(6), pp. 84 - 89. (Rus) [26] Novikov V.U., Kozlov G.V., and Boronin D.V., Materialovedenie, 1999, No. 3, pp. 25 – 28. (Rus) [27] Meakin P., Phys. Rev. Lett., 1983, vol. 51(13), pp. 1119 - 1122. [28] Kolb M., Botet R., and Jullien R., Phys. Rev. Lett., 1983, vol. 51(13), pp. 1123 - 1126. [29] Family F., Phys. Rev. Lett., 1983, vol. 51(23), pp. 2112 - 2115. [30] Irzhak V.I., Rozenberg B.A., and Enikolopyan N.S., Polymer Networks: Synthesis, Structure, Properties, 1978, Moscow, Nauka, 248 p. (Rus) [31] Kozlov G.V., Beloshenko V.A., Stroganov I.V., and Lipatov Yu.S., Doklady NAN Ukrainy, 1995, No. 10, pp. 117 - 118. (Rus) [32] Kozlov G.V., Burya A.I., and Zaikov G.E., Inzhenerno-Fizicheskii Zhurnal, 2003, vol. 77, No. 1 (in press). (Rus) [33] Katz A.J. and Tompson A.H., Phys. Rev. Lett., 1985, vol. 54(12), pp. 1325 1328. [34] Kozlov G.V. and Novikov V.U., Uspekhi Fizicheskikh Nauk, 2001, vol. 171(7), pp. 717 - 764. (Rus)

References

89

[35] Kozlov G.V., Beloshenko V.A., Varyukhin V.N., and Lipatov Yu.S., Polymer, 1999, vol. 40(4), pp. 1045 - 1051. [36] Beloshenko V.A. and Kozlov G.V., Mekhanika Kompozitnyikh Materialov, 1994, vol. 30(4),pp. 451 - 454. (Rus) [37] Kozlov G.V., Belousov V.N., Serdyuk V.D., and Kuzhetsov E.N., High Pressure Physics and Technology, 1995, vol. 5(3), pp. 59 - 64. (Rus) [38] Smirnov B.M., Uspekhi Fizicheskikh Nauk, 1986, vol. 149(2), pp. 177 219. (Rus) [39] Kozlov G.V., Beigelzimer Ya.E., Gazaev M.A., Novikov V.U., and Mikitaev A.K., Fractal Physics Of The Polymer Amorphous State, Manuscript deposited to VINITI RAS, Moscow, December 05, 1995, No. 3221-V95. (Rus) [40] Flory P.J., J. Chem. Phys., 1977, vol. 66(12), pp. 5720 - 5729. [41] Kozlov G.V., Aloev V.Z., and Lipatov Yu.S., Doklady NAN Ukrainy, 2001, No. 3, pp. 150 - 154. (Rus) [42] Kozlov G.V., Beloshenko V.A., Gazaev M.A., and Varyukhin V.N., High Pressure Physics and Technology, 1995, vol. 5(1), pp. 74 - 80. (Rus) [43] Careri G., Ordine E Disordine Nella Materia, Laterza, 1982, 228 p. [44] Ivanova V.S., Synergism. Strength And Destruction Of Metal Materials, 1992, Moscow, Mir, 160 p. (Rus) [45] Wu S., J. Polymer Sci., Part B, Polymer Phys., 1989, vol. 27(4), pp. 723 741. [46] Wu S., J. Appl. Polymer Sci., 1992, vol. 46(4), pp. 619 - 624. [47] Boyer R.F., Macromolecules, 1992, vol. 25(20), pp. 5326 - 5330. [48] Boyer R.F. and Miller R.L., Macromolecules, 1977, vol. 10(5), pp. 1167 1169. [49] Balankin A.S., Pis’ma V ZhTF, 1990, vol. 16(7), pp. 14 - 20. (Rus) [50] Aliguliev R.M., Khiteeva D.M., and Oganyan V.A., Vysokomol. Soedin., 1988, vol. B30(4), pp. 268 - 272. (Rus) [51] Aliguliev R.M., Khiteeva D.M., Oganyan V.A., and Nuriev R.A., Doklady AN AzSSR, 1989, vol. 45(5), pp. 28 - 31. (Rus) [52] Perepechko I.I. and Maksimov A.V., Vysokomol. Soedin., 1989, vol. B31(1), pp. 54 - 57. (Rus) [53] Aharoni S.M., Macromolecules, 1983, vol. 16(9), pp. 1722 - 1728. [54] Novikov V., Gazaev M., and Kozlov G., Proc. Second Symposium “Advances in Structured and Heterogeneous Continua”, August 14 - 16, 1995, Moscow, Russia, p. 45. [55] Kozlov G.V., Gazaev M.A., Novikov V.U., and Mikitaev A.K., Behavior Of Dissipative Structures In Deformable Polymer Matrices, Manuscript

90

[56] [57] [58] [59]

[60] [61] [62] [63]

[64] [65] [66] [67] [68] [69] [70] [71] [72] [73]

G. V. Kozlov and G. E. Zaikov deposited to VINITI RAS, Moscow, November 03. 1995, No. 2944-V95. (Rus) Kozlov G.V., Beloshenko V.A., Novikov V.U., and Lipatov Yu.S., Ukrainsky Khimichesky Zhurnal, 2001, vol. 67(3), pp. 57 - 60. (Rus) Shogenov V.N., Belousov V.N., Potapov V.V., Kozlov G.V., and Prut E.V., Vysokomol. Soedin., 1991, vol. A33(1), pp. 155 - 160. (Rus) Kozlov G.V., Shustov G.B., and Temiraev K.B., Vestnik KBGU, Ser. Khimicheskie Nauki, 1997, No. 2, pp. 50 - 52. (Rus) Kozlov G.V. and Sanditov D.S., Anharmonic Effects And Physicomechanical Properties Of Polymers, 1994, Novosibirsk, Nauka, 261 p. (Rus) Budtov V.P., Physical Chemistry Of Polymer Solutions, 1992, SaintPetersburg, Khimia, 384 p. (Rus) Kozlov G.V., Temiraev K.B., and Shustov G.B., Plast. Massy, 1998, No. 9, pp. 27 - 29. (Rus) Kozlov G.V., Burmistr M.V., Korenyako V.A., and Zaikov G.E., Voprosy Khimii I Khimicheskoi Tekhnologii, 2002, No. 6, pp. 77 – 81. (Rus) Kozlov G.V., Beloshenko V.A., Gazaev M.A., and Novikov V.U., Mekhanika Kompozitnyikh Materialov, 1996, vol. 32(2), pp. 270 - 278. (Rus) Gazaev M.A., Kozlov G.V., Milman L.D., and Mikitaev A.K., High Pressure Physics and Technology, 1996, vol. 6(1), pp. 76 - 81. (Rus) Lyubchenko L.S. and Lyubchenko M.L., Khimicheskaya Fizika, 1997, vol. 16(8), pp. 24 - 51. (Rus) Kozlov G.V., Burya A.I., Sviridenok A.I., and Zaikov G.E., Doklady NAI Belarusi, 2003, vol. 47 (in press). Kozlov G.V., Gazaev M.A., Novikov V.U., and Mikitaev A.K., Pis’ma V ZhTF, 1996, vol. 22(16), pp. 31 - 38. (Rus) Kozlov G.V., Novikov V.U., Gazaev M.A., and Mikitaev A.K., InzhenernoFizicheskyi Zhurnal, 1998, vol. 71(2), pp. 241 - 247. (Rus) Porter D., Polymer, 1987, vol. 28(8), pp. 1652 - 1656. Donald A.M., Kramer E.J., and Bubeck R.A., J. Polymer Sci., Polymer Phys. Ed., 1982, vol. 20(7), pp. 1129 - 1141. Wu S., ”Benibana” Int. Symp. October 8-11, 1990, Yamagata, Japan, Abstract, Yamagata, Japan, 1990, pp. 130 - 137. Lipatov Yu.S. and Privalko V.P., J. Macromol. Sci.-Phys., 1973, vol. B7(3), pp. 431 - 444. Haward R.N. and Thackray G., Proc. Royal Soc. Lond., 1968, vol. A302(1471), pp. 453 - 472.

References

91

[74] Plummer C.J.G. and Donald A.M., Macromolecules, 1990, vol. 23(7), pp. 3929 - 3937. [75] Edwards S.F. and Vilgis T., Polymer, 1987, vol. 28(3), pp. 375 - 378. [76] Balankin A.S., Ivanova V.S., and Breusov V.P., Doklady AN, 1992, vol. 322(6), pp. 1080 - 1085. (Rus) [77] Kozlov G.V., Temiraev K.B., Shetov R.A., and Mikitaev A.K., Materialovedenie, 1999, No. 2, pp. 34 - 39. (Rus) [78] Kozlov G.V., Ozden S., and Zaikov G.E., In book: Fractal Analysis of Polymers: From Synthesis to Composites, Ed. Kozlov G., Zaikov G., and Novikov V., New York, Nova Science Publishers, Inc., 2003, p. 113-121. [79] Caush G., Destruction Of Polymers, 1981, Moscow, Mir, 440 p. (Rus) [80] Kozlov G.V., Belousov V.N., Sanditov D.S., and Mikitaev A.K., Izvestiya VUZov, Severo-Kavkazsky Region, Estestvennye Nauki, 1994, No. 1 – 2(86), pp. 54 - 58. (Rus) [81] Aharoni S.M., Macromolecules, 1985, vol. 18(12), pp. 2624 - 2630. [82] Hong S.-D., Chung S.Y., Fedords R.F., and Moacanin J., J. Polymer Sci.: Polymer Phys. Ed., 1983, vol. 21(9), pp. 1647 - 1660. [83] Sanditov D.S., Kozlov G.V., Belousov V.N., and Lipatov Yu.S., Ukrainian Polymer J., 1992, vol. 1(3-4), pp. 241 - 258. [84] Frenkel Ya.I., Kinetic Theory Of Liquids, 1945, Moscow-Leningrad, Izd. AN SSSR, 424 p. (Rus) [85] Ferry J.D., Viscoelastic Properties of Polymers, 3rd Ed., New York, Wiley and Sons, 1980, 522 p. [86] Sanditov D.S. and Bartenev G.M., Physical Properties of Non-Oriented Structures, 1982, Novosibirsk, Nauka, 256 p. (Rus) [87] Sanditov D.S. and Kozlov G.V., Vysokomol. Soedin., 1996, vol. A36(8), pp. 1389 - 1393. (Rus) [88] Sanditov D.S., Sangadiev S.Sh., and Kozlov G.V., Fizika I Khimia Stekla, 1998, vol. 24(6), pp. 758 - 766. (Rus) [89] Sanditov D.S., Kozlov G.V., Belousov V.N., and Lipatov Yu.S., Fizika I Khimia Stekla, 1994, vol. 20(1), pp. 3 - 13. (Rus) [90] Belousov V.N., Kozlov G.V., Mikitaev A.K., and Lipatov Yu.S., Doklady AN SSSR, 1990, vol. 313(3), pp. 630 - 633. (Rus) [91] Sanditov D.S. and Kozlov G.V., Fizika I Khimia Stekla, 1993, vol. 19(4), pp. 593 - 601. (Rus) [92] Kozlov G.V., Beloshenko V.A., and Lipskaya V.A., Ukrainsky Fizichesky Zhurnal, 1996, vol. 41(2), pp. 222 - 225. (Rus) [93] Belousov N.V., Beloshenko V.A., Kozlov G.V., and Lipatov Yu.S., Ukrainsky Khimichesky Zhurnal, 1996, vol. 62(1), pp. 1 - 4. (Rus)

92

G. V. Kozlov and G. E. Zaikov

[94] Lipatov Yu.S., Uspekhi Khimii, 1978, vol. 47(2), pp. 332 - 366. (Rus) [95] Sanchez I.C., J. Appl. Phys., 1974, vol. 45(10), pp. 4204 - 4215. [96] Beloshenko V.A., Kozlov G.V., and Varyukhin V.N., High Pressure Physics And Technology, 1994, vol. 4(2), pp. 70 -74. (Rus) [97] Sanditov D.S. and Kozlov G.V., Fizika I Khimia Stekla, 1995, vol. 21(6), pp. 547 - 576. (Rus) [98] Knopoff L. and Shapiro J.N., Phys. Rev. B, 1970, vol. 1(10), pp. 3893 3895. [99] Sharma B.K., Acoust. Lett., 1980, vol. 4(2), pp. 19 - 23. [100] Sharma B.K., Acoust Lett., 1980, vol. 4(1), pp. 11 - 14. [101] Olemsky A.I., Katsnelson A.A., and Umrikhin V.V., Fizika Tverdogo Tela, 1985, vol. 27(2), pp. 318 - 321. (Rus) [102] Kozlov G.V. and Mikitaev A.K., Vysokomol. Soedin., 1987, vol. B29(7), pp. 490 - 492. (Rus) [103] Kozlov G.V., Shetov R.A., and Mikitaev A.K., Doklady AN SSSR, 1986, vol. 290(4), pp. 885 - 888. (Rus) [104] Cohen M.H. and Grest G.S., Phys. Rev. B, 1979, vol. 20(3), pp. 1077 1098. [105] Chen H.S., J. Non-Cryst. Solids, 1981, vol. 46(3), pp. 289 - 305. [106] Manevich L.I., Oshmyan V.G., Gai M.I., Akopyan E.L., and Enikolopyan N.S., Doklady AN SSSR, 1986, vol. 289(1), pp. 128 - 131. (Rus) Margolina A. and Wu S., Polymer, 1988, vol. 29(12), pp. 2170 - 2173. [107] [108] Bridge B., J. Mater. Sci. Lett., 1989, vol. 8(2), pp. 102 - 103. [109] Patrikeev G.A., Doklady AN SSSR, 1968, vol. 183(9), pp. 636 - 639. (Rus) [110] Patrikeev G.A., Mekhanika Polimerov, 1971, No. 2, pp. 221 - 231. (Rus) [111] Kozlov G.V., Sanditov D.S., Milman L.D., and Serdyuk V.D., Izvestiya VUZov. Severo-Kavkazskyi Region, Estestvennye Nauki, 1993, No. 3 – 4(83-84), pp. 88 - 92. (Rus) [112] Prevorsek D.C. and De Bona B.T., J. Macromol. Sci.-Phys., 1981, vol. B19(4), pp. 605 - 622. [113] Shustov G.B., Belousov V.N., Kozlov G.V., and Mikitaev A.K., Carcass Coherency And Mechanical Properties Of Extruded Amorphous Polymers, Manuscript disposed to VINITI RAS, Moscow, February 26, 1997, No. 626-V97. (Rus) [114] Kozlov G.V., Aloev V.Z., Bazheva R.Ch., and Zaikov G.E., In Coll.: IV AllRussian Sci.-Tech. Conf. “New Chemical Technologies: Production and Application”, Penza, PGU, 2002, pp. 59 – 61. (Rus) [115] Shklovsky B.I. and Efros A.L., Uspekhi Fizicheskikh Nauk, 1975, vol. 117(3), pp. 401 - 436. (Rus)

References

93

[116] Family F., J. Stat. Phys., 1984, vol. 36(5/6), pp. 881 - 896. [117] Kozlov G.V. and Dolbin I.V., Mater. Intern. Conf. “Physics of Electronic Materials”, Kaluga, Russia, Oct. 1-4, 2002, p. 134 - 135. [118] Kozlov G.V., Beloshenko V.A., and Lipatov Yu.S., Ukrainsky Khimichesky Zhurnal, 1998, vol. 64(3), pp. 56 - 59. (Rus) [119] Bobryishev A.N., Kozomazol V.N., Babin L.O., and Solomatov V.I., Synergism Of Composite Materials, 1994, Lipetsk, NPO ORIUS, 153 p. (Rus) [120] Kozlov G.V., Serdyuk V.D., and Dolbin I.V., Materialovedenie, 2000, No. 12, pp. 2 - 5. (Rus) [121] Beloshenko V.A., Kozlov G.V., and Lipatov Yu.S., Fizika Tverdogo Tela, 1994, vol. 36(10), pp. 2903 - 2906. (Rus) [122] Bartenev G.M. and Frenkel S.Ya., Physics Of Polymers, 1990, Leningrad, Khimia, 432 p. (Rus) [123] Kozlov G.V., Beloshenko V.A., Varyukhin V.N., and Novikov V.U., Zhurnal Fizicheskikh Issledovanii, 1997, vol. 1(2), pp. 204 - 207. (Rus) [124] Aloev V.Z., Kozlov G.V., and Beloshenko V.A., Izvestiya KBNTs RAN, 2000, No. 1(4), pp. 108 - 113. (Rus) [125] Berstein V.A. and Egorov V.M., Differential Scanning Calorimetry In Physicochemistry Of Polymers, 1990, Leningrad, Khimia, 256 p. (Rus) [126] Bittrich H.-J., Acta Polymerica, 1982, vol. 33(12), p. 741. [127] Kozlov G.V., Burya A.I., Sanditov D.S., Serdyuk V.D., and Lipatov Yu.S., Materialy, Tekhnologii, Instrumenty, 1999, vol. 4(2), pp. 51 - 54. (Rus) [128] Kozlov G.V. and Lipatov Yu.S., Vysokomol. Soedin., 2003, vol. B45(4), pp. 660 - 664. (Rus) [129] Kozlov G.V., Sanditov D.S., and Lipatov Yu.S., In Coll.: Fractals And Local Order In Polymeric Materials, Ed. G.V. Kozlov and G.E. Zaikov, New York, Nova Science Publishers, Inc., 2001, pp. 65 - 82. [130] Adam G. and Gibbs J.H., J. Chem. Phys., 1965, vol. 43(1), pp. 139 - 146. [131] Witten T.A. and Sander L.M., Phys. Rev. Lett., 1981, vol. 47(19), pp. 1400 1403. [132] Meakin P., Phys. Rev. A, 1983, vol. 27(3), pp. 1495 - 1507. [133] Kokorevich A.G., Gravitis Ya.A., and Ozon’-Kalnin V.G., Khimia Drevesiny, 1989, No. 1, pp. 3 – 24. (Rus) [134] Kozlov G.V., Beloshenko V.A., and Varyukhin V.N., Ukrainsky Fizichesky Zhurnal, 1998, vol. 43(3), pp. 322 - 323. (Rus) [135] Botet R., Jullien R., and Kolb M., Phys. Rev. A, 1984, vol. 30(4), pp. 2150 2152. [136] Brady R.M. and Ball R.C., Nature, 1984, vol. 309(5965), pp. 225 - 229.

94

G. V. Kozlov and G. E. Zaikov

[137] Witten T.A. and Meakin P., Phys. Rev. B, 1983, vol. 28(10), pp. 5632 5642. [138] Mosolov A.B. and Dinariev O.Yu., Problemy Prochnosti, 1988, No. 1, pp. 3 - 7. (Rus) [139] Witten T.A. and Sander L.M., Phys. Rev. A, 1983, vol. 27(9), pp. 5686 5697. [140] Meakin P. and Witten T.A., Phys. Rev. A, 1983, vol. 28(5), pp. 2985 - 2988. [141] Kozlov G.V., Shogenov V.N., and Mikitaev A.K., Inzhenerno-Fizicheski Zhurnal, 1998, vol. 71(6), pp. 1012 - 1015. (Rus) [142] Litt M.H., Koch P.J., and Tobolsky A.V., J. Macromol. Sci.-Phys., 1967, vol. B1(3), pp. 587 - 594. [143] Wunderlich B. Macromolecular Physics, Volume 1, New York – London, Academic Press, 1973, 623 p. [144] Burya A.I., Shogenov V.N., Kozlov G.V., and Arlamova N.T., Pridneprovsky Nauchny Vestnik, 1998, No. 83, pp. 9 - 16. (Rus) [145] Kozlov G.V., Beloshenko V.A., and Gazaev M.A., Ukrainski Fizicheski Zhurnal, 1996, vol. 41(11-12), pp. 1110 - 1113. (Rus) [146] Mashukov N.I., Gladyishev G.P., and Kozlov G.V., Vysokomol. Soedin., 1991, vol. A33(12), pp. 2538 - 2546. (Rus) [147] Afaunov V.V., Shogenov V.N., Mashukov N.I., and Kozlov G.V., Elektr. Zhurnal “Issledovano V Rossii”, 1999, 33. http://zhurnal mipt.rssi.ru/articles /1999/033.pdt. (Rus) [148] Graessley W.W. and Edwards S.F., Polymer, 1981, vol. 22(10), pp. 1329 1334. [149] Bessonov M.I., Koton M.M., Kudryavtsev V.V., and Laius L.A., Polyimides – The Class of Thermoresistant Polymers, 1983, Leningrad, Nauka, 302 p. (Rus) [150] Willbourn A.H., Polymer, 1976, vol. 17(10), pp. 965 - 976. [151] Mikitaev A.K., Kozlov G.V., and Shogenov V.N., Plast. Massy, 1983, No. 2, pp. 32 - 33. (Rus) [152] Koton M.M., Artemieva V.N., Kukarkina N.V., Kuznetsov Yu.P., and Dergacheva E.N., Vysokomol. Soedin., 1987, vol. B29(8), pp. 571 - 575. (Rus) [153] Kozlov G.V., Temiraev K.B., and Afaunova Z.I., The Effect of Intermolecular Interaction Energy On Structure Of Heterochain Polyesters, Manuscript deposited to VINITI RAS, Moscow, June 15, 1999, No. 1918V99. (Rus) [154] Kozlov G.V., Temiraev K.B., and Bedanokov A.Yu., Vestnik Adyigeiskogo Universiteta, 1999, No. 3, pp. 79 - 82. (Rus)

References

95

[155] Kalinichev E.L. and Sakovtseva M.B., Properties And Processing Of Thermoplasts, 1983, Leningrad, Khimia, 288 p. (Rus) [156] Vasnev V.A. and Kuchanov S.I., Uspekhi Khimii, 1973, vol. 42(12), pp. 2194 - 2220. (Rus) [157] Privalko V.P. and Lipatov Yu.S., Vysokomol. Soedin., 1971, vol. A13(12), pp. 2733 - 2738. (Rus) [158] Lee W.A. and Sewell J.H., J. Appl. Polymer Sci., 1968, vol. 12(6), pp. 1397 - 1409. [159] Meakin P., J. Chem. Phys., 1983, vol. 79(5), pp. 2426 - 2429. [160] Kozlov G.V., Burya A.I., Sviridenok A.I., and Zaikov G.E., Doklady NAI Belarusi, 2003, vol. 47 (in press). (Rus) [161] Jullien R. and Kolb M., J. Phys. A, 1984, vol. 17(12), pp. L639 - L643. [162] Kozlov G.V., Doklady Adyigeiskoi (Cherkesskoi) Mezhdunarodnoi AN, 2001, vol. 6(1), pp. 83 – 87. (Rus) [163] Kozlov G.V., Beloshenko V.A., Gazaev M.A., and Lipatov Yu.S., Vysokomol. Soedin., 1996, vol. B38(8), pp. 1423 - 1426. (Rus) [164] Kozlov G.V., Beloshenko V.A., and Varyukhin V.N., Prikladnaya Mekhanika I Tekhnicheskaya Fizika, 1996, vol. 37(3), pp. 115 - 119. (Rus) [165] Kozlov G.V., Beloshenko V.A., and Varyukhin V.N., Ukrainski Fizicheski Zhurnal, 1996, vol. 41(2), pp. 218 - 221. (Rus) [166] Kozlov G.V., Afaunova Z.I., and Zaikov G.E., Elektron. Zh. “Made In Russia”, 2003, Iss. 42, pp. 489 – 501; http: // Zhurnal.apl.relarn.ru/articles/ 2003/042.pdf. (Rus)

INDEX A access, 69 accuracy, 13, 70 Adams, 60 adhesion, 63, 64, 81 adjustment, 78, 80 agent, 12, 66 aggregates, 64 aggregation, 63, 64, 65, 66, 67, 81 aging, 7, 12, 52, 54 aging process, 12 alternative, 72, 85 alternatives, 7, 70 amine, 7, 52 amorphous, 1, 3, 4, 8, 14, 15, 16, 17, 19, 20, 24, 25, 26, 27, 28, 29, 33, 36, 37, 38, 41, 45, 47, 48, 49, 50, 51, 52, 53, 56, 59, 60, 64, 65, 67, 69, 70, 71, 73, 74, 77, 78, 79, 80, 84, 85, 86 amorphous polymer, 17, 19, 37, 38, 41, 47, 48, 50, 52, 53, 59, 60, 67, 74, 77, 78, 79, 80 amorphous polymers, 17, 19, 37, 38, 47, 48, 52, 59, 67 amorphous-crystalline polymers, 25, 29, 47, 49, 51, 56, 84, 85, 86 angstroms, 2, 14 anharmonicity, 41, 45 annealing, 59 annihilation, 35, 36

application, 6, 7, 11, 12, 13, 14, 27, 37, 41, 45, 47, 64, 70, 77, 78 aromatic, 74 assessment, 20, 29, 30, 42, 44, 48, 57, 70, 72, 82, 83 asymptotic, 23 atom, 35 atoms, 14, 35, 36 autocorrelation, 79 averaging, 24

B balanced state, 59 behavior, 3, 4, 6, 14, 25, 38, 53, 54, 55, 68, 85 binding, 5, 23, 56 block-copolymer, 74 blocks, 74, 75 bonds, 13, 26, 37, 78 Brownian motion, 63

C candidates, 71 capacity, 41 CEC, 7 chain molecules, 13 chain rigidity, 27, 31, 33, 76, 77

98

Index

chemical, 7, 10, 11, 14, 15, 16, 17, 38, 53, 55, 74, 82, 83 chemical cross-links, 17, 74 classes, 13, 26, 68 classical, 50, 52 classified, 51 cluster functionality, 36, 51 cluster model, 3, 4, 6, 10, 14, 17, 20, 33, 35, 37, 38, 41, 42, 45, 50, 52, 53, 56, 59, 60, 64, 65, 73, 77, 85 cluster network, 10, 17, 27, 45, 47, 48, 49, 53, 54, 55, 69, 82 cluster WS, 68 cluster-cluster, 65 clusters, 1, 2, 4, 7, 8, 10, 12, 17, 18, 20, 23, 24, 25, 26, 27, 28, 32, 35, 36, 48, 49, 50, 53, 54, 55, 56, 63, 65, 67, 69, 71, 77, 78, 81, 82, 83, 85 coherence, 49 cohesion, 74 coil, 21 collisions, 81 competition, 6 complement, 6, 12 components, 38, 41, 53, 55, 64, 78 composite, 72, 93 composites, 71, 72, 73 composition, 74 compressibility, 6 compression, 18 computer, 6, 63 Computer simulation, 64 concentration, 7, 51, 65, 70, 71, 72, 73, 74, 75, 76, 84, 85 concordance, 25 configuration, 4, 52, 54 conformational, 56 conformity, 15, 22, 27, 31, 33, 56, 57, 66, 70, 71, 73, 80, 84, 85 Congress, iv construction, 14 construction materials, 14 copolymer, 74, 75 copolymers, 75, 77

correlation, 5, 8, 9, 20, 21, 23, 26, 29, 31, 42, 48, 50, 51, 56, 66, 67, 68, 72, 76, 77, 78, 79, 82 correlations, 6, 27, 38, 59, 67, 69, 74, 76 covalent, 26, 78 covalent bond, 26, 78 critical behavior, 50 critical value, 36, 51, 82 cross-linked, 6, 16, 83 cross-linked polymer, 16, 83 cross-linked polymers, 16, 83 cross-linking, 7, 8, 12, 52, 81 crystal, 7 crystal growth, 7 crystalline, 15, 16, 17, 20, 25, 26, 27, 28, 29, 47, 49, 51, 56, 69, 71, 79, 84, 85, 86 crystallinity, 56, 74 crystallites, 7 crystals, 7 curing, 66

D Debye, 41, 42, 43, 44 decomposition, 1, 14, 36 deduction, 11 defects, 24, 68 deformability, 28 deformation, 17, 20, 24, 37, 80 degradation, 2, 29, 55 degradation process, 2 degree, 7, 56, 57, 74, 78 degrees of freedom, 36 delivery, 66 density, 2, 3, 42, 68, 69, 71, 72, 73, 74, 75, 76, 77, 78, 79, 84 destruction, 29 detachment, 35, 36, 37, 65 deviation, 22, 51, 60, 72, 80, 84 diaminodiphenylmethane, 25 dichloranhydride, 74 Differential Scanning Calorimetry, 93 diffraction, 22 diffusion, 63, 67, 81, 84

Index dimensionality, 2, 4, 6, 7, 10, 11, 12, 20, 21, 22, 23, 25, 29, 53, 54, 55, 56, 57, 64, 65, 68, 74, 79, 80, 81, 82, 83, 85 dislocations, 24 dispersion, 15, 76, 84 disposition, 75 dissipative structure, 14 dissipative structures, 14 dissociation, 37 distribution, 24, 27, 68 domains, 71, 72, 74, 76 double logarithmic coordinates, 3, 42, 43, 50, 51, 59, 68, 69

E elastic deformation, 17, 37 elasticity, 38, 45, 48, 49 elasticity modulus, 45, 48, 49 electronic, iv electrostatic, iv energy, 14, 17, 18, 19, 20, 21, 23, 29, 35, 36, 37, 42, 74, 75, 76, 77 energy density, 74, 75, 76, 77 energy transfer, 24 entanglement, 10, 14, 16, 17, 27, 31, 49, 69 entanglement network, 27, 31 entanglements, 14, 15, 16, 17, 27, 28, 29, 31, 47, 48, 70 EP, 4, 7, 8, 11, 12, 18, 22, 38, 51, 52, 53, 54, 55, 66, 81, 83 EP-1, 4, 7, 12, 18, 38, 51, 52, 53, 54, 55, 66 EP-2, 4, 7, 12, 18, 38, 51, 52, 53, 54, 55, 66, 81, 83 EP-3, 52, 53, 54, 55, 81, 83 epoxy, 7, 12, 24, 25, 38, 51, 52, 53, 54, 55, 82 epoxy polymer, 7, 24, 25, 38, 52, 53, 54, 55, 82 epoxy polymers, 7, 24, 25, 38, 52, 53, 54, 55, 82 equality, 28, 29, 47, 55, 69 equilibrium, 1, 2, 4, 6, 7, 12, 13, 14, 20, 22, 24, 52, 54, 55, 57, 59, 60, 61, 83, 85, 86 equilibrium state, 54, 55, 57, 59, 60, 61, 83, 85, 86

99

ester, 30 ethylene, 58 Euclidean, 2, 6, 22, 53, 65 Euclidean object, 6, 65 Euclidean objects, 6 Euclidean space, 2, 53 evolution, 14, 17 expert, iv extrapolation, 38, 55, 76 extrusion, 22

F February, 92 film, 22 films, 22 fixation, 28, 32, 33 flexibility, 16, 21, 27, 75 flow, 17, 18, 20, 23, 24, 38 fluctuation free volume, 35, 36, 37, 38, 65 fluctuations, 60 forecasting, 6, 74 fractal, 1, 2, 4, 5, 6, 10, 11, 12, 13, 21, 22, 23, 24, 25, 27, 29, 32, 33, 53, 54, 55, 56, 57, 58, 64, 65, 66, 68, 69, 70, 72, 73, 79, 80, 81, 82, 83, 85 fractal analysis, 1, 4, 6, 12, 13, 27, 32, 33 fractal dimension, 2, 5, 7, 10, 11, 12, 21, 22, 24, 25, 29, 53, 54, 55, 56, 57, 58, 65, 66, 68, 70, 72, 73, 79, 80, 81, 82, 83 fractal dimensionality, 2, 7, 10, 11, 12, 21, 22, 24, 25, 29, 53, 54, 55, 56, 57, 65, 68, 79, 80, 81, 82, 83 fractal objects, 1 fractal properties, 2, 69 fractal structure, 1, 6, 7 fractality, 1, 2, 3, 4, 5, 6, 12, 23, 52 fractals, 4, 6, 24 fracture, 1, 29 fragmentation, 24 free volume, 35, 36, 37, 38, 57, 58, 65, 77 freedom, 36 freezing, 63, 70 frequency, 7, 8, 12, 17, 27, 31, 33, 42, 43, 45, 48, 69, 71, 72, 74, 81, 82, 83, 84

100

Index

fulfillment, 1, 43 future, 12, 63

G gel, 6, 8, 11, 12, 23, 63, 65 gel formation, 7, 8, 11, 12, 23, 65 generation, 35, 37, 67 Gibbs, 1, 2, 6, 60, 93 glass, 22, 35, 36, 38, 50, 52, 58, 60, 74, 75, 76 glass transition, 35, 36, 38, 50, 52, 58, 60, 74, 75, 76 glass transition temperature, 36, 38, 50, 74, 75, 76 glasses, 35, 37, 41 glassy polymers, 6, 12, 36, 37, 41, 51, 67, 70 glassy state, 7, 11, 12, 27, 28, 32, 33, 41, 49, 56, 82 graph, 50 groups, 14 growth, 7, 55, 66, 70, 77, 78, 82, 83

H Hausdorff dimension, 6 HDPE, 36, 48, 49, 57, 69, 70, 71, 72, 73, 77 heat, 36, 41, 42, 54, 60 heat aging, 54 heat capacity, 41 homogeneous, 4, 6 hypothesis, 64

I identification, 69, 75, 84 independence, 43 indices, 4, 7, 52, 53, 54, 55, 65, 66 inequality, 50 infinite, 47, 50, 63 injection, 71 injury, iv intensity, 75, 78 interaction, 36, 37, 41, 42, 54, 70, 74, 78, 83, 85, 94

interactions, 52, 54, 64, 75 interdependence, 76 intermolecular, 37, 74, 75, 77, 78 intermolecular interaction, 74, 75, 78 intermolecular interactions, 75 interphase, 71 interpretation, 15, 17, 18, 28, 53, 70 interval, 8, 33, 43, 48, 79 isotropic, 14

J Japan, 90

K kinetic equations, 7

L lattice, 41, 79 laws, 50 light, 17 limitations, 28 linear, 2, 3, 14, 15, 16, 18, 22, 24, 25, 26, 31, 37, 38, 43, 44, 47, 48, 50, 51, 59, 60, 66, 68, 69, 76, 79, 82 linear defects, 24 linear dependence, 26, 76 linear function, 38 linear polymers, 14, 15, 22, 38 links, 17, 74 liquids, 35, 41 literature, 15, 23, 27, 31, 48, 84 local order, 1, 4, 5, 6, 7, 10, 12, 14, 23, 24, 25, 36, 41, 51, 54, 55, 57, 59, 65, 66, 69, 70, 71, 73, 77, 78, 79, 81, 83, 85 localization, 17, 18, 19, 20, 21 logarithmic coordinates, 3, 42, 43, 50, 51, 59, 68, 69 London, 94 low temperatures, 48

Index

M macromolecular coil, 21 macromolecular entanglements, 27, 47, 48 macromolecules, 8, 14, 33, 47, 48, 71, 82 magnetic, iv, 71 magnetic field, 71 magnetic fields, 71 mass, 42 mathematical, 4, 47 Matrices, 89 matrix, 17, 19, 22, 35, 37, 38, 53, 54, 55, 57, 66, 69, 77, 78, 85, 86 maximal local, 10 mechanical, iv, 14, 17, 20, 29, 47, 49 mechanical energy, 29 mechanical properties, 14, 47, 49 mechanical stress, 17 mechanical stresses, 17 media, 23 melt, 71 mercury, 41 metals, 24 methyl methacrylate, 30, 58 microcavity, 35, 36, 37, 65 migration, 35 mobility, 28, 29, 32, 52, 54, 56, 82 models, 4, 27, 28, 47, 52, 64, 65, 70, 74, 84, 85 modulus, 17, 18, 21, 45, 48, 49 molecular mass, 11, 48 molecular mobility, 28, 29, 32, 52, 54, 56, 82 molecular structure, 13 molecules, 7, 13, 41 Monte-Carlo, 63 Moscow, 87, 88, 89, 90, 91, 92, 94 motion, 36, 63, 78 multifractal, 6 multiplication, 66

N natural, 13, 47, 52, 71

101

network, 6, 10, 11, 12, 14, 17, 23, 27, 31, 33, 38, 45, 47, 48, 49, 53, 54, 55, 65, 66, 69, 71, 72, 82, 84 networks, 7, 22, 38, 47 New York, iii, iv, 87, 88, 91, 93, 94 nucleation, 7, 8, 9

O oligomer, 12, 66 organization, 6, 24, 25, 26 orientation, 41, 45, 52, 54, 55, 58, 81 oriented polymers, 20 oscillations, 41, 42

P PAr, 1, 2, 22, 36, 37, 38, 42, 43, 44, 45, 48, 49, 50, 51, 67, 68, 70, 71, 74 parameter, 6, 13, 18, 19, 21, 23, 27, 28, 29, 41, 42, 44, 48, 51, 52, 53, 55, 56, 65, 67, 68, 71, 72, 79, 80, 84, 85 particle-cluster, 63 particles, 63, 64, 65, 66, 69, 71, 72, 77, 78, 79, 81, 83, 84, 85, 86 PC, 1, 2, 22, 32, 33, 36, 37, 38, 48, 49, 50, 51, 57, 59, 60, 67, 68, 69, 70, 71, 77, 79, 80, 81 percolation, 4, 47, 50, 51, 52, 53, 54, 55, 59 percolation cluster, 4, 50, 51, 52, 53, 55 percolation clusters, 4, 55 percolation theory, 4, 47, 51 periodicity, 1, 3 phenolphthalein, 74 physical aging, 7, 12 physicochemistry, 1 physics, 1, 12, 13, 14, 41, 64 plasticity, 38 PMMA, 50, 51, 57, 60, 61 Poisson, 5, 32 polyamide, 75 polyarylate, 22, 74 polyesters, 74 polyethylene, 22, 84 polyethylenes, 48, 49

102

Index

polymer, 1, 2, 3, 4, 5, 6, 8, 10, 11, 12, 13, 14, 15, 16, 17, 19, 20, 21, 22, 23, 25, 26, 27, 28, 29, 32, 33, 36, 38, 41, 45, 47, 49, 51, 52, 53, 54, 55, 56, 57, 58, 59, 60, 63, 64, 65, 66, 69, 70, 71, 73, 74, 76, 77, 78, 79, 80, 81, 82, 83, 84, 85 polymer amorphous state, 3, 4, 8, 14, 25, 33, 38, 45, 52, 64, 69, 70, 73, 85 polymer amorphous state structure, 4, 25, 33, 38, 45, 64, 69, 70, 71, 73 polymer density, 69, 78 polymer network structures, 65 polymer networks, 7, 11, 12, 14, 15, 16, 17, 20, 25, 26, 27, 28, 38, 51, 55, 69, 81 polymer properties, 13, 27, 74, 77 polymer structure, 2, 3, 4, 5, 6, 10, 12, 21, 22, 25, 39, 50, 52, 53, 54, 55, 56, 57, 58, 59, 60, 71, 74, 77, 78, 83, 85 polymers, 1, 4, 6, 7, 11, 12, 13, 14, 15, 16, 17, 19, 20, 22, 23, 24, 25, 26, 27, 28, 29, 30, 31, 35, 36, 37, 38, 41, 43, 47, 48, 49, 51, 52, 53, 54, 55, 56, 57, 59, 60, 67, 68, 69, 70, 71, 74, 75, 82, 83, 84, 85, 86 polyvinylchloride, 75 potential energy, 42 power, 68, 70 preparation, iv, 22 pressure, 7, 42 probability, 24, 25, 26, 27, 47, 49, 50, 63, 79 probability distribution, 24 process, 18, 24, 52, 63, 64, 84 propagation, 63, 65, 66, 69, 71, 81, 84, 85 propane, 74 properties, 7, 11, 12, 13, 22, 23, 28, 35, 38, 47, 66, 71, 72, 75 property, iv, 17, 23 proportionality, 15, 36, 82 PSP, 36 PVC, 36

Q quantitative estimation, 85 quasi-equilibrium, 52, 54, 55, 57, 59, 60, 61, 83, 85, 86

quasi-equilibrium state, 54, 55, 57, 59, 60, 61, 83, 85, 86

R radius, 68, 70, 79, 85 random, 24, 35, 36, 37, 63 random walk, 63 range, 3, 6, 8, 14, 27, 32, 50, 52, 69, 72 RAS, 89, 90, 92, 94 redistribution, 78 regular, 75 regulation, 55 relaxation, 84 rheology, 27 rigidity, 6, 13, 27, 31, 33, 47, 49, 56, 75, 76, 77 rubber, 27, 55 rubbers, 29, 30 rubbery state, 29, 32, 82 Russia, 89, 93, 95 Russian, 88, 92

S sample, 22, 47, 65 scaling, 50, 65, 66, 79 science, 1 seeding, 70, 71, 72, 73, 84 Self, 53 self-assembly, 1 self-organization, 6 self-similarity, 8, 12, 14, 15, 16, 18, 20, 21, 29 series, 28, 37, 44, 52, 53, 55, 68, 70, 82, 84 services, iv shape, 2, 75 shear, 6, 17, 18 short-range, 37 sign, 69 signs, 69 similarity, 8, 12, 14, 15, 16, 18, 20, 21, 24, 29, 53 simulation, 6, 52, 63, 64, 70, 77, 78, 81, 83, 84

Index simulations, 70 solid phase, 1, 36 solid polymers, 4, 35, 49 solution, 13, 22 spatial, 14, 17, 18, 20 spectrum, 6 stability, 17 stages, 24, 69 steric, 64, 81, 83 strain, 83, 84 strength, 47 stress, 17, 80, 84 structural changes, 17, 72 structural characteristics, 7, 20, 52 structure formation, 1, 6, 47, 71, 74, 77 substitution, 5, 57 sulfur, 25 supermolecular structure, 6, 11, 21 superposition, 10 suppression, 54 symmetry, 6 systematic, 19 systems, 6, 11, 13, 25, 26, 64, 66

T temperature, 5, 28, 32, 35, 36, 37, 38, 41, 42, 43, 44, 45, 47, 48, 49, 50, 51, 57, 58, 59, 60, 67, 68, 69, 70, 74, 75, 76, 80, 81 temperature dependence, 5, 32, 35, 36, 41, 42, 45, 58 tensile, 22 theoretical, 1, 22, 30, 31, 50, 51, 58, 60, 70, 80, 82, 83 theory, 4, 9, 22, 35, 37, 41, 47, 51, 58, 60 thermal, 52, 53, 55, 59, 60 thermal cluster, 52, 53, 55, 59, 60 thermodynamic, 1, 6, 57, 58, 59, 60 thermodynamic equilibrium, 57, 60 thermodynamics, 14, 20 three-dimensional, 10, 22, 23, 50, 51, 53, 83 three-dimensional space, 10, 22, 83 threshold, 4, 47, 50 time, 3, 7, 8, 22, 66, 69 topological, 13, 28, 32, 33, 55

103

topology, 15, 27 transfer, 24 transformation, 24 transition, 1, 2, 6, 15, 28, 32, 35, 36, 52, 57, 58, 60, 63, 65, 69, 70, 74, 76, 82 transition temperature, 74 translational, 6 turbulence, 23, 24 turbulent, 23 turbulent flows, 23

U uncertainty, 13 uniform, 18 universality, 53, 64, 65, 66, 69

V valence, 13, 31, 32, 56, 57 values, 11, 15, 20, 22, 23, 27, 30, 31, 32, 43, 45, 48, 51, 52, 53, 55, 56, 66, 69, 72, 75, 78, 80, 81, 83, 84, 85 variable, 38 variables, 42 variation, 1, 4, 15, 23, 37, 39, 42, 52, 64, 68, 72, 78, 79 Viscoelastic, 91 viscosity, 23, 35, 36

W walking, 63 water, 41 WS model, 64, 65, 70, 72, 73, 74, 77, 78, 80, 84, 85

X X-ray, 22 X-ray diffraction, 22

104

Index

Y

yield, 17, 80

CLUSTER MODEL INTERRELATION WITH MODERN PHYSICAL CONCEPTS

G. V. KOZLOV AND

G. E. ZAIKOV

Nova Science Publishers, Inc. New York

Copyright © 2009 by Nova Science Publishers, Inc.

All rights reserved. No part of this book may be reproduced, stored in a retrieval system or transmitted in any form or by any means: electronic, electrostatic, magnetic, tape, mechanical photocopying, recording or otherwise without the written permission of the Publisher. For permission to use material from this book please contact us: Telephone 631-231-7269; Fax 631-231-8175 Web Site: http://www.novapublishers.com NOTICE TO THE READER The Publisher has taken reasonable care in the preparation of this book, but makes no expressed or implied warranty of any kind and assumes no responsibility for any errors or omissions. No liability is assumed for incidental or consequential damages in connection with or arising out of information contained in this book. The Publisher shall not be liable for any special, consequential, or exemplary damages resulting, in whole or in part, from the readers’ use of, or reliance upon, this material. Independent verification should be sought for any data, advice or recommendations contained in this book. In addition, no responsibility is assumed by the publisher for any injury and/or damage to persons or property arising from any methods, products, instructions, ideas or otherwise contained in this publication. This publication is designed to provide accurate and authoritative information with regard to the subject matter covered herein. It is sold with the clear understanding that the Publisher is not engaged in rendering legal or any other professional services. If legal or any other expert assistance is required, the services of a competent person should be sought. FROM A DECLARATION OF PARTICIPANTS JOINTLY ADOPTED BY A COMMITTEE OF THE AMERICAN BAR ASSOCIATION AND A COMMITTEE OF PUBLISHERS. LIBRARY OF CONGRESS CATALOGING-IN-PUBLICATION DATA Kozlov, G. V. Cluster model interrelation with modern physical concepts / G.V. Kozlov & G.E. Zaikov. p. cm. Includes index. ISBN 978-1-60741-684-5 (E-Book) 1. Polymers--Structure. I. Zaikov, Gennadii Efremovich. II. Title. QC173.4.P65K69 2009 547'.7--dc22 2008047189

Published by Nova Science Publishers, Inc. + New York

CONTENTS

Chapter 1

Fractality of the Polymer Structure and the Cluster Model 1

Chapter 2

Clusters as Dissipative Structures

13

Chapter 3

Cluster and Fluctuation Free Volume Models

35

Chapter 4

The Cluster Model and the Anharmonicity Concept

41

Chapter 5

Cluster Structure as a Percolation System

47

Chapter 6

Cluster model as the Model of Irreversible Aggregation

63

References

87

Index

97

Chapter 1

FRACTALITY OF THE POLYMER STRUCTURE AND THE CLUSTER MODEL During recent 20 years methods of fractal analysis were widely spread in theoretical physics [1] and general material science [2], in physicochemistry of polymers [3 – 8], in particular. This tendency is explained by a broad spreading of fractal objects in the nature. There are two basic factors determining interrelation between the local order and fractal origin of the polymer solid phase: thermodynamic non-equilibrium and dimensional periodicity of the structure. A simple relation between the non-

~ im

equilibrium index, which is the Gibbs function variation, ΔG , at polymer selfassembly (the cluster structure formation), and a relative part of clusters, ϕcl, as follows:

~ ΔG im ~ ϕcl.

(1)

Figure 1 shows graphical presentation of this relation for amorphous glassy

~ im

= 0 [10, 11], the relation (1) PC and PAr polymers. Since at Т = Тg(Tm) ΔG indicates necessary complete decomposition of the cluster system (ϕcl = 0) at these temperatures or transition to thermodynamically equilibrium structure. As for interrelation between fractality and thermodynamic non-equilibrium, Hornbogen [12] has indicated that exactly thermodynamically non-equilibrium processes form fractal structures. The classic example of this regularity fulfillment is represented by fracture surfaces of solids: many experimental researches have indicated their fractality independently of thermodynamic conditions of the solid

2

G. V. Kozlov and G. E. Zaikov

itself [12]. This is stipulated by thermodynamic non-equilibrium of the degradation process [13]. This very fact does also determine experimentally proved fractality of the polymer structure [14 – 16]. Similar to every real (physical) fractal, fractal properties of the polymer structure are limited by definite linear scales. For example, in works [14, 17] these scales are limited by several angstroms (the lower limit) to several ten angstroms (the upper limit). The lower limit is associated with the finite size of structural elements and the upper limit with irregular approaching the limit of the fractal dimensionality of the structure, df [18]. The above-mentioned scales are in good keeping with the border dimensions of the cluster structure: the lower with the static segment length, lst, and the upper with the distance between clusters, Rcl [19]. In these scales, fractality of the polymer structure assumes dependence of density, ρ, on scale, L, of the following shape (Figure 2) [1]: d f −d

ρ~L

,

(2)

where d is dimensionality of the Euclidean space, to which the fractal is inserted.

Figure 1. Dependence of the relative cluster part, ϕcl, on the absolute value of specific Gibbs function for non-equilibrium phase transition

ΔG im

for PC (1) and PAr (2) [8]

Fractality of the Polymer Structure and the Cluster Model

3

Figure 2. Dependence of density ρ on linear scale L for a solid in double logarithmic coordinates. Fractal behavior is observed in the Lmin-Lmax range [18]

Figure 3. Schematic presentation of the cluster structure of the polymer amorphous state [5]

Figure 3 presents schematic image of the cluster structure of the polymer amorphous state. Clearly within the borders of the above-mentioned dimensional periodicity data in Figures 2 and 3 correspond to one another, i.e. the cluster model suggests ρ decrease with removing from the cluster center. At the same time, the Flory “felt” model [20] does not fit this criterion (for it ρ = const). Since fractality of the polymer structure was proved in experiments [14 – 16], it is

4

G. V. Kozlov and G. E. Zaikov

obvious that the cluster model conforms to the structure of real solid polymers, whereas the “felt” model does not correspond to it. Obviously the reverse dependence for final ρ is also true: ρ variation in definite limits necessarily suggests structure periodicity. However, one should remember that fractal analysis gives just general mathematical description of polymers, i.e. it does not identify structural units (elements), from which any real polymer is formed. Physical description of thermodynamically non-equilibrium polymer structure in the framework of the local order ideas gives the cluster model of the polymer amorphous state structure that quantitatively identify its elements. Since these models consider the polymer structure somewhat from two sides, they are excellent completing one another [21]. It is common knowledge [22] that structures displaying fractal behavior on small length scale and being homogeneous on large length scale are named homogeneous fractals. These fractals are percolation clusters at the percolation threshold [1]. As shown below, the cluster structure represents the percolation system and, due to the above-said, the homogeneous fractal. To put it differently, the presence of the local order in the condensed phase of polymers determines fractality of their structures. Fractal dimensionality, df, of the percolation system can be expressed by the equation as follows [22]:

df =d−

βp νp

,

(3)

where βp and νp are critical indices in the percolation theory. Table 1. Percolation cluster characteristics [5] Parameter

βp νp βp/νp df

Experimentally determined indices EP-1 EP-2 0.54 0.58 1.20 1.15 0.45 0.504 2.55 2.50

Theoretical “configuration” indices [22] 0.40 0.88 0.455 2.545

Fractality of the Polymer Structure and the Cluster Model

5

As a consequence, the condition βp ≠ 0 that follows from Table 1 does also determine fractality of the polymer structure. Obviously this condition and, consequently, fractality of the polymer structure determined temperature dependence of ϕcl, e.g. thermofluctuation origin of the local order. To put it differently, the structure fractality and the local order “frozen” below Tg (ϕcl = const) represent mutually exclusive notions. The above-considered statements allow binding the fractal dimension, df, and local order characteristics (ϕcl or υcl) by an analytical relation. The following equation binds df value to the Poisson coefficient ν [18]: df = (d – 1)(1 + ν);

(4)

in its turn, ν value is associated with νcl. Equation (4) allows obtaining of the interconnection between df and ϕcl or νcl as follows:

⎛ ϕ df = 1.5(d – 1) – 3.22(d – 1)×10 ⎜⎜ cl ⎝ SC ∞ -10

12

⎞ ⎟⎟ ⎠

,

(5)

or df = 1.5(d – 1) – 3.22(d – 1)×10-10(l0νcl)1/2.

(6)

These expressions, most frequently used for the case d = 3, are reduced to the simple form as follows [4]:

⎛ ϕ df = 3 – 6.44×10 ⎜⎜ cl ⎝ SC ∞ -10

12

⎞ ⎟⎟ ⎠

,

(7)

or df = 3 – 6.44×10-10(l0νcl)1/2.

(8)

Turning back to correlation (5.1), note that its substitution into equation (5) or (7) allows obtaining of the following expression (for d = 3) [9]:

6

G. V. Kozlov and G. E. Zaikov

(

~ ΔG im ~ C ∞ S 3 − d f

)2 .

(9) ~ im

The Gibbs specific function of supermolecular structure formation, ΔG , is given for non-equilibrium “overcooled liquid – solid” phase transition [11]. As

~ im

follows from the relation (9), ΔG = 0 at df = 3, e.g. at df = d and transition to the Euclidean behavior. To put it differently, fractal structures are induced by nonequilibrium processes only, as it has been assumed before [12]. One more noteworthy analogy can be traced between glassy polymers and homogeneous fractals. It is known [23] that the mentioned polymers do not fit the Prigozhine-Defye criterion that means that to be described they require more than one order parameter. Concerning Euclidean objects (spaces), they possess translational symmetry and, consequently, require one parameter to be described, namely, the Euclidean dimensionality d [24]. Fractal objects (spaces) possess dilatation symmetry and, therefore, require three dimensionalities for characterization: the Hausdorff df, spectral ds, and d. Even if in the latter case d is assumed constant and equal 3, correct description of the fractal requires, at least, two dimensionalities: df and ds. Even this qualitative comparison proves fractality of the glassy polymer structure. General ideas for the benefit of the local order existence in polymers were considered based on the Ramsey theorem [18, 21]. By analogy, it can be proved that any structure consisting of N elements (N > BN(i)) represents an aggregate of a finite number k ≤ j of self-similar structures enclosed in one another, the Hausdorff dimensionality of which, in general, can be different. This means that any structure consisting of quite large number of elements, independently of its physical origin, represents a multifractal (fractal, in particular) and is characterized by a spectrum of Regnier dimensionalities dq, q = 0, 1, 2, … [18]. It has been shown [25] that the tendency of condensed systems to self-organization in the scale-invariant multifractal forms originate from the fundamental thermodynamic principles of open systems, and dq is determined by the competition of short- and long-range interatomic correlations, which determine volumetric compressibility and shear rigidity of solids, respectively. As mentioned above, the cluster model and the fractal analysis are complement approaches and their combined application discloses new possibilities for simulation of the polymer structure. This point is considered on the example of forecasting parameters of polymer network cluster structure [26]. It is known [27 – 29] that computer simulation of the processes has induced a conclusion that in the gel-formation point cross-linked backbones of these

Fractality of the Polymer Structure and the Cluster Model

7

polymers represent fractal structures, cross-linking frequency increase inducing an increase of the fractal dimensionality of such backbone. However, from positions of practice the cross-linking frequency is not suitable enough, though at the present time polymer networks are preferably characterized using the value νnw [30]. Nevertheless, it has been shown [31] that at constant νnw for one and the same polymer network, different properties (for example, different Tg) can be obtained. This is explained by the change of supermolecular (cluster) structure of polymer network during physical aging, namely, by increase of the local order degree [31]. In its turn, the local order degree determines df value (equations (5) – (8)). Thus there occurs a possibility of forecasting structural characteristics (and as a consequence properties) of polymer networks in the glassy state basing on chemical cross-linking degree in the gel formation point. One of possible alternatives of solving this problem was discussed [32] on the example of typical representatives of the polymer network class – epoxy polymers of amine (EP-1) and anhydride (EP-2) cross-linking type, as well as their homologues solidified under pressure of 200 MPa (EP-1-200 and EP-2-200). The relation between νnw and df of studied EPs was deduced on the basis of the model suggested in the work [33]. The essence of this model is as follows. Competing processes of crystal growth and nucleation were described in the framework of two kinetic equations [33]: dR/dt = k1cm,

(10)

dN/dt = k2cp,

(11)

where R is the crystal dimension; t is the current time; k1 and k2 are equilibrium constants; N is the number of crystals; c is the concentration of molecules at the surface; m and p are indices. The application of equations (10) and (11) to description of the local order zones (clusters) nucleation and growth in EP is based on the fact that clusters in itself represent analogues of crystallites with extended chains (CEC) [34]. The characteristic size of cluster is accepted equal the length of segments in it, i.e. the statistic segment length lst. Similar to [33], m =1, because cluster growth represents addition of a single segment with the length lst [35]; therefore, p > 1, because cluster nucleation requires occurrence of two or more segments in the nucleation point. However, application of the equation (10) to a single separate EP requires sufficient modification. Obviously, if R = lst is accepted, the equation (10) becomes meaningless, because for every studied EP lst = const and dlst/dt = 0. The latter means that clusters has not the ability to grow. That is why, denoting the

8

G. V. Kozlov and G. E. Zaikov

number of segments in a single cluster by nseg, the equation (10) will be presented as follows [32]:

dn seg dt

= k1c .

(12)

The border value of nseg is limited by nucleation of new clusters of the thermofluctuation origin. That is why [33]:

l st =

(dnseg dt ) . (dN

dt )

(13)

Obviously the part of segments of macromolecules, c, capable of forming clusters must be decreased with time during the cluster formation and, taking into account the condition lst = const for every EP, nseg must also be decreased. This fact explains the presence of unstable (possessing low nseg) clusters in the structure of the polymer amorphous state [36, 37]. This also explains selfsimilarity of the cluster structure in the scale range of its existence. Note back again the important circumstance that the system of equations (10) and (11) can be applied to the totality of studied EPs, and the system of equations (11) and (12) is applicable to any separate EP of the totality [32]. For the totality of studied EPs, one can write down the following equations [33]:

N (l st ) = (dN cl dt )t gel ,

(14)

and

l st ~

(dl st dt ) , (dN cl dt )

(15)

where Ncl is the number of clusters; tgel is the time interval of the gel formation. The relation (15) forecasts C∞ decrease with cross-linking frequency, νnw, increase and consequent lst decline. This intensifies nucleation of new clusters, i.e. Ncl increase. Assuming R = lst, m = 1 and dividing equation (10) by (11), the following correlation is obtained:

Fractality of the Polymer Structure and the Cluster Model

l st ~

dl st dt c ~ p = c1− p , dN cl dt c

9

(16)

because k1 and k2 are constants. The equation (14) combined with the expression (11) under the conditions tgel = const, k2 = const and, as before, N = Ncl, gives the following correlation: Ncl(lst) = k2tgelcp,

(17)

or with regard to k2tgel = const: Ncl(lst) ~ cp.

(18)

Equations (10) and (11) allow determination of c as follows: −1 /( p −1)

c ~ l st

,

(19)

and 1/ p

c ~ N cl .

(20)

Making equal the right parts of equations (19) and (20), it is obtained that [32]: 1/ p −1 /( p −1) N cl ~ l st

(21)

or − p /( p −1)

Ncl(lst) ~ l st

.

(22)

It has been indicated [33] that the classic nucleation theory requires р ≤ 2 and, consequently, the condition occurs as follows:

p ≥ 2. p −1

(23)

10

G. V. Kozlov and G. E. Zaikov

Moreover, there is one more restriction that states that the volume of clusters must not exceed total volume of the polymer, wherefrom one more condition follows [33]:

p ≤ 3. p −1

(24)

Thus index in the relation (22) falls within the same limits as the fractal dimensionality of the object in the three-dimensional space [34]. The accurate interrelation between p/(p – 1) and df can be obtained from comparison of the expression (22) with the ones deduced in the work [39]: −d f

Ncl(lst) ~ l st

,

(25)

therefore [32]: p/(p – 1) = df.

(26)

The value Ncl can be presented as follows [34]:

N cl =

2ν Vcl = cl . n seg F

(27)

One more important circumstance shall be mentioned. The comparison of equations (11) and (25) indicates that the maximal rate of the cluster formation is reached at p =2 or df = 2.To put it differently, it is assumed that the minimal fractal dimensionality of the polymer structure is corresponded to the maximal local order. In the framework of the cluster model [34] polymer network can be considered as a superposition of two carcasses – chemical cross-link network and physical entanglement cluster network possessing frequencies νnw and νcl, respectively. As each of these carcasses is accepted as the ideal structure (i.e. the effect of end chains is neglected), one can write down as follows [40]:

M ceff =

Mc f , 2

(28)

Fractality of the Polymer Structure and the Cluster Model

11

eff

where M c is the effective molecular mass of a chain part between chemical cross-link points; Mc is the value of the latter; f is the functionality of chemical cross-link point. With regard to equations (27) and (28), the relation (25) can be reduced to the following form [32]:

2ν nw −d ~ l st f . f

(29)

An equation linking parameters С∞ and df for d = 3 was deduced [41]. Full deduction and complete form of this equation will be given in the following Section:

⎛ df 4⎞ + ⎟. C∞ = ⎜ ⎜33−d f 3 ⎟⎠ ⎝

(

)

(30)

Combined equations (29) and (30) give the following expression [32]:

d l0 f

⎛ df 4⎞ ⎜ + ⎟ ⎜ 3(3 − d f ) 3 ⎟ ⎝ ⎠

df

= 3.75 × 10 28

f

ν nw

,

(31)

where the empirical numerical coefficient in the right part of the equation is obtained by equaling df values, calculated from equations (4) and (31), at νnw = 1027 m−3 [32]. Figure 4 compares df values, calculated by equations (4) and (31) as the function of νnw, for studied EPs under the conditions l0 = 1.25 Å [5] and f = 4. Clearly good correspondence of two selections of the fractal dimensionalities was obtained. This means that the increase of the carcass fractal dimensionality before the gel formation point [29] induces a decrease of the fractal dimensionality df of the supermolecular structure of polymer network in the glassy state. It should be noted also that knowledge of df allows the forecast of EP properties [35, 42]. Thus varying Kst or terminating the reaction at a definite stage, one can obtain polymers with required properties. However, from positions of practical significance, application of stoichiometric values Kst = 1.0 is more preferable. It gives the most stable systems [18], including polymer networks [35]. In this case, properties of

12

G. V. Kozlov and G. E. Zaikov

the final product can be varied by changing functionality of the cross-linking agent, f, or molecular characteristics of epoxy oligomer. Thus fractal analysis application allowed clearing up an interrelation between polymer network characteristics before the gel formation point (or at it) and in the glassy state. Note that this can be made for just synthesized polymer only. Further on, df will vary due to physical aging processes, unavoidable due to thermodynamically non-equilibrium origin of the polymer glassy state. Nevertheless, the methodology suggested allows forecast of properties of glassy polymer networks already at the cross-linking stage. Moreover, the model considered forecasts qualitatively previously expected effects, namely, the existence of unstable clusters [36, 37], self-similarity of the cluster structure [5, 34] and df decrease with the local ordering increase. For a brief resume, it should be noted that in the case of glassy polymers, notions of the local order and fractality are tightly connected basing on the fundamental ideas of physics. This interrelation is expressed by simple analytical equations (5) - (8). It is also shown that combined application of these complement concepts allows significant broadening and improvement of the analytical description of the polymer structure and properties. The mentioned combination will be multiply used in the future discussion.

Figure 4. Dependence of fractal dimensionality, df, of EP structure on cross-linking frequency, νnw, calculated as follows: by equation (4) for EP-1 (1), EP-2 (2), EP-1-200 (3) and EP-2-200 (4), and by equation (5.31) for all EPs [32]

Chapter 2

CLUSTERS AS DISSIPATIVE STRUCTURES Obtaining of relations between structure and properties of polymers was always the foreground task of the polymer physics. However, solution of this problem is significantly complicated by the presence of a multilevel structure in polymers – molecular, topological, supermolecular (super-segmental), etc. That is why a polymer structural model is required, which would allow association of structural parameters of the mentioned levels by quantitative relations. Obviously such relations should better be deduced on the basis of fundamental physical principles. Recent rapid development of synergism of non-equilibrium systems [43, 44] and fractal analysis allows application of these fundamental concepts to solution of the tasks mentioned, because a solid-phase polymer represents thermodynamically highly non-equilibrium system. The basic feature differing polymers from other classes of solids is their structure, composed of long chain molecules. That is why the assumption seems natural that the structural hierarchy of polymers must be based on their molecular structure. Recently, the characteristic relation С∞ [45 - 47] is more and more frequently used as the molecular parameter for description of polymer properties, hence substituting, for example, such characteristics as relation а/δ (where a in the chain “thickness” and δ is its rigidity [48]). To the point of view of Boyer and Miller [48], this is stipulated by higher uncertainty of δ compared with С∞, because the former depends upon valence angles of bonds in the macromolecule and the latter on the length of these bonds. Usually, bond lengths are determined with significantly higher accuracy than the valence angles. Not contradicting to the rightfulness of such conclusion, nevertheless, the authors assume that the reasons for broad application of С∞ parameter are much deeper and fundamental; one of the objectives of the current Section is demonstration of declared

14

G. V. Kozlov and G. E. Zaikov

fundamentality of С∞ in the framework of thermodynamics of non-equilibrium processes [43, 44]. The behavior of a deformable solid subject to mechanical impact is determined by formation (decomposition) and evolution of dissipative structures (DS) providing for the optimal mode of supplied energy dissipation [18, 25, 49]. This general statement is also true for polymers. Broad application of polymers as construction materials requires the detail study of their mechanical properties which is impossible without understanding of fundamental processes, on which their behavior under load is based. At present, it is known well that polymers possess a local order that exists in them in the form of dissipative structures (DS) [50 – 52]. However, direct application of fundamental principles of thermodynamics and statistical physics of non-equilibrium processes to the study of behavior of any class of materials is often quite difficult or even impossible without knowing particular quantitative model of the structure of this material. For such model, the cluster model of the polymer amorphous state will be used below. As shown [18, 49], the feature of DS, also formed in polymers [50 – 52], is existence of a universal hierarchy of spatial scales (structural levels), which is reflected in the hierarchy of linear sizes of the structure. For example, even in elastically isotropic bodies, at least, three independent length scales do exist: lp, lε, and le, bound with one another by the following relations [49]: lp = aM; lε = aMΛ0; le = lεΛ1,

(32)

where aM is the linear size; Λ0 and Λ1 are self-similarity coefficients. At personification of these length scales related to polymers the atomic level must be neglected, because polymer represents a solid consisting of long chain macromolecules which, in turn, are composed of various groups of atoms. That is why the minimum scale, aM, in equation (32) for polymers must be the length of the macromolecule backbone, l0, varied within the range of several angstroms [45, 53]. Then the next higher structural (segmental) level will be determined by the statistical segment length, lst. As a consequence, for this structural level, the selfsimilarity coefficient Λ0 = С∞ under the condition lp = l0 [5, 41, 54, 55]. Topological level is the consequent structural level in polymers. Its parameters are determined by characteristics of macromolecular entanglement (“hooking”) network in linear polymers and by parameters of chemical cross-link network in polymer networks. For this level, the distance between entanglements or chemical cross-link points, Rnw, is the typical linear scale, le.

Clusters as Dissipative Structures

15

As a consequence, it follows from the above discussion that if for the consequent structural levels the self-similarity coefficient value (Λ0 = С∞) is preserved, then for polymers the equation (32) can be reduced to the following form [5, 55]: 2

lp = l0; lε = lst = l0C∞; le = Rnw = l 0 C ∞ .

(33)

( ) 2

Figure 5 shows dependence Rnw C ∞ , which is linear and passes through the origin of coordinates, though it is fractioned into two straight lines. We are not to analyze the latter circumstance, though it should be mentioned that there are some obvious reasons for it, among which the following are: firstly, broad dispersion of parameters from the literature (l0, С∞, νnw) [45, 53], required for calculation; secondly, there are different approaches to interpretation of the value lε = lst [45, 2

53]. Nevertheless, proportionality of Rnw and C ∞ , shown in Figure 5, proves that C∞ is the self-similarity coefficient at DS-size scale transition from lst to Rnw.

Figure 5. Dependence of the distance between entanglements (chemical cross-link points), Rnw, on the square characteristic relation, C∞, for amorphous glassy (1) and amorphouscrystalline (2) polymers, and polymer networks (3) [5]

Figure 6 compares Rnw values, calculated from equation (33) (Rnw1 and Rnw2, respectively). Data from the Figure indicate tight quantitative conformity between Rnw1 and Rnw2 for the majority of polymers. Possible reasons for occurrence of two lines have been already discussed. Thus C∞ is regulated by the polymer topology, which can be changed by variation of νnw. For a great number of linear polymers,

16

G. V. Kozlov and G. E. Zaikov

Aharoni [53] has observed Rnw increase with the chain flexibility (C∞ increase), expressed by the following equation: Rnw = 10C∞.

(34)

For cross-linked polymers, similar equation as follows was obtained [56]: Rnw = 5C∞.

(35)

Figure 6. The relation between inter-entanglement (between chemical cross-link points) distances, Rnw1 and Rnw2 calculated from the equation (33), for amorphous glassy (1) and amorphous-crystalline (2) polymers, and polymer networks (3) [5]

One more specific length scale, which is the chain part length between entanglements or chemical cross-link points, Lc, does exist in polymers. It can be determined from the equation as follows [5]:

Lc =

F 2ν c S

.

(36)

Figure 7 shows the dependence of “transitional” chain length between 3

entanglements (cross-link points), Lc, calculated by equation (36), on C ∞ . It was also found linear and passing through the origin of coordinates. Expectedly, the straight line slope equals ~1 Å, i.e. possesses the order of magnitude of l0 [53]. This indicates that for this structural level, typical of polymers, C∞ represents the self-similarity coefficient [54, 55].

Clusters as Dissipative Structures

17

DS evolution on the example of polymer networks during their deformation will be considered below using the cluster model for the structure personification. It has been shown [21] that elastic deformation of amorphous polymers is specifically realized in clusters, and the yield stress is the function of entanglement cluster network frequency, νcl, only, i.e. the number of closely packed segments per specific polymer volume [57]. In the light of these facts the yielding can be considered as stability loss by clusters in the field of mechanical stresses. Cold flow of the polymer is considered as deformation of devitrified packless matrix, in which chemical cross-links are represented by clusters [57]. Such interpretation allows personification of structural changes proceeding at polymer deformation in the framework of the model [18, 21, 25].

Figure 7. Dependence of macromolecule segment length between entanglements (chemical cross-link points), Lc, on cubic characteristic relation,

C ∞3 , for amorphous glassy (1) and

amorphous-crystalline (2) polymers, and polymer networks (3) [5]

As mentioned above, the feature of DS formed (or existing) in deformed solid is existence of the universal hierarchy of structural levels [25]. As Balankin has suggested [18, 49], the hierarchic structure of DS is based on the fundamental property of solids, the shearing stability that determines the difference of typical spatial scales of localization zones and dissipation of energy “injected” to deformed body under external impact. Typical scale of the zones (ls), in which excessive energy is dissipated, is proportional to the shear modulus, G. Since in accordance with the above discussion, in the framework of the cluster model, these zones can be associated with the clusters, it is suitable to use their characteristic size, lst, as ls. Figure 5.8 shows relation between G and lst, which is

18

G. V. Kozlov and G. E. Zaikov

approximated by a straight line passing through the origin of coordinates. This proves correctness of lst use for ls.

Figure 8. Relation between statistical segment length, lst, and shear modulus, G, for EP-1 (1), EP-2 (2), EP-1-200 (3) and EP-2-200 (4) [5]

Concerning the next stage in the hierarchy of the structural levels, taking into account the above-mentioned interpretation of the cold flow process and equation (33), the distance between clusters, Rcl, should be taken for ls. The typical size of injected energy localization zones, le, is proportional to (В + 4/3G), where B is the uniform compression modulus [49]. The possibility of associating Rcl with le can be checked as follows. It is known [49] that the relation of DS spatial scales of DS

neighbor structural levels, Li

DS

and Li +1 , can be expressed by the following

equation:

LiDS +1 LiDS

=

l e B + 4 / 3G = = Λi , ls G

(37)

where Λi is the self-similarity coefficient. Obviously le can be obtained by multiplying (В + 4/3G)/G by ls, which equals lst. The relation between le and (В + 4/3G), shown in Figure 9, was also found linear that proves principal possibility of using parameter le as the characteristic dimension of injected energy localization zones. However, at the structural level

Clusters as Dissipative Structures

19

this assumption can be finally proved by comparison of le and Rcl. It displayed the presence of correspondence between these parameters, but also indicated systematic exceeding of Rcl over le by, approximately, 8 Å. The relation observed between le and Rcl is explained on the basis of schematically depicted cluster structure of amorphous polymers, shown in Figure 10. Obviously for obtaining le, the mentioned decrease of Rcl by 8 Å, which is approximately equal lst, means that injected energy is localized not in the whole volume of the polymer, but in the packless matrix, because cluster with the characteristic dimension lst is excluded from the consideration.

Figure 9. Correlation between characteristic dimensions of injected energy localization zones, le, and parameter (В + 4/3G). For the legend, refer to Figure 8 [5]

Figure 10. Schematic presentation of the cluster structure of amorphous polymer [5]

20

G. V. Kozlov and G. E. Zaikov

Comparison of le and Rcl – lst values, shown in Figure 11, proves this conclusion. As a consequence, structural characteristics lst and Rcl – lst estimated in the framework of the cluster model, considered as spatial scales of DS in neighboring levels, allow assessment of the self-similarity coefficient of polymer mechanical deformation, Λi, from the equation (37). The interrelation of DS scales and injected energy localization processes allow an assumption of a definite correlation between Λi and dimensionality, Df, of excessive energy localization zones in elastically deformable medium [18]. Parameter Df value can be determined from the following equation [18]:

Df =

2(1 − ν ) . 1 − 2ν

(38)

Figure 11. Correlation between characteristic size of injected energy localization zone, le, and Rcl – lst value. For the legend, refer to Figure 8. Straight line marks 1 : 1 relation [5]

Figure 12 shows comparison of Df and the self-similarity coefficient, Λi, for polymer networks. Clearly both absolute values and tendencies of changes of these parameters conform well. Analogous correlation between Rcl and Df – lst was obtained [58] for amorphous, amorphous-crystalline and oriented polymers. As a consequence, in the framework of thermodynamics of non-equilibrium processes, yielding and cold flow processes are described well; the cluster model describes structure of these materials properly. Obviously clusters are identified as DS [5, 54, 55]. Basing on the above-stated, one may suggest that Λi in the equation (37) also equals C∞. Then this equation can be reduced to the following form [5, 41]:

Clusters as Dissipative Structures

B 4 + = C∞ . G 3

21

(39)

In their turn, B and G can be expressed via Young’s modulus, E, and fractal dimensionality, df, of the polymer structure as follows [18]:

B=

E , d d −df

G=

(d − 1)E .

(

)

(40)

(41)

2d f

Figure 12. Correlation between dimensionality of injected energy localization zones, Df, and self-similarity coefficient, Λi. For the legend, refer to Figure 8. Straight line marks 1 : 1 relation [5]

Substitution of equations (40) and (41) into (39) gives quantitative correlation between the molecular parameter C∞, which characterizes statistical flexibility of the macromolecule [60] and compactness of macromolecular coil [53], and supermolecular structure characteristic df as follows [41]:

C∞ =

2f 4 + . d (d − 1) d − d f 3

(

)

(42)

22

G. V. Kozlov and G. E. Zaikov

For the Euclidean three-dimensional space (d = 3), this equation is reduced to the form (30).

Figure 13. Dependence of the polymer structure fractal dimensionality df on characteristic relation C∞. Experimental data: 1 – linear polymers (blow tests); 2 – linear polymers (d calculation by data from [59]); 3 – EP networks; 4 – ultrahigh-molecular polyethylene, produced by solid extrusion; 5 – polyarylate produced by solid extrusion at T > Tg; 6 – linear polymers (tensile tests); 7 – linear polymers (df calculation from small-angle X-ray diffraction results [15]). Continuous line presents calculation by the equation (42). The circle encloses experimental points with the highest deviation from the theoretical curve. For samples 7, experimental errors are indicated [41]

Figure 13 presents comparison of df(C∞) dependencies, calculated by the equation (42) and obtained by different methods [41] for polymers, enumerated in the Figure legend. It is indicated that almost all samples shown display good conformity between the theory and the experiment, except for samples 5, experimental points for which in Figure 13 are enclosed in the circle. All these polymers (PC, PSF, and PAr) represent heterochain polymers with similar structures and properties, possessing relatively low (close to the minimum, as shown below) C∞ values (2.2 – 2.4) [45, 53]. Samples of these polymers were produced by press molding (for blow tests) or cut from films, prepared by solution pouring on a glass support (for tensile tests). At the same time, data for PAr, prepared by solid extrusion at temperatures above Tg, conform much better with the calculation by equation (42). In this method of PAr sample preparation [61] devitrified polymer relaxes rapidly at the extrusion nozzle output that gives high νcl value and induces formation of relaxed packless matrix. A state formed is much closer to the equilibrium, than for press molded or film samples [61]. As a consequence, equations (30) and (42) give the more accurate df values, the closer

Clusters as Dissipative Structures

23

the structure of the polymeric sample approaches thermodynamically equilibrium one. To put it differently, for the current polymers, equations (30) and (42) give minimal df values [41]. Further on, variation limits for С∞, determined from the equation (42), will be appraised. As is known [1, 18], df values for bulky samples at d = 3 vary within the limits as follows: 2 ≤ df < 3. At df = 2, parameter С∞ possesses the minimal value equal 2. As observed from the literature [45, 53, 59], many polymers do not display С∞ < 2. Concerning the minimal value of С∞, at df = 3 it approaches the infinity. Actually, it has been indicated [53] that for some polymers С∞ can reach ~700, which is equivalent of the mentioned tendency in practice, if the asymptotic run of df(C∞) curve at large С∞ is considered (Figure 13). The expression binding dimensionalities Df and df is the following [18]:

D f = 1+

1 . d −df

(43)

For d = 3, it is reduced to the following form:

Df =

4−df 3−d f

.

(44)

Substitution of equation (44) into (30) gives the accurate result: С∞ = Df

(45)

that proves the empirical correlation shown in Figure 12. Two-level DS (micro- and macro-DS) are formed with the polymer network structure [62]. Micro-DS represent the local order zones (clusters), and their formation is due to high viscosity of the reaction mixture during the gel formation. This induces turbulence of viscous media and formation of oriented zones [18]. One more fundamental property of turbulent flows is fractality of the structures formed by them [18]. It is accepted that in three-dimensional turbulent flows energy dissipation mainly proceeds on a multitude with the fractional (fractal) dimensionality. However, experimental data on the rate fluctuation moments testify about impossibility of describing small-scale properties of the turbulent flow with the help of a self-similar fractal. That is why “inhomogeneous

24

G. V. Kozlov and G. E. Zaikov

fractals”, the rules of formation of which at every stage of the scale hierarchy are random in accordance with some probability distribution, are applied to description of turbulent DS. Hence, the energy transfer is described with the help of a random fragmentation model under the assumption that different stages of the process do not correlate. Therefore, the fractal volume does not possess the global invariance property in relation to similarity transformation. Nevertheless, one can calculate fractal dimensionality df determined by the relation as follows [18]: −d

N n ~ Ln f ,

(46)

where Nn is the number of active whirls at the n-th fragmentation step; βn is the part of the volume occupied by whirls of the Ln scale. Therefore:

d f = 3 + log 2 {β }.

(47)

The symbol {…} indicates averaging by ρ(β) distribution. It shall be expected that due to the above-mentioned connection between the turbulence and the order, a definite part of active whirls is finally transformed into clusters. That is why the relative part of clusters, ϕcl, must be proportional to β. Figure 14 shows the relation ϕcl(β) that proves the effect of turbulence of the local order zone formation in epoxy polymers. The dependence presented does not pass through the origin of coordinates. This means that not all active whirls are transformed into clusters, by just a definite part of them. The part of transformed whirls depends on β: the higher β is, the greater the part of such whirls is. Note also that the reverse interrelation does also exist: the presence of the local order in the structure of polymers induces deformation turbulence at the cold flow plateau [63, 64]. The amorphous solid is considered as a fractal non-equilibrium nonergodic system [65] with hierarchically subordinate levels of the structural organization of self metastable defective states. Remind that in [34] the parts of chains participating in the clusters are taken for linear defects of the structure, analogous to dislocations in metals. In this case, dependencies of the cluster ensemble realization probability on the distance l between clusters in the ultrametric space can be presented as follows [65]:

ωω (l ) ~ exp(− l l n ) ,

(48)

Clusters as Dissipative Structures

ω s (l ) ~ l − D ,

25 (49)

where ωω(l) describes low hierarchic systems; ωs(l) describes highly hierarchic systems; ln and D are positive parameters.

Figure 14. Dependence of the relative part of clusters, ϕcl, on the part of volume, β, occupied by active whirls, for sulfur-containing epoxy polymers cured by isomethyltetrahydrophthalic anhydride (1), 4,4’-diaminodiphenylmethane (2), and 4,4’diaminodiphenylsulfone (3) [62]

In this connection, two main questions occur: how good concordance between the concepts of hierarchic organization of the polymer amorphous state structure presented in [34] and [65] (equations (33) and (48), (49)) is, and what type of hierarchy structure is observed in polymers. The answer to these questions is given [66] on the example of 16 amorphous glassy and amorphous-crystalline polymers and polymer networks. Similar to the works [67, 68], it is suggested that relative part of the local order zones (clusters), ϕcl, organizing the hierarchy of the polymer amorphous state structure must be a function of ensemble realization probability for such clusters (ωω(l) or ωs(l)). To calculate probabilities ωω(l) and ωs(l) by equations (48) and (49), respectively, the following assessments were used. The value l is accepted equal Rcl and is calculated as shown in Chapter 2; ln = const = 100 Å, and this selection is stipulated by the fact that 100 Å size represents the upper linear scale of the fractal behavior of the polymer condensed state [4, 5]. Finally, index D in the equation (49) is equaled to the fractional part of the fractal dimensionality df of the polymer structure as follows:

26

G. V. Kozlov and G. E. Zaikov D = df – 2,

(50)

because the fractional part, df, characterizes the structure change (2 ≤ df < 3 [5]).

Figure 15. Dependence of the relative part of clusters, ϕcl, on low hierarchy system realization probability, ωω(l), for amorphous glassy (1) and amorphous-crystalline (2) polymers, and polymer networks (3) [66]

Figures 15 and 16 show dependencies of ϕcl on cluster ensemble realization probabilities, ωω(l) (low hierarchy systems) and ωs(l) (highly hierarchy systems), respectively. Clearly for all three classes of polymers under consideration, the correlation ϕcl(ωω(l)) is approximated by a linear dependence passing though the origin of coordinates, whereas the correlation ϕcl(ωs(l)) clearly represent the curve. Linearization of the latter correlation in the form as follows: ϕcl = f[(ωs(l))1/2], is shown in Figure 17, which indicates satisfactory linear approximation of this function by a straight line passing though the origin of coordinates. As a consequence, the dependence ϕcl(ωω(l)) is much stronger (magnitude 1) than the dependence ϕcl(ωs(l)) (magnitude 1/2). To put it differently, in the second case, the hierarchy structure is formed much less intensively than allowed by the probability ωs(l). These results assume that hierarchic organization of the polymer supermolecular (supersegmental) structure occupies the intermediate position between high and low hierarchy systems, shifted towards the latter. This situation is explained by the macromolecular origin of polymers. Segments forming the hierarchy, which participate in the clusters, are linked by strong covalent bonds to the polymeric chain that strictly limits their ability to form similar structures. Moreover, the above-mentioned data have

Clusters as Dissipative Structures

27

proved the hierarchy of supermolecular (supersegmental) structure of the amorphous state and conformity of models [34] and [65] for three main classes of polymers. Note also that the basic reason for distribution of data in Figures 15 – 17 is application of С∞ values from the literature, which can vary in significantly broad range for the same polymer [59].

Figure 16. Dependence of the relative part of clusters, ϕcl, on the high hierarchy system realization probability, ωs(l), for amorphous glassy (1) and amorphous-crystalline (2) polymers, and polymer networks (3) [66]

To complete this Section, the authors discuss the way of obtaining two fundamental conclusions in the framework of synergism and fractal analysis: dependence of the “hooking” network frequency on statistical flexibility of the chain and increase of the physical entanglement network frequency (e.g. cluster network formation) in the polymer glassy state. The idea of macromolecular entanglements’ network is one of the basic positions in the rheology of polymers [45], though attempts to apply other approaches shall also be mentioned [69]. Multiple attempts were also made to apply a model of such network, cross-link points of which are interpreted as macromolecular "hookings" [45], to description of glassy polymer properties (for example, [70, 71]). This has induced the increased interest to investigation of possible correlations between molecular characteristics of polymers and topology of macromolecular entanglement network [48, 53, 72]. Essentially, the authors of these works have come to the single point of view that macromolecular “hooking” network frequency, νnw, increases with polymer chain rigidity. However, it should be noted that parameter νnw is experimentally determined for the rubber-like state of polymers (at T > Tg);

28

G. V. Kozlov and G. E. Zaikov

it is assumed that at transition to the glassy state νnw does not change. Disadvantages of this interpretation became clear very soon. Actually, if crosslink points of such molecular hookings are considered as the points of topological chain fixation, then the assumption of equality of their frequencies in the rubbery and glassy states is very ambiguous. For example, polymer deformability decrease at transition from the rubbery to the glassy state is known well, but according to the indicated assumption this change must not happen, and for both cases, the stretch rating λ is determined from the known formula [73]:

Figure 17. Dependence of the relative part of clusters, ϕcl, on parameter [ωs(l)]1/2 for amorphous glassy (1) and amorphous-crystalline (2) polymers and polymer networks (3) [66]

λ = n1st 2 , (51) where nst is the number of statistical segments in the chain intersect between entanglements. To explain the observed change in properties at coming over Tg, a series of models has been suggested. For example, it is assumed [74] that chain sliding through entanglements, which explains λ increase with temperature, is intensified with temperature. In the models [34, 75] increase of the number of chain fixation points is assumed at transition from the rubbery to the glassy state. These fixation points are called the “sliding units” [75] or clusters [34]. In any case, they determine limitations of molecular mobility of the chain in the glassy state [42].

Clusters as Dissipative Structures

29

In the framework of deformable solid synergism, it has been shown [76] that the part of dissipating energy, η, can be estimated from the following equation: β

η = 1− Λ p ,

(52)

where Λ is the structure self-similarity coefficient; βp is the fractional part of the fractal dimensionality of the fracture surface, dp. In accordance with the above-shown, for the structure of polymers, the following equality is true: Λ = С∞, and in the case of quasi-friable destruction, dp value can be assessed as follows [18]:

dp =

10(1 + ν ) . 7 − 3ν

(53)

Fractal dimensionality, D, of the chain part between entanglements is the structural parameter characterizing molecular mobility level and, consequently, the energy dissipation level [77]. Techniques for D assessment are given in the work [5]. Good correlation between (D – 1) and η parameters was obtained for 15 amorphous and amorphous-crystalline polymers [78] (remind that 1 ≤ D ≤ 2 and 0 ≤ η ≤ 1). Physical basis for this correlation is obvious. As mentioned above, D parameter characterizes molecular mobility, and intensification of the latter always induces increase of mechanical energy dissipation applied to the polymer [79]. The length of the chain segment between “hookings”, Lc, is calculated for the rubbery state that allow modification of the equation (52) as follows. For rubbers, ν is close to 0.5 (but not equals it [18]). That is why dimensionality, dp, must be calculated for viscous degradation under the condition ν ≥ 0.375 [18]. In this case, the equation for dp calculation is as follows [18]:

dp =

2(1 + 4ν ) . 1 + 2ν

(54)

As ν ≈ 0.45 is chosen for rubbers [80], calculation by the equation (54) gives dp ≈ 2.95, i.e. in the first approximation one can accept β ≈ 1 in equation (52). Then under the above-mentioned conditions (η = D – 1 and Λ = С∞) modified equation (52) is obtained:

30

G. V. Kozlov and G. E. Zaikov

D = 2−

1 . C∞

(55)

In its turn, dimensionalities D and df are interrelated by the following expression [5]:

D=

ln n st . ln 4 − d f − ln 3 − d f

(

) (

)

(56)

Combined equations (54) – (56) allow calculation of nst for rubbers practically by known C∞ values only, because ν (or df and dр) values are fixed. The equation for Lc assessment is deduced as follows [78]: Lc = nstlst = nstl0C∞.

(57)

Table 2. Values of characteristic relations С∞, backbone real bond lengths l0, e

t

experimental Lc and theoretical Lc lengths of the chain intersects between macromolecular “hookings” for some polymers [78] Polymer Poly-n-dodecylmethacrylate Poly-n-octylmethacrylate Polystyrene Polyvinylacetate Poly-n-butylmethacrylate Poly(methyl methacrylate) Polyethylene Polyvinylchloride Polytetrafluoroethylene Polyamide-6 Polypropylenoxide Polyethylenoxide Poly(ethyleneterephthalate) Poly(ester terephthalate) Polycarbonate

C∞ [45,53] 13.4 10.0 10.0 9.4 9.1 8.6 6.8 6.7 6.3 5.3 5.1 4.2 4.2 3.3 2.4

l0 [45,53], Å Lec , nm [81] Ltc , nm 1.54 1.54 1.54 1.54 1.54 1.54 1.54 1.54 1.54 1.49 1.49 1.49 1.25 1.25 1.25

226 177 104 88 130 97 56 31 41 46 60 45 21 28 29

208 149 149 136 131 92 88 87 80 61 58 43 36 30 17

Clusters as Dissipative Structures

31

Table 2 shows parameters l0 and C∞ required for calculation and accepted in

( )

accordance with [45, 53], Lc Lec values from the literature (in accordance with

( )

[81]), and Lc Ltc values calculated by the method above. The Table indicates good conformity between theoretical and experimental results.

Figure 18. Dependence of theoretical lengths of the chain intersect between entanglements

Ltc

on characteristic relation C∞ for polymers listed in Table 2 [78]

Figure 18 shows correlation Ltc (C∞) for polymers, mentioned in Table 2. Good linear correlation obtained proves already known principle of entanglement network frequency increase with statistical chain rigidity [45]. At Ltc = 0, the dependence Ltc (C∞) is extrapolated to С∞ ≈ 2 that corresponds to tetrahedral valence angle θ (≈ 70.5°) in the chain model with fixed valence angles [60]. However, this value of С∞ cannot be considered the border one. As follows from the equation (55), С∞ = 1 at the border value D = 1 [5]. In the mentioned model of the chain with fixed valence angles С∞ is determined as follows [60]:

C∞ =

1 + cos θ . 1 − cos θ

(58)

32

G. V. Kozlov and G. E. Zaikov

Obviously at С∞ = 1, cosθ = 0 and θ = 90°. Thus the fractal analysis assumes С∞ falling within the range of 1 – 2 and arbitrary sharp valence angles. It is known [80, 82] that transition from the rubbery to the glassy state is accompanied by the Poisson coefficient decrease, which value below Tg depends on the test temperature. This means decrease of df in accordance with the equation (4) and nst (i.e. decrease of Lc) in accordance with the equation (56) in the glassy state rather than in the rubbery state even at invariable D. This effect is intensified by the appropriate decrease of D that follows even from the well known fact as follows: the decrease of molecular mobility in the polymer glassy state [59], and is proved experimentally [5]. Thus the fractal analysis suggested enables forecast of the topological chain fixation point number increase at T < Tg, suggested before [75, 83].

Figure 19. Dependencies of

Lec Lcl

(1) and

Ltc 0 Ltc

(2) (see text for details) on the

test temperature for PC [78]

Quantitatively, this forecast can be checked by temperature dependence of two relations. The first of them is the relation of chain intersect lengths between e

“hookings” Lc (the rubbery state) [81] and between clusters Lcl (the glassy state) t

[83]. The second one is the relation between lengths, Lc , obtained by the abovet

mentioned method at ν = 0.45 ( Lc 0 , the rubbery state) and at ν values. The first

Clusters as Dissipative Structures

(

33

) gives results, obtained within the framework of the cluster model [83]; the second one (L 0 L ) - in the framework of the fractal analysis. e

relation Lc Lcl

t c

t c

Figure 19 shows temperature dependencies of both relations for PC, for which t

good conformity was observed. Values of Lc were calculated at randomly chosen D = 1.75, but any other choice in the above-mentioned interval will not change symbate type of dependencies, shown in Figure 19, but just slightly deviate their quantitative conformity. Thus in the framework of the fractal analysis the increase of macromolecular “hookings” network frequency with statistical chain rigidity was proved. In contrast with previous studies, the fractal analysis forecasts increase of the number of topological fixation points of macromolecules in the glassy state rather than in the rubbery one. The cluster model of the polymer amorphous state structure gives correct quantitative description of this effect [78].

Chapter 3

CLUSTER AND FLUCTUATION FREE VOLUME MODELS The fluctuation free volume model is widely spread in descriptions of the physical meaning of liquids and glasses [84 – 86]. Hence, the physical meaning of the model parameters is yet mainly unclear [87, 88]. Moreover, difficulties appear in the free volume theory concerning explanation of the temperature dependence of kinetic properties, in particular, viscosity at fixed volume of the system. The relative part of the fluctuation free volume, ff, is determined, for instance, by data in the glass transition zone [85, 86]. If ff is known, one can calculate the formation energy of the minimal free volume microcavity, εh, by the formula as follows [86]:

εh = kTgln(1/ff).

(59)

Let us now turn to comparison of the cluster model with the fluctuation free volume for solid polymers [83, 89]. Obviously in accordance with the cluster model the fluctuation free volume is accumulated in the packless matrix. In terms of the free volume theory, detachment of a kinetic unit (an atom or a group of atoms) from a cluster means formation of a random microcavity, and addition of a kinetic unit to a cluster means its “implosion” (annihilation). As a consequence, random change of the free volume with temperature can be realized in principle at a constant volume of the system due to microcavity exchange between clusters and the packless matrix. This approach to the mechanism of generation and migration of random microcavities overcomes the above-mentioned difficulty in

36

G. V. Kozlov and G. E. Zaikov

explanation of the temperature dependence of viscosity at fixed volume of the system [89]. νcl, and cluster functionality, F, with temperature increase for amorphous glassy polymers [90]. Analysis of these data induces a conclusion that the number of clusters per specific volume of the polymer remains practically unchanged with temperature increase, but the number of segments in each cluster decreases. However, at T = Tg in the glass transition zone clusters are completely decomposed (νcl = 0), and excessive fluctuation free volume reaches the critical value. Thus from these positions, devitrification of a glassy polymer is caused by cluster decomposition (i.e. annihilation of the local order). Therefore, energy of the cluster formation or decomposition, Ucl, must possess the magnitude of the average energy of kinetic unit (statistical segment) heat motion at the glass transition temperature: Ucl ≅ (i/2)kTg, where i is the number of degrees of freedom of the kinetic unit. If one takes into consideration that a segment consists of many atoms, then in the first approximation i must equal the number of degrees of freedom in a multiatomic molecule, i = 6 [89].

Figure 20. Correlation between the segment interaction energy in the cluster, Ucl, and kTg value for the polymer solid phase at T = 293 K: 1 – HDPE, 2 – PP, 3 – PA-6, 4 – PETP, 5 – PVC, 6 – PHE, 7 – PTPE, 8 – PC, 9 – PSP, 10 – PAr [89]

Expectedly, the energy of segment detachment from the cluster was found proportional to the glass transition temperature of polymers (Figure 20). It is noteworthy that the slope of Ucl(kTg) line is practically coincident with i/2 value and the coefficient of proportionality between energy of the minimal random microcavity formation (see equation (59)): Ucl = 3.3 kTg and εh = 3.5 kTg. It is

Cluster and Fluctuation Free Volume Models

37

taken into account here that common value of ff for glassy polymers equals 0.025 and ln(1/ff) = 3.5. As a consequence, the energy of random microcavity formation is practically coincident with the energy of segments’ interaction in the cluster (εh = Ucl). From this point of view, generation and implosion of a random microcavity in amorphous polymers are stipulated by dissociation and segment association into a cluster, respectively. Microcavity formation energy equals the work for collinear segments detachment from one another in the cluster by breaking intermolecular bonds between them, and the magnitude of the microcavity minimum size (≈ 4 – 5 Å [89]) equals the border elastic deformation of the intermolecular bond between segments. Ucl decrease with temperature due to the presence of temperature dependencies of G and ν [91]. It can be shown that for glassy polymers, ff increases (though slowly) with temperature [92] that induces the corresponded decrease of εh. However, it should be noted that temperature dependencies of energies εh and Ucl are very weak. Apparently, this is explained by the fact that parameters εh and Ucl represent characteristics of the short-range (local) order of glasses, weakly responding to temperature variation (anyway, at T < Tg′ [90]).

Figure 21. Dependence of the relative fluctuation free volume, ff, on volumetric part of the packless matrix, ϕp.m., for linear amorphous polymers: PC (1) and PAr (2) [93]

Besides the above-considered correspondence between the cluster model and the kinetic theory of the fluctuation free volume, application of the former one allowed obtaining of a series of new ideas on the interconnection between structure and free volume [93]. For example, Figure 21 shows dependencies of the relative random volume, ff, on the volumetric part of packless matrix, ϕp.m., for

38

G. V. Kozlov and G. E. Zaikov

two linear amorphous polymers, PC and PAr. The dependencies are linear, and their extrapolation to ϕp.m. = 0 gives ff = 0. The latter means that in this case, an amorphous polymer represents a huge cluster without a fluctuation free volume. Clearly this circumstance does not exclude the presence of a configurative free volume [94]. At ϕp.m. = 1.0 ff is extrapolated to a finite value, approximately equal 0.14 and corresponded to ff at the glass transition temperature [95]. For glassy polymer networks, the type of dependencies ff(ϕp.m.) differs from the above-considered one (Figure 22). Similar to the case of linear amorphous polymers, they are approximated well by a straight line. However, the line does not pass through the origin of coordinates, but at ϕp.m. = 0 cuts an intersect ff ≈ 0.024 on the axis of ordinates. One can assume that this value of ff is associated with the presence of a network of chemical cross-link points. Thus in contrast with linear polymers, in polymer networks the relative fluctuation free volume consists of two components. One of them is constant and connected with the zones of chemical cross-link points; the second one is the linear function of ϕp.m. and is determined by supersegmental (cluster) structure. Various components of ff determine different properties of epoxy polymers: variable part of ff regulates elasticity and local plasticity, and total value of ff regulates properties in the zone of macroscopic flow behavior [96].

Figure 22. Dependence of the relative fluctuation free volume, ff, on volumetric part of the packless matrix, ϕp.m., for epoxy polymers: EP-1 (1), EP-2 (2), EP-1-200 (3), and EP-2-200 (4) [93]

Thus correlations obtained using the cluster model of the polymer amorphous state structure allow an observation that the fluctuation free volume, and the type

Cluster and Fluctuation Free Volume Models

39

of its variation with respect to structural factors are significantly determined by the type of polymer structure [93].

Chapter 4

THE CLUSTER MODEL AND THE ANHARMONICITY CONCEPT In recent 20 years, increased interest to the Grüneisen parameter, γ, is observed in physics of liquids and glasses. This parameter participates in the equation of state and represents the anharmonicity index of quasi-lattice oscillations and nonlinearity of interatomic interaction forces [59, 97]. The Grüneisen parameter was successfully applied to analysis of the cluster formation event and orientation of molecules in liquids [98 – 100]. Since a liquid and the glassy state are structurally indistinguishable [101], of interest is the Grüneisen parameter application to studies the local order in glassy polymers. In the framework of the cluster model temperature dependence of γ for amorphous polymer was interpreted [83]. Knopoff and Shapiro [98] have indicated that for water and mercury, γ decrease with the specific volume increase can be assigned to the change of the average number of molecules in the cluster, N. They have suggested a semiquantitative one-dimensional model, which enables description of γ dependence on volume. It is assumed that γ represents the sum of two components [98]:

γ = γD +ξ

∂ ln N ∂ ln V

,

(60)

T

where γD is the component of γ corresponded to the Debye heat capacity theory; ξ is a factor dependent on N.

42

G. V. Kozlov and G. E. Zaikov

The equation (60) describes γ variation with pressure, P, but due to equivalence of P and T variables in the equation of state it can be used for assessment of the temperature dependence of γ under constant pressure. In this case, index T in the equation (60) is replaced by P. The Debye component γD in the Grüneisen parameter can be assessed as follows [98]:

γ = −ξ

∂ ln ω D ∂ ln V

,

(61)

P

where ωD = πω0 is the Debye frequency of polymeric chain oscillations; ω0 is determined as follows:

ω0 =

U . M

(62)

Here M is the mass of oscillating kinetic unit of the chain; U is the potential energy of interaction between two kinetic units, accepted equal Ucl in the framework of the cluster model. Temperature dependence of the specific volume, V, is calculated by the following equation [100]:

(V~

13

)

−1 =

αT , 3(1 + αT )

(63)

~

where V = V/V* is the reduced specific volume; V* is the characteristic specific volume; α is the volumetric coefficient of heat expansion, temperature dependence of which is determined as follows [83]:

⎛α 2 ⎞ ⎛ ∂α ⎞ ⎟. ⎜ ⎟ = (7 + 4αT )⎜⎜ ⎟ ∂ T 3 ⎝ ⎠P ⎝ ⎠

(64)

Accepting α value at T = 293 K [83] and characteristic volume as the reverse density, ρ, one can obtain correlation lnωD(lnV), shown in Figure 23 for PAr and PSF. Clearly the correlation between ωD and V in double logarithmic coordinates

The Cluster Model and the Anharmonicity Concept

43

is well approximated by a linear correlation. In accordance with the equation (61), this means that γD constancy in the considered temperature interval (293 – 453 K for PAr and 293 – 433 K for PSF). Absolute values of γD can be estimated from the slope of lines in Figure 23, which are independent of V* selection: these values (γD = 12 for PAr and γD = 13.75 for PSF) are close to the ones previously obtained for polymers of this type [102].

Figure 23. Variation of the Debye frequency, ωD, with the specific volume, V, present in double logarithmic coordinates for PAr (1) and PSF (2) [83]

Figure 24. Correlation between the average number of segments in the cluster, nseg, and the specific volume, V, present in double logarithmic coordinates for PAr (1) and PSF (2) [83]

Thus for the case of temperature independence of the segments’ number in the cluster, the above-shown results indicate obligatory fulfillment of the following condition (equation (60)) [83]:

γ = γD = const.

(65)

44

G. V. Kozlov and G. E. Zaikov

Indicated in the above discussion was γ decrease with temperature [59]. It is assumed that dN ≠ 0, whence the necessity of assessment of the second term in the equation (60) follows. As indicated in Chapter 2, N = nseg = F/2. Figure 24 shows dependence lnnseg(lnV) for PAr and PSF; both dependencies are described by single linear relation that gives an opportunity to assess the relation ∂lnnseg/∂lnV ≈ 6.5. For large nseg, parameter ξ in equation (60) at temperatures above the Debye point is approximated by the following series expansion [98]:

ξ = 0.6942 +

0.03780 + ... . n seg

(66)

Figures 25 and 26 show temperature dependencies of γ, calculated by equation (60) for PAr and PSF, respectively.

Figure 25. Temperature dependence of the Grüneisen parameter γ for PAr: the Debye component γD (1), calculations by equations (60) (2), (67) (3), and (68) (4) [83]

Figure 26. Temperature dependence of the Grüneisen parameter γ for PSF: the Debye component γD (1), calculations by equations (60) (2), (67) (3), and (68) (4) [83]

The Cluster Model and the Anharmonicity Concept

45

The value of γ can also be calculated by two independent methods as follows. The first method uses simple relation for temperature dependence of the elasticity modulus, E [103]: Е = Е0(1 - γαТ),

(67)

where Е0 is the value of E extrapolated to 0 K. The second method is based on application of the Sharma equation [100]:

(

)

⎛ 1 ⎞ 1 ~1 3 ⎟ − 5V − 2 . ⎝ 2αT ⎠ 3

γ = 1+ ⎜

(68)

The values of γ calculated for PAr and PSF by equations (67) and (68) are also shown in Figures 25 and 26, respectively. Clearly calculation results by three equations mentioned display high coincidence. Previously, γ decrease with temperature was attributed to accompanying the elasticity modulus decrease; in its turn, the latter was attributed to decrease of the cluster network frequency, e.g. nseg decrease [57]. Thus the above-shown results conform to previously suggested explanation of the effect observed. Equations (60), (67) and (68) give adequate description of γ(Т) dependence by both the general tendency and absolute values. In its turn, this proves correctness of the cluster model and suitability of application of the anharmonicity concept to description of the local orientation of the polymer amorphous state structure [83].

Chapter 5

CLUSTER STRUCTURE AS A PERCOLATION SYSTEM Percolation models are widely used for description of many physical problems [22], including polymers [104 – 108]. These models are differed by simplicity and demonstrativeness [22], and their application to description of the structure and properties of polymers allows the use of the well-developed mathematical apparatus of the percolation theory. The cluster structure formation at Tg sharply changes properties of amorphous polymers attributing their rigidity typical of solids [90]. That is why one may suggest Tg representing the percolation threshold on the temperature scale in this case, at which an infinite cluster (in the sample borders) is formed. Relating to description of polymers, the “carcass coherency” concept [109, 110], suggested 35 years ago, can be accepted to be the predecessor of percolation models. This concept assumes that the existence of carcass coherency of macromolecules in polymers is the necessary condition of their rigidity and strength. It also gives a relation for assessing probability of the carcass bond formation, ηх. The most probable candidate for the carcass role in linear amorphous and amorphous-crystalline polymers is the network of macromolecular entanglements. As mentioned above, two basic concepts of the structure of such network do exist now: the “hooking” network and the cluster network. The contribution of these networks to the carcass coherency of amorphous and amorphous-crystalline polymer and, consequently, their mechanical properties were determined [111]. If the cluster network of macromolecular entanglements is accepted to be such carcass, it is natural to assume equality of the probability of this “carcass”

48

G. V. Kozlov and G. E. Zaikov

formation, ηх, to the relative part of clusters, ϕcl. The value of ηх can be assessed as follows [109]:

ηx =

S , ac E

(69)

where S is the cross-section of the macromolecule; ac is the analogue to Young’s modulus for elastic stretch of macromolecules; E is the elasticity modulus, determined experimentally. The value of ac can be assessed in accordance with recommendations in the ref. [109], which gives the following results [11]: 2.22×10−1 N for LDPE; 4.5×10−10 N for HDPE; 7.5×10−10 N for PC and PAr. Figure 27 shows comparison of ϕcl and ηх for PC and PAr. Clearly a linear correlation between them is observed, but ηх values regularly exceed appropriate ϕcl values. At ϕcl = 0 ηх is extrapolated to ηх0 ≈ 0.18 that assumes existence of two carcasses in amorphous PC and PAr. Moreover, frequency of one of these carcasses (the cluster one) is the function of temperature, whereas the second carcass (macromolecular hookings) possesses constant frequency. Macromolecular hookings’ carcass frequency, ηх0, is assessed from the following equation [109]:

ηx0 = nx0S.

(70)

Then the molecular mass, Mx0, of the chain segment between neighbor hookings can be calculated. For PC and PAr, Мх0 ≈ 1,610 g/mol. Values of this parameter shown in the literature are as follows: 1,780 – 2,250 g/mol [45] and 1,400 – 2,426 g/mol [112], which correlate well with the assessment. Thus for amorphous glassy PC and PAr polymers, the cluster network of macromolecular entanglements represents the "carcass", and contribution of the macromolecular “hooking” network is rather low (especially at low temperatures) and constant [111]. Figure 28 shows the same comparison of ϕcl and ηх for LDPE and HDPE. Similar to two amorphous polymers (Figure 27), linear correlation between ϕcl and ηх is observed. However, for LDPE and HDPE linear approximation passes through the origin of coordinates, i.e. ϕcl ≈ ηх. This fact is explained by the devitrified state of the polyethylenes’ amorphous phase in the temperature interval studied; thus the elasticity modulus of the phase (and, respectively, ηх) is very low

Cluster Structure as a Percolation System

49

(~2.1 MPa [45]). That is why ηх0 value is much lower than inaccuracy of the graphical correlation ηх(ϕcl).

Figure 27. Dependence of the coherency carcass formation probability, ηх, on the relative part of clusters, ϕcl, for PC (1) and PAr (2) [111]

Figure 28. Dependence of the probability of coherence carcass formation, ηх, on the relative part of clusters, ϕcl, for LDPE (1) and HDPE (2) [111]

Thus the above results allow the statement that the macromolecular entanglement cluster network represents the “carcass” for amorphous and amorphous-crystalline polymers. As a consequence, this very network causes the main impact on mechanical properties of solid polymers (especially amorphous ones [57]). Contribution of the macromolecular hooking network is independent of temperature and is sufficient in the glassy state of polymer only. Estimation performed by the equation (69) has indicated that the presence of the macromolecular hooking network only in PC and PAr would give, approximately, three-fold lower elasticity modulus compared with the experimentally observed one, and polyethylenes would completely lose rigidity [111, 113].

50

G. V. Kozlov and G. E. Zaikov

It is known [22] that at approach of percolation threshold, хс, critical behavior of the infinite cluster cardinality, Р∞ (the probability of cross-link point belonging to the current cluster), is described by the scaling relation as follows:

P∞ ~ ( x − xc )β n .

(71)

In the framework of the cluster model, ϕcl is the obvious selection for Р∞, and the glass transition temperature, as mentioned above, is accepted for хс [67, 68]. In this case, the test temperature, T, is accepted as the current probability, X, and the relation (71) can be reduced to as follows [67]:

ϕ cl ~ (Tg − T )β n = (ΔT )β n ,

(72)

where changing over Tg and T is caused by the inequality Tg > T. Figure 29 shows dependence ϕcl(ΔТ) in double logarithmic coordinates, corresponded to correlation (72). The graph of this dependence is linear that enables calculation of βn ≈ 0.46.

Figure 29. Dependence of the relative part of clusters, ϕcl, on temperature difference (Tg – T), presented in double logarithmic coordinates for PMMA (1), PC (2), and PAr (3) [67]

This value is close to theoretical “classical” one βn = 0.40 for a threedimensional percolation cluster [22]. The graph in Figure 29 is plotted for the temperature range Tg – (Tg – 80 K), because correlation (71) is true under the condition х → хс [22] (or Т → Тg). Thus the amorphous polymer structure represents a percolation cluster, which can be described by general laws of the

Cluster Structure as a Percolation System

51

percolation theory [67]. The same result was obtained for glassy polymer networks [68] and amorphous-crystalline polymers [114]. For example, in the framework of these general laws, the number of cross-link points, S, in a finite cluster, which can be the local order zone consisting of F/2 closely packed segments (where F is the cluster functionality [90]), depends upon dimensionless deviation of concentration, τ, from its critical value (τ = (х – хс)/хс [22]) at τ → 0 as follows:

S~τ

−γ n

.

(73)

As mentioned above, the number of cross-link points, S, in the local order zone (classified as the cluster [34, 90]) equals F/2, and for τ parameter (Тg – Т)/Тg should be accepted. Figure 30 shows dependencies of F/2 on (Тg – Т)/Тg in double logarithmic coordinates for epoxy-polymers. The dependencies were found linear that allowed estimation of the index in correlation (73) as 1.28 for EP-1 and 2.28 for EP-2. For amorphous glassy polymers the following values of γn were obtained: ~1.45 for PMMA, ~1.36 for PC, and ~1.14 for PAr. All calculated values of γn satisfactorily correlate with its theoretical value (= 1.84) for a threedimensional cluster [22].

Figure 30. Dependencies of the number of cross-link points (segments) in a finite cluster, F/2, on dimensionless temperature deviation, τ = (Тg – Т)/Тg, presented in double logarithmic coordinates for EP-1 (1) and EP-2 (2) [68]

As a consequence, the results obtained [67, 68, 114] indicate that at temperature Tg (Tmelt) a structure of statistical segments is formed in amorphous (amorphous-crystalline) polymers representing a percolation cluster and being

52

G. V. Kozlov and G. E. Zaikov

described properly in the framework of the cluster model. This circumstance assumes the polymer glass transition represents the phase transition, and ϕcl value is the orientation parameter [22]. Moreover, this is one more proof for fractality of the polymer structure in the range of ~3 – 100 Å (refer to Section 1). Of special interest is the fact that critical indices of the orientation parameter, βn, obtained in refs. [67, 68, 114], though are very close to the classical percolation indices (βn = 0.37 – 0.40 [115]), but differ from them by the absolute value. The reason for such inconsistency is the percolation cluster representation as a pure geometrical structure, which is too simplified simulation of natural amorphous polymers, which possess thermodynamically non-equilibrium structure. That is why the structure of the mentioned polymers is affected by thermal interactions (remind that the cluster structure is postulated as a thermofluctuational system [34]). This means that the percolation cluster (carcass) of the polymer structure consists of elements (statistical segments) possessing molecular mobility, e.g. they oscillate around some quasi-equilibrium position. Such elements form a virtual volume, which exceeds the volume of a cluster from static elements that makes the percolation process simpler and allows formation of the percolation carcass from smaller number of elements or with higher βn value. Moreover, cluster formation is studied by the scale of relative temperatures, but not by the scale of concentrations as for the percolation cluster [22, 115]. As a consequence, thermal cluster, i.e. the cluster which equilibrium configuration is determined by both geometrical and thermal interactions [116], is more correct simulation of the polymer amorphous state. In this case, the orientation parameter ϕcl of the polymer structure is determined from the following equation [116]:

ϕ cl

⎛ Tg − T ⎞ ⎟ =⎜ ⎜ Tg ⎟ ⎝ ⎠

βT

,

(74)

where index of the orientation parameter, βТ, is not necessarily equal to the appropriate critical index, βn, in pure configuration percolation models. An attempt was made [117] to estimate variation of βТ absolute values, detect possible connection between this index and structural characteristics of polymers, and determine factors affecting βТ value. This was performed on the example of three series of epoxy polymers: amine (EP-1) and anhydride (EP-2) cross-linking type, and EP-1 after natural aging under atmospheric conditions during 3 years (EP-3) [18].

Cluster Structure as a Percolation System

53

It has been shown [119] that universality of critical indices of the percolation system is directly bound to the fractal dimensionality of this system. Selfsimilarity of the percolation system assumes the presence of a series of subsets possessing the order n (n = 1, 2, 4, …), which in the case of the amorphous polymer structure are identified as follows [117]. The first subset (n = 1) is the carcass of the percolation cluster or, as shown above, cluster network of the polymer. The second subset (n = 2) represents the packless matrix, to which cluster network is buried. In this interpretation, critical indices βn, νn, and tn are given as follows (in the three-dimensional Euclidean space) [119]:

βn =

1 , df

(75)

νn =

2 , df

(76)

tn =

4 , df

(77)

where df is the fractal dimensionality of the polymer structure, determined by the equation (4). Thus βn, νn, and tn parameters represent border values for βТ pointing out the structural component of the polymer that determines its behavior. As βТ = βt, this component are clusters or, more accurately, the percolation cluster carcass identified with the cluster network. As βn < βT < νn, the polymer behavior is determined by joint influence of clusters and packless matrix. As βТ = νn, the determining structural component will be the packless matrix, and at βТ = tn the chemical cross-link network; at νn < βT < tn a joint influence of two abovementioned structural components is observed. For three series of epoxy polymers under consideration, assessments of βT parameter have indicated their possible approximation by the following values: ≈ 0.54 for EP-1, ≈ 0.55 for EP-2, and ≈ 0.38 for EP-3. Figure 31 compares ϕcl values as the function of Kst, experimental [5] and calculated by the equation (74), using the above βT values. In the framework of the thermal cluster model, experimental and calculated values conform well. The average Df value for three studied series of epoxy polymers equals 2.613. This means that according to

54

G. V. Kozlov and G. E. Zaikov

equations (75) and (76) βn ≈ 0.38 and νn ≈ 0.77. Comparison of these assessments and βT values, calculated from the equation (74), indicates that the cluster network is the basic structural factor for EP-3, and behavior of EP-1 and EP-2 is regulated by the joint effect of cluster network and packless matrix. Thus for aged epoxy polymers (EP-3) only indices of the orientation parameter of percolation and thermal clusters coincide. For the case under consideration, this indicates insufficiency of thermal interaction for the polymer structure and that its equilibrium configuration is determined by geometrical interactions only. It has been shown [118] that during heat aging the structure of epoxy polymer EP-3 reaches its quasi-equilibrium state, characterized by the balance between the tendency to local order increase, the index of which is ϕcl, and entropic chain straining. Hence chain intersects between clusters are stretched, and their fractal dimensionality D approaches 1. This indicates [5, 77] full suppression of molecular mobility of these parts of the chains.

Figure 31. Dependencies of the relative part of clusters, ϕcl, obtained experimentally (1 – 3) and calculated by equation (74) (4 – 6), on Kst for epoxy polymers: EP-1 (1), EP-2 (2), and EP-3 (3) [117]

For EP-1 and EP-2, D > 1 [5] and, as follows from Figure 5.31, βТ > βn. Consequently, it may be assumed that the condition βТ > βn is induced by nonzero molecular mobility, e.g. 1 < D ≤ 2 [5]. To check this assumption, one shall calculate D value that can be made differently, (for example, using equation (55) or (56)), but the authors in the work [117] have used a simple formula as follows [77]:

Cluster Structure as a Percolation System

2

ϕ cl

= C ∞D .

55

(78)

Figure 32 shows the dependence βТ(D) for three series of studied epoxy polymers. Expectedly, increase of D leads to βТ growth. As D = 1, βТ ≈ 0.38, i.e. the condition βТ = βn is fulfilled. The condition βТ = νn is reached at D ≈ 1.42, and extrapolation of the dependence βТ(D) shown in Figure 5.32 to D = 2 gives βТ ≈ 1.35. As known [120], D = 2 indicates a rubber-like state of polymer (df ≈ 3), characterized by complete degradation of the cluster structure [121]. In accordance with the equation (77), at df ≈ 3 tn ≈ 1.33, i.e. for rubber-like polymers the condition βТ ≈ tn and, consequently, its behavior is completely determined by the chemical cross-link network, which is the well-known fact [122]. Taking into account that for glassy epoxy polymers βn ≤ βT ≤ tn, one should assume incorrectness of the latter conclusion for them and general regulation of their behavior by the totality of three structural components: cluster network (local order zones), packless matrix and partly (at high D) chemical cross-link network (topological structure level).

Figure 32. Dependence of index βt on the fractal dimensionality D of the chain segment between clusters for EP-1 (1), EP-2 (2), and EP-3 (3). Horizontal dashed lines indicate βn (4) and νn (5) values for the percolation cluster [117]

As a consequence, the above-discussed results indicate that the structure of polymer networks can be simulated by a thermal cluster. Hence, correspondence between thermal and percolation clusters, expressed by the equality of critical indices of the orientation parameter βТ = βn, is reached for quasi-equilibrium state of the polymer structure only. Actually, βТ value is the function of molecular

56

G. V. Kozlov and G. E. Zaikov

mobility, characterized by the fractal dimensionality (D) of the chain segment between clusters [117]. Some other important points should be noted, associated with the possibility of describing the polymer structure in the framework of equation (72). For the "rigidity segment", the statistical segment with the length lst, is accepted in the cluster model. The value of lst is several times lower than the Kuhn segment length, A, which characterizes rigidity of freely joint chain [60]. Selection of A as the “rigidity segment” mostly gives ϕcl above the unit, which is physically meaningless. The following correlation binds parameters lst and A [60]: lst = Acos(θ/2),

(79)

where θ is the valence angle. Thus shorter length of the chain “rigidity segment”, lst, in the glassy state is caused by conformational restructurings typical of this state [9]. For amorphous-crystalline polymers, reduced relative part of clusters,

ϕ clr , is

used. It characterizes this parameter in relation to the entire volume of the polymer, but not its amorphous phase exclusively [123, 124]:

ϕ clr =

ϕ cl 1− K

,

(80)

where K is the crystallinity degree. Thus for amorphous-crystalline polymers, the equation (5.72) can be reduced to the form as follows [9]:

ϕ cl ~ (1 − K )(Tg − T )βT .

(81)

Figure 33 shows correlation between Df and ϕp.m. for three polymers. Clearly at ϕp.m. = 0 the value of Df does not approach its border value equal 2.0 [5], 0

namely, d f value, which is different for different polymers. Obviously, this is the minimum of Df that can be reached for current polymers. The equation (42) binding parameters Df and С∞ and gives Df values close to the minimum. Table 3 T

0

shows comparison of d f values, calculated by the equation (42), and d f (Figure 33), which indicate their good conformity. Since the equation (42) gives

Cluster Structure as a Percolation System

57

the better correspondence to the experiment, the closer the polymer structure 0

approaches thermodynamic equilibrium [41], dimensionality of d f characterizes some quasi-equilibrium state of the structure. As follows from this equation, Df = 2 can be approached for polymers possessing С∞ = 2, i.e. for chains with 0

T

tetrahedral valence angle [60]. Thus substitution of d f or d f into equation (5) or (7) can help in the local order assessment,

ϕ cl0 , maximum approachable for the

current polymer, as the function of С∞ and S, the most important characteristics of the polymer. As temperature decreases below the point, at which

ϕ cl0 is

approached, the local order remains unchanged, so this temperature T0 can be assumed to be the analogue of Т∞, at which the polymer reaches constant free volume level [125]. In its turn, this temperature can be determined from the equation (42) under the condition ϕcl =

ϕ cl0 . The values of T0 and Т∞, obtained in

this manner [125], are compared in Table 4.

Figure 33. Dependencies of the structure fractal dimensionality, df, on the relative part of packless matrix, ϕp.m., for PC (1), PMMA (2) and HDPE (3) [9]

Good conformity was obtained for all polymers, except for PC, for which calculation by the equation (42) gave physically meaningless ΔТ ≈ 670 K. The reason for this seeming non-correspondence is as follows. Previously [5], the notion of quasi-equilibrium state of the polymer structure was introduced, to which Df ≈ 2.5 is corresponded. For real polymers, the tendency of transition to thermodynamically more equilibrium state (i.e. in the state with higher local order degree, ϕcl) at a definite stage must be balanced by entropic chain straining forces.

58

G. V. Kozlov and G. E. Zaikov

To put it differently, for the majority of polymers thermodynamic balance by means of the local orientation cannot be reached. That is why Df = 2.5 instead of T

theoretical value d f should be used. Moreover, data from Figure 33 indicate that the value ϕp.m. = 1.0 (i.e. ϕcl = 0) is approached at Df = 2.92, but not at Df = 3 as suggested by the equation (5). With respect to these adjustments, calculation by the equation (42) gives T0 = 318 K for PC that properly correlates with T∞ = 323 K (Table 4).

( ) T

Table 3. Critical fractal dimensionalities of polymer structures: d f , 0

calculated by equation (42), and d f , estimated from graphs in Figure 33 [9] Polymer

(d ) T f

d 0f

2.83 2.82 2.58 2.29

2.66 2.50 2.51 2.31

Poly(methyl methacrylate) Polyethylene Epoxy polymer Polycarbonate

Table.4. Transition temperatures to “frozen” free volume (Т∞) and structure (Т0) [9] Polymer Poly(ethylene terephthalate) Polyamide-6 Polyethylene Polypropylene Polystyrene Poly(methyl methacrylate) Polyvinylchloride Polycarbonate

ϕ cl0

Т∞ , K

Т0, K

0.24 0.14 0.10 0.24 0.23 0.36 0.17 1.0 0.36

280 277 227 227 324 290 270 323

300 304 243 199 320 269 333 − 318

It is known [126] that the fluctuation glass transition theory assumes the following temperature dependence of the characteristic length of cooperatively restructured zones (CRZ), ξА:

Cluster Structure as a Percolation System

ξA ~ (T – T0)2/3,

59 (82)

where T0 is the Foegel temperature in the VLF equation. Actually, the relation (82) is the percolation one or, more exactly with respect to the above discussion, the thermal cluster model relation. ξA value is equivalent to the local order diameter, Dcl. That is why Figure 34 shows the dependence Dcl(Тg – Т) plotted in double logarithmic coordinates, corresponded to the relation (5.82) (under the condition ξА = Dcl and Т0 = Тg) for the initial PC and the one, annealed at 393 K during 6 hours [127]. Clearly in both cases dependencies of lnDcl on ln(Tg – T) were found linear, i.e. are described by the relation (82), by the slope of this dependence is lower than that for annealed PC [128]. Thus the index in the relation (82) is smaller for annealed PC compared with the initial one. It is known [127, 129] that annealing of amorphous polymers shifts their structure towards thermodynamically higher balanced state. As a consequence, data in Figure 34 allow an assumption about connection between the index in the relation (82) with the polymer structure thermodynamic state: the more unbalanced the structure is, the higher the index is [128].

Figure 34. Dependencies of the cluster diameter, Dcl, on temperature difference (Tg – T) in double logarithmic coordinates, corresponded to the relation (82), for initial (1) and annealed (2) PC [128]

For a hypothetical polymer existing in the quasi-equilibrium state, Dcl can be estimated with the help of the above-mentioned thermal cluster model, namely, by the equation (74) at βТ = 0.40. Figure 35 shows temperature dependencies of Dcl for three types of PC polymer: initial, annealed and existing in a hypothetical quasi-equilibrium state. Clearly linear correlations of Dcl(T) conforming with ref. [126] are observed for all three cases. However, the slope of linear graphs is

60

G. V. Kozlov and G. E. Zaikov

decreased with the approach of the polymer structure to thermodynamic equilibrium: from initial (0.63) to hypothetical (0.47) PC. Discussed below are data from the work [126], which indicate that though linear decrease of ξА with temperature responds to Adams and Gibbs theory [130], the slope of these dependencies is much higher than that forecasted theoretically: by three times, approximately, for PMMA and by 6 times for PS. For one of the possible reasons for this deviation (Bittrich, [126]) the nonequilibrium origin of heat fluctuations is assumed. The above-obtained results on PC allow more exact explanation of this deviation.

Figure 35. Temperature dependencies of the cluster diameter, Dcl, for PC: initial (1), annealed (2) and existing in a quasi-equilibrium state (3) [128]

Figure 36 compares of temperature dependencies of ξА in accordance with the data from [126] and Dcl, calculated for the hypothetical quasi-equilibrium state for PMMA and PS structures. Clearly the slope of Dcl(Т) dependencies is much smaller than for ξА(Т): by three times, approximately, for PMMA and by 3.5 times for PS. This approximately conforms to the deviation in slopes of theoretical and experimental ξА(Т) dependencies for the mentioned polymers, obtained in the work [126]. As a consequence, the above results indicate that the thermal cluster model correctly describe both structure of the entire amorphous polymer and its basic element (cluster) separately that might be expected due to thermofluctuation origin. Moreover, the cluster model is more general than the fluctuation glass transition theory, because it allows correct theoretical calculation of structural parameters both in thermodynamically non-equilibrium and quasi-equilibrium states, whereas Adams and Gibbs theory allows it for the latter case only [128].

Cluster Structure as a Percolation System

61

Figure 36. Temperature dependencies of CRZ characteristic length, ξА, (1, 2) and cluster diameter, Dcl, for quasi-equilibrium state (3, 4) for PMMA (1, 3) and PS (2, 4) [128]

Chapter 6

CLUSTER MODEL AS THE MODEL OF IRREVERSIBLE AGGREGATION In 1981, Witten and Sander developed the model of the particle-cluster (P-Cl) diffusion-limited aggregation (DLA) [131]. Imagine a particle present in space. Another particle making the Brownian motion appears remote from the first one. Meeting the first particle, it adheres to it, the adhesion being irreversible. Then another particle appears in the distance, diffuses and touching the primary two particles adheres to them. This process is multiply repeated. Some particles do not touch the propagating cluster during random walk, but diffuse infinitely far from it. These particles are neglected from the future consideration. Such cluster is shown in Figure 37. It was obtained using computerized Monte-Carlo method. In this method, all the totality of events is simulated in detail (the Brownian motion is given by a random number generator). Particularities of computer simulation are discussed in the work [132]. The reason for formation of branched structures (refer to Figure 37) in the P-Cl DLA model is as follows. A particle walking randomly will most probably contact cluster branches first thus increasing its size. Therefore, the probability of its penetration inside the cluster that would cause formation of a compact structure with Df = D is infinitely low. Thus cluster branches shield the internal structure of it, somewhat freezing it. As mentioned above [133], propagation of such a cluster should be considered as the phase transition between finite and infinite clusters. This formalization allows comparison of the P-Cl DLA model with others which simulate formation of an infinite system (a polymer gel). Mikin [132] has performed computerized simulation of P-Cl DLA for the case of D = 2 - 6. As

64

G. V. Kozlov and G. E. Zaikov

detected, the fractal (Hausdorff) dimensionality Df ≈ 2.5 for the Witten-Sander cluster with D = 3.

Figure 37. Two-dimensional Witten-Sander cluster composed of 11,260 particles. The adhesion coefficient (steric factor) p = 1 [132]

As indicated [8], the Witten-Sander (WS) P-Cl DLA model allows description of a great number of real physical processes and structures formed by them. Computer simulation gives an opportunity, at least, to determine the tendencies in structure variation of final aggregates under the effect of one or another factor, which is of importance for WS model application to description of the real objects. Nevertheless, under consideration of the latter computerized simulation schemes require clear physical particularization in relation to structure of the studied object. Advantages of the description of one or another process (aggregate) in the framework of P-Cl DLA model (or other aggregation models [8]) are obvious. If the cluster model of the polymer amorphous state structure can be described as WS cluster, this means their belonging to the same class of universality of physical events. Remind that the essence of the universality hypothesis is the following: if the same limiting conditions (interactions between system components) are typical of different systems, these systems belong to the same class of universality of physical events [133]. The more so this means that the polymer amorphous state structure belongs to much broader class of physical events, but not represents something isolated from other braches of physics. In

Cluster Model as the Model of Irreversible Aggregation

65

this case, it is subordinate to the general regularities of systems from the current universality class that proves theoretically the description of modern physical concepts within its framework, and the universality class is characterized by a definite selection of scaling indices [133]. It has been shown on this basis [134] that model presentations of WS clusters allow description of polymer network structures using the same scaling index, for which the fractal (Hausdorff’s) dimensionality is taken. There are many reasons (one of which is the cluster appearance, Figure 3) for association of the polymer amorphous structure in the framework of the cluster model and WS cluster. Here are three of them. The first is correspondence of the scaling index (fractal dimensionality, Df) in both models [67, 131]. The second reason is the well-known fact [135] that transition from one universality class to another is observed in the gel formation point, e.g. from cluster-cluster (Cl-Cl) to P-Cl DLA. This means that after the gel formation point the polymer represents the WS cluster. Finally, the third reason is the mechanism of local order zone formation in the cluster model. It is indicated [89] that detachment of a single segment from such zone means formation of one microcavity of fluctuation free volume, whereas addition of a segment induces “implosion” of the microcavity. In the framework of DLA model such mechanism can be identified with P-Cl aggregation that, besides Df parameter, is the basic characteristic of this class of universality [133]. Note also that the meaning of the “cluster” term in models [34] and [131] are different. In the WS model by the cluster both the local order zone (or close packing zone [136]) and chains (branches) coming out of it are meant. In the cluster model by “cluster” statistical segments only participating in the local order zone are meant. Obviously, the polymer sample structure should not be considered as WS cluster, because in such scales it represents the Euclidean object. That is why by analogy with the modified WS model [137], the polymer network structure was associated [134] with a selection of WS clusters, where every cluster is sized about 2Rcl. In accordance with the model [137] WS cluster propagation is realized on a great number of “seedings”, and Rcl parameter is bound to concentration of freely diffusing particles, c, by the following equation [137]: d −d

c = Rcl f

.

(83)

Let us discuss the physical meaning of parameter c. Figure 3 indicates that the only statistical segments of the macromolecule have the opportunity to be added

66

G. V. Kozlov and G. E. Zaikov

to the local order zone, which exist in the packless matrix. Thus c decreases with the local order, and under the condition Rcl = const this means decrease of (Df – D) or Df. Parameter c value was accepted as multiplication of the number of particles (statistical segments) per specific volume and relative part of the packless matrix. Figure 38 shows comparison of the fractal dependencies of EP e

t

structure, d f [63], and WS cluster, d f , calculated by the equation (83). The e

t

data in this Figure indicate good conformity of d f and d f values. As a consequence, modified P-Cl DLA aggregation model [137] gives good description of the polymer network structure using the expected scaling indices Df. This allows belonging of the polymer network structure to the mentioned universality class of physical systems and describes its properties in the framework of this class of relations [134]. Basically, cluster growth is induced by diffusive aggregation of particles, whereas under the stationary mode (cr = const) the following correlation is valid [138]:

c dR ~ KR , K = dr , dt R f

(84)

where t is time; cr is the rate of particle delivery to the propagation zone; R is the typical linear size of the cluster.

Figure 38. Dependencies of structure fractal dimensionalities, experimentally determined

d ef

(1, 2) and calculated by the equation (83)

Kst, for EP-1 (1, 3) and EP-2 (3, 4) [134]

d tf

, on the curing agent:oligomer relation,

Cluster Model as the Model of Irreversible Aggregation

67

If lst is accepted for R, the correlation (84) can be transformed to the following form [39]:

d ⎛⎜ l st f ⎞⎟ ⎠ ~ cr , ⎝ d −1 d T −1 l st f d

( )

(85)

where T is the cluster formation temperature. d

( ) −1

Figure 39 shows l st f T dependencies, calculated in the above-described manner, for two amorphous glassy polymers (PC and PAr). Clearly the plots show that the assumed correlation does exist, and its nonlinearity is caused by the d f −1

presence of l st term in the right part of equation (85). This means that for glassy amorphous polymers, aggregation of segments into clusters is caused by its d

( ) graphs means decrease of the

f diffusion mechanism. Curvature of l st T

−1

defect generation rate with temperature, and linearity of correlations l st (T ) , shown in Figure 40, proves this conclusion followed from consideration of the correlation (85). df

df

Figure 39. Dependencies of parameter l st [39]

on reverse temperature for PC (1) and PAr (2)

68

G. V. Kozlov and G. E. Zaikov

Power-series size distribution of objects is widely spread in the nature. Some examples of the power-series correlation between the number, N, and size, r, of defects are shown in the work [138]. General form of the correlation is as follows: N(r) ~ r-α,

(86)

where α is a constant.

d f −1

l Figure 40. Dependencies of parameter st [39]

on test temperature T for PC (1) and PAr (2)

Figure 41 shows the dependence νcl(lst) in double logarithmic coordinates for 16 polymers of different classes that corresponds to the correlation (86). This dependence is linear, which is typical fractal behavior proving the abovementioned results [39]. For the cluster WS, the following correlation characterizing variation of its density, ρWS, with the cluster radius, RWS, and fractal dimensionality, Df, is presented [136]:

⎛ RWS ⎞ ⎟ ⎝ a ⎠

ρWS = ρ c. p. ⎜

d f −d

,

(87)

where ρc.p. is the substance density in closely packed WS cluster; a is the lower border of WS cluster fractal behavior.

Cluster Model as the Model of Irreversible Aggregation

69

Figure 41. Dependence of entanglement cluster network frequency, νcl, on the length of statistical segment, lst, in double logarithmic coordinates for amorphous (1) and amorphous-crystalline (2) polymers and polymer networks (3) [39]

Let us consider equation (87) in more detail. For WS cluster, correlations Df < D and ρWS < ρc.p. (change of signs in these two inequalities by the equality sign means cluster transition to another universality class, for example, transition to the Iden cluster [133]) are determined by the condition a < RWS. At the same time, since ρWS ≠ 0 and ρc.p. ≠ 0, a cannot equal zero. Thus a compact zone (Df ≈ D) sized a does always exist in the center of WS cluster. For the polymer amorphous state structure, this compact zone is identified as the local order zone (Figure 3). This circumstance is one of the conditions of WS cluster existence [139]. Two remarks should be presented on this point. Firstly, the reason for formation of the compact zone on primary stages of WS cluster formation is easy for understanding. The fractal origin of WS cluster is determined by the screening effect of its “branches” preventing access of particles to internal cluster zones [139, 140]. However, on the primary propagation stages these “branches” are low developed, and their screening effect is also low. Secondly, the structure of polymers, as any real (physical) fractal, possesses fractal properties in a definite range of linear scales only [14]. Thus, identification of the polymer amorphous state structure as WS cluster (or, more exactly, the totality of huge amount of clusters) and the necessary existence of local order zones in the amorphous state [141]. This conclusion has been confirmed [141] by results of a value comparison in accordance with the equation (87) and sizes of the local order zones, rc.p. shown in Figure 42. For ρWS, density of the polymer packless matrix was accepted that coincides with the polymer density above Tg [93]; for ρc.p., density of crystalline zones in PC and HDPE are accepted [142, 143]. As indicated by data from Figure 42, both absolute values and tendencies of temperature variations of rc.p. and а

70

G. V. Kozlov and G. E. Zaikov

parameters display good conformity. A definite spread in a values in relation to rc.p. is induced by inaccuracy of Df assessment due to power-series dependence of a on Df (equation (87)) that causes a significant effect of the comparison accuracy. Data from Figure 42 prove the above assumption about local order zones’ necessary existence in the structure of the polymer amorphous state [141].

Figure 42. Temperature dependencies of sizes of local order zones rc.p. (1) in the model [34] and compact zones a (2) in the model [131, 139] for PC (a) and HDPE (b) [141]

As mentioned above, one of the advantages of WS model application to simulation of the polymer amorphous state structure is its thoroughly developed theoretical basis, proved by great number of computerized simulations. WS cluster growth on many “seedings” and their interaction are discussed in detail in [137]. In the framework of this model, on the example of PC and PAr, temperature variations of the structure fractal dimensionalities, Df, and the chain segment between entanglements, D, were forecasted. Two alternatives of WS cluster growth on many “seedings” (models A and B) were considered [137]. These models are thoroughly described in the works [8, 137]. Here it should be mentioned that the model A possesses two alternatives, too: with low and high −d

seeding concentrations, c0, the border between which is the concentration Rc

,

where Rc is the critical (border) radius of the WS cluster. The border value c0, calculated in this manner, was found equal 3.36×1025 and 6.40×1025 m−3 for PC and PAr polymers, respectively [144]. Let us consider physical interpretation of “seedings” for the case of the polymer amorphous state. In accordance with the model [145], an avalanche-like formation and “freezing” of local order zones proceed with temperature, T > Tg, at transition over Tg. These very local order zones are the basic structural feature of glassy polymers [34, 90]. At T > Tg macromolecular “hookings” and short-living

Cluster Model as the Model of Irreversible Aggregation

71

local order zones exclusively exist in the polymer structure [125]. As shown above, the "frozen" local order zones represent the central oriented part of the WS cluster in relation to the polymer amorphous state structure. That is why, essentially, in the case under consideration, the only candidates for the role of “seedings” are macromolecular “hookings” [144]. For the polymers under consideration, the “hooking” network frequency equals, approximately, the magnitude of 1027 m−3, more precisely, 7×1026 m−3 [112]. Thus in this case, the −d

frequency of “seedings”, c0, is greater than Rc

, and WS cluster propagation is −d f

terminated, when the amount of initial diffusing particles becomes equal Rc [137]. Analytically, this condition is expressed as follows [133]: d −d

c = Rc f

.

(88)

As before, for diffusing particles a statistical segment is accepted. In this case, c value equals [144]:

c=

1 L = , l st Sl 0 C ∞

(89)

where L is total length of macromolecules per specific polymer volume. For PC and PAr polymers, calculation of parameter Df by the equation (88) gives good conformity to experimental results [144]. As shown in Chapter 2, injection of relatively low concentrations (~ 0.01 – 1.0 wt.%) of highly disperse Fe/FeO (Z) mixture into HDPE causes significant changes in the structure and properties of HDPE + Z composites [146]. It is also indicated [146] that these effects are stipulated by formation of local order zones (clusters) by local magnetic fields of superparamagnetic domains Z. Thus Z domains represent somewhat “seedings” for amorphous phase structure formation in HDPE + Z. In its turn, this affects the structure of crystalline and interphase zones in HDPE + Z during their formation from melt. That is why the method different from the above-described one was suggested for determination of the “seedings” density, c0 [147]. Accepting in the first approximation for HDPE that Rc = 50 Å [147], the border “seeding” concentration equal ~0.8×1025 m−3 is obtained. In a natural polymer, the “seeding” density must equal the amount of clusters per specific polymer volume, Ncl, determined by the following relation: 2νcl/F [144].

72

G. V. Kozlov and G. E. Zaikov

Figure 43. Dependence of the “seeding” density, c0, on Z concentration, CZ, for HDPE + Z composites. The dashed line shows frequency of macromolecular “hooking” network for HDPE [147]

Figure 43 shows the dependence с0(Ncl) at Z concentration, CZ, for HDPE + Z composites. Dashed line in the Figure shows frequency of macromolecular “hooking” network, νh, calculated in the work [148]. Clearly the dependence с0(CZ) is of clear extreme type, corresponded to the type pf HDPE + Z composite properties variation [146]. At CZ = 0.05 wt.%, the number of “seedings” by, approximately, 2.5-fold exceeds their concentration for unmodified HDPE. For HDPE and HDPE + Z composites with CZ ≥ 0.10 wt.%, the value of νh parameter is approximately equal c0. Thus data from Figure 5.43 induce an assumption that previously detected extreme variation of HDPE + Z composite properties in CZ range of 0.01 – 0.10 wt.% is induced by the same change of the “seeding” density. In the rest cases, e.g. when Z particles do not form superparamagnetic domains, с0 = νh. Assessment of the structure change induced by c0 variation can be performed in the framework of the above-described WS model [137]. Since the minimal value of c0 (Figure 43) is, approximately, five-fold higher than the border concentration of “seedings”, the alternative of high “seedings” concentration (alternative A [137]), the basic correlation of which is equation (88), was used for assessment of structural changes [147]. Figure 44 shows comparison of fractal dimensionalities, Df, of HDPE + Z composite structure, calculated by equations (4) and (88). Clearly good correspondence by run of Df concentration dependence and absolute values of this parameter (maximal deviation does not exceed 1.5%) was obtained. The number of particles (statistical segments), nseg, in the central closely packed zone of WS cluster can be determined by the following equation [119]:

Cluster Model as the Model of Irreversible Aggregation

73

12

Rcl ⎛ n seg S ⎞ ⎟ = ⎜⎜ ⎟ 2 ⎝ πϕ cl ⎠

(90)

in accordance with equation (90) (under the condition F = 2nseg), i.e. in accordance with the cluster model of the polymer amorphous state structure and WS model, respectively. Both good qualitative and quantitative conformity is obtained again.

Figure 44. Comparison of fractal dimensionalities, df, of the structure, calculated by equations (4) (1) and (88) (2) as the function of CZ for HDPE + Z composites [147]

Figure 45. Comparison of local order zone functionality, F, calculated by equation (90) (2) as the function of Z concentration, CZ, for HDPE + Z composites [147]

As a consequence, the results have displayed [147] that besides molecular parameters S and С∞, “seeding” density, c0, is one more the important factor determining structure of the polymer amorphous state. It should be noted that the

74

G. V. Kozlov and G. E. Zaikov

crystallinity degree is the function of Df and, consequently, c0, too [123, 124]. Application of modified WS model gives an opportunity of forecasting the structure of polymers as the function of density of artificially injected “seedings” (Z in the present case) or frequency of macromolecular “hookings” [144] (chemical cross-links [134]). The energy of intermolecular interaction characterized either by molar cohesive energy, Ec, or cohesive energy density, Wc, is (besides the glass transition temperature, Tg) one of the most important characteristics of the polymer condensed state [149]. However, at present, correlations of these parameters with polymer properties are usually considered [150, 151], and there is no description of Ec (or Wc) effect on the polymer structure, though such influence is assumed quite frequently [149, 152]. Using the above-discussed models, the effect of cohesive parameters on amorphous polymer structure formation was cleared out on the example of two heterochain polyesters [153, 154]: aromatic copolyester sulfone formals (APESF) and 2,2-di-(4-oxyphenyl)propane oligoformal, phenolphthalein and isophthalic dichloranhydride (SP-OFD-10/F-1) diblock-copolyesters. Molar cohesion, Ec, can be estimated by the following equation [149]:

Tg = Tg 0

2 RTg20 n Ec

,

(91)

where Tg is the glass transition temperature of copolymer; Tg0 is the glass transition temperature of more rigid-chain component (polysulfone (PSF) for APESF and polyarylate (PAr) for SP-OFD-10/F-1); n is the part of more flexiblechain component (polyformal) in block-copolymer. However, in the framework of models applied to description of the polymer structure characteristics calculated per specific volume of the polymer are used. That is why to obtain correct correlations between cohesive characteristics and parameters of the structure, the use of density of cohesive energy, Wc, possessing “energy/volume” dimensionality (usually, MJ/m3) instead of Ec is required [155]. Figure 46 shows Wc dependencies on the composition of copolyesters, namely, on concentration of rigid blocks (PSF or PAr: CPSF and CPAr, respectively) in them. The data shown indicate that increase of rigid-chain component concentration leads to Wc increase. As a rule, such correlations are explained by formation of domains from closely packed segments in the polymer structure [149, 152]. Figure 47 shows dependencies of Tg on the formal block concentration, Cform, comparison of which with the data from Figure 46 gives

Cluster Model as the Model of Irreversible Aggregation

75

interesting results. It is known [156] that disposition of Tg dependencies with respect to composition of copolymers allows identification of their type. For example, for APESF, dependence Тg(Сform) is located above the additive glass ad

transition temperature, Tg . That is why for this polymer a tendency to regular ad

alternation of units shall be expected. For SP-OFD-10/F-1, Тg < Tg , i.e. the copolymer is inclined to formation of long sequences of the same blocks [156]. Nevertheless, for both these copolymers dependencies of Wc on composition occur beneath the appropriate additive dependence. This circumstance induces two conclusions. Firstly, in contrast with Tg dependencies on composition, the shape of analogous Wc dependence is independent of the type of copolymer. Secondly, Tg and Wc values characterize different properties of copolymers, though interdependent ones. For example, Tg is determined by rigidity of the polymer chain [157], and Wc by intensity of intermolecular interactions. In this connection, of interest is comparison of two polymers: polyamide-6 and polyvinylchloride, for which Tg are approximately equal (~323 and 343 K, respectively [155]). This is caused by approximately equal flexibility of their chains, determined by characteristic relation С∞ (6.2 and 6.7, respectively [45, 53]). However, Wc values for these polymers differ by two times (783 and 389 MJ/m3, respectively [155]).

Figure 46. Dependencies of cohesive energy density, Wc, on concentration of rigid-chain blocks, CPSF for APESF (1) and CPAr for SP-OFD-10/F-1 (2) [153]

76

G. V. Kozlov and G. E. Zaikov

Figure 47. Dependencies of the glass transition temperature, Tg, on formal block concentration, Cform, for APESF (1) and SP-OFD-10/F-1 (2) [153]

Figure 48. Correlation between cohesive energy density, Wc, and glass transition temperature, Tg, for APESF (1) and SP-OFD-10/F-1 (2) [153]

Nevertheless, correlation between Tg and cohesive characteristics are known well [158], which is explained by the above-mentioned interdependence of these parameters (refer to equation (91)). Simultaneously, the increase of the polymer chain rigidity with Tg promotes formation of closely packed domains that increases Wc (or Ec) [152]. Figure 48 shows correlation Wc(Тg) for APESF and SP-OFD-10/F-1, which is linear and reflects the above-considered interrelation. Since all data were obtained at T = 293 K, extrapolation of linear dependence Wc(Тg) to Tg = 293 K means polymer transition to devitrified state, and at this temperature Wc = 0 (anyway, in the scale of Figure 48). Broad dispersion usually observed for such correlations is caused by the fact that Тg and Wc (or Ec)

Cluster Model as the Model of Irreversible Aggregation

77

characterize different polymer properties that follows from comparison of data from Figures 46 and 47.

Figure 49. Correlation between relative part of clusters, ϕcl, and cohesive energy density, Wc, for APESF (1), SP-OFD-10/F-1 (2), PC (3), and HDPE (4) [153]

The effect of attraction and repulsion forces between particles forming WS cluster on its structure was studied [159]. It is shown that attraction force increase makes the cluster, more precisely, its external zones more packless. This aspect of amorphous polymer structure formation can also be considered in the framework of the cluster model [8]. Figure 49 shows dependence ϕcl(Wc) for APESF and SP-OFD-10/F-1. Expectedly, Wc or intermolecular attraction force intensification causes increase of the relative part of closely packed local order zones in the structure of copolymers. Data in the Figure on PC and HDPE [5] conform to ϕc(Wc) correlation, obtained for copolymers under consideration. This indicates quite high generality of the correlation [8]. Figure 50 shows dependencies of WS cluster density, ρfr (equation (2)) on the relative part of packless matrix, ρp.m., for APESF and SP-OFD-10/F-1, which indicate ρfr increase with ρp.m., i.e. ϕcl or Wc decreased (Figure 49). Thus similar to computerized simulation [159], attraction forces increase between particles (statistical segments), characterized by Wc increase, induces higher loosening (ρfr decrease) of external zones in WS clusters, identified as the packless matrix [154]. Note also that at Tg relative free volume, ff, increases with the polymer chain rigidity (or Wc, refer to Figure 48) [95]. Clearly Wc increase induces ϕcl growth (Figure 49) and ρp.m. decrease (Figure 50) and consequently, ff increase. Thus application of the WS model does also explain this feature of amorphous polymer structure [154].

78

G. V. Kozlov and G. E. Zaikov

Figure 50. Dependencies of WS cluster density, ρfr, determined by equation (2) (1, 2) and packless matrix density, ρp.m., determined by equation (92), on the relative part of packless matrix, ϕp.m., for APESF (1, 3) and SP-OFD-10/F-1 (2) [154]

Free particles are used in computerized simulation of WS clusters, whereas the principal difference of the polymer structure is linking of statistical segments forming it to the chain by strong covalent bonds. This restricts their motion. That is why ϕcl and ϕp.m. variations can be accompanied by redistribution of frequencies of these structural components only. This effect can be estimated using simple rule of mixtures:

ρ = ρclϕcl + ρp.m.ϕp.m.,

(92)

where ρ is the polymer density; ρcl and ρp.m. are densities of clusters and the packless matrix, respectively. Taking for ρ experimentally determined densities of copolyesters and assuming ρcl = 1.08ρ [142], one can estimate ρp.m. variation with ϕp.m., (under the assumption that ρfr ~ ρp.m.). Figure 50 shows the dependence ρp.m.(ϕp.m.), which can be coincident with the correlation ρfr(ϕp.m.) by simple adjustment of the scale, because ρfr values are given in relative units. Thus application of the WS model gives quite full picture of intermolecular interaction forces effect on formation of the amorphous polymer structure. The increase of Wc characterizing intensity of intermolecular attraction forces induces growth of the local order degree, ϕcl. This effect is accompanied by loosening of the packless matrix by means of segments redistribution in structural components of the amorphous polymer [154].

Cluster Model as the Model of Irreversible Aggregation

79

It has been shown [131] that autocorrelation function: c(r) = (p(r′)⋅p(r′ + r)),

(93)

where р(r′) and р(r′ + r) are probabilities of the presence of particles, from which the cluster is composed (the probability equals 1 in the presence and 0 in the absence of the particle), in points r′ and r′ + r, can be presented by the following scaling relation: с(r) ~ r−α,

(94)

for distances r greater than several steps of the lattice. In the relation (94), α is determined by the difference as follows [139]:

α = D − Df.

(95)

As a consequence, by determining the slope, α, of linear autocorrelation function, one can estimate the fractal dimensionality of the object, Df, using relations (94) and (95) [160]. Figure 51 shows schematic presentation of the autocorrelation function for the structure of amorphous polymer. Here variation of density is presented by the function of distance, r, and the origin of coordinates (r = 0) is disposed in the center of the local order zone (refer to Figures 2 and 3). In some interval from 0 to rlz (where rlz is the radius of the local order zone) parameter ρ is constant and equals density of the local order zone, which in the first approximation is accepted equal the appropriate ρcr value for crystalline polymer (particularly, for PC [160]). Then in the interval from rlz to Rcl a linear decrease of ρ to some ρmin value is assumed, assessed as follows. The average density of amorphous PC, ρа, was calculated [142], corresponded to the middle of the sloped linear part of ρ(r) dependence in Figure 51.Then basing on simple geometrical ideas, one may obtain the following [160]:

ρmin = ρа – (ρcr − ρа).

(96)

Further on, parameter α can be assessed from the following correlation [160]: (ρcr − ρmin) ~ (Rcl – rlz)−α,

(97)

80

G. V. Kozlov and G. E. Zaikov

and then Df value by equation (95) can be calculated. Figure 52 shows comparison of temperature dependencies of the fractal dimensionality values of PC structure:

( ) calculated by the equation (4) and theoretical ones within the framework of the model suggested (d ) calculated by equations (95) e

experimental values d f

t f

and (97).

Figure 51. Schematic presentation of the function ρ(r) for amorphous polymer [160]

Clearly good conformity between theoretical and experimental results is observed (deviation below 10%). However, this conformity can be improved e

using the following methodological method. To assess d f in accordance with the equation (4), ν parameter was determined from the equation (12). If in this equation the real yield stress,

σ yr , estimated as follows, is used instead of

technical one, σy, [59]:

σ yr = σy(1 + εy),

(98)

where εy is the yield deformation, somewhat lower ν value will be obtained. Data in Figure 52 indicate that the adjustment gives much better conformity between

d ef and d tf for PC. For PC also at T = 293 K Df value was determined [67] by five different methods that gave, on average, Df = 2.51. This result conforms well to Df value at T = 293 K, obtained in the framework of the WS model (Df = 2.56, Figure 53) [160].

Cluster Model as the Model of Irreversible Aggregation

81

Figure 52. Dependence of fractal dimensionality, df, of PC structure on test temperature, T. r Calculation was performed by equation (4) using σy (1) and σ y (2); by equations (95) and (97) (3) [160]

Figure 53. Dependence of steric factor, p, on cross-linking frequency, νс, for EP-2 (1) and EP-3 (2) [162]

As observed in the framework of computerized simulation of DLA clusters, the steric factor p (р ≤ 1) indicating that not all collisions of particles happen with orientation necessary for particle “adhesion” to the cluster plays the important role basically defining the aggregation mechanism and structure of the final aggregate, characterized by its fractal dimensionality, Df [159, 161]. For example, at high p approaching 1 the diffusion-limited mechanism of the aggregate propagation with relatively low values Df is realized. On this basis an attempt was made [162] to clear out the effect of cross-linking frequency, νс, on p and conditions of local order zone formation for polymer networks, EP-2 and EP-3. For WS clusters, one can write down as follows [133]:

82

G. V. Kozlov and G. E. Zaikov

p~

1 , rlz

(99)

The proportionality factor in the correlation (99) can be approximately assessed as follows. The distance between chemical cross-link points, Rc, was calculated and then the proportionality factor was determined from the correlation (99) under the condition rlz = Rc and the appropriate minimal value p = 0.1. Figure 53 shows dependence р(νс), found linear. Clearly νс increase leads to p growth, which is accompanied by Df decrease [68]. This conforms to general statements of the model [161]. There are data [163, 164] displaying that νс increase induces cluster network frequency increase, νсl, and decrease of the number of segments, nseg, in a single cluster. This means formation of a large number of small clusters, Ncl (= νcl/nseg). Figure 54 shows dependence Ncl(р) that indicates linear increase of Ncl with p (or νс, refer to Figure 53). However, dependence Ncl(р) does not pass through the origin of coordinates, and at Ncl = 0 value of p is finite and equals ~0.215. This means that at р ≤ 0.215 the cluster network is not formed or, to put it differently, polymer network does not transit to the glassy state. Figure 53 indicates that p = 0.215 corresponds to νс = 2.2×1026 m−3, and at νс below the mentioned value the cross-linkable polymer does not transit to the condensed state. The critical value

( )

ν c ν ccr can also be estimated

theoretically. The condition Ncl = 0 and, consequently, νcl = 0 is the criterion of polymer transition to the rubbery state [121]. For such state, fractal dimensionality D of a part of chain between cross-link points that characterizes molecular mobility equals 2 [120]. Moreover, for the series of epoxy polymers under consideration, the maximum of С∞ (at the minimum of νс) equals 4.8 [165]. This allows determination of maximal Df for epoxy polymers by equation (42) and then the number of segments, nseg, between chemical cross-link points by equation (56). In accordance with the relation (42) and at D = 2 and Df = 2.737, nseg = 23.3 was obtained from equation (56) and the chain length between cross-link points, Lc, was calculated by equation (57). After assessment of the total length of macromolecules, L, per specific volume of the polymer one can determine via L/Lc, whence it follows that

ν ccr

ν ccr = 2.1×1026 m−3. This theoretical value of

ν ccr conforms properly to the appropriate experimental one, graphically estimated from the data in Figure 54 (ν c = 2.2×1026 m−3). cr

Cluster Model as the Model of Irreversible Aggregation

83

Extrapolation of р(νс) curve (Figure 53) to the maximum p = 1 gives the maximum of νс

(ν ) equal ~26×10 max c

26

m−3. At this νс value the following fractal

dimensionalities shall be obtained: D = 1 and Df = 2 [5]. Under these conditions, nst = 2 from equation (56) and Lc = 12 Å from equation (57) are obtained. Then theoretical value of

ν cmax may be estimated as ~24.5×1026 m−3, which again

conforms well to the above experimental assessment. Moreover, the minimum of nst = 2 conforms completely to the analogous assessment for completely crosslinked polymers [125].

Figure 54. Dependence of the number of local order zones, Ncl, per specific volume of the polymer on steric factor, p, for EP-2 (1) and EP-3 (2) [162]

Thus the above-considered results indicate that chemical cross-link point frequency, νс, regulating conformation of the chain part between them determines the steric factor, p: the higher νс is, the greater p is. This means that νс increase forms the chain conformation favorable for statistical segments’ packing in the local order zone. Therefore, this circumstance determines formation of a large number of small clusters at high νс values [162]. In Section 5 the notion of quasi-equilibrium state of the polymer structure corresponded to the balance of tendencies to local order and entropic chain strain increase was introduced [9]. Generally, this state is characterized by Df = 2.5. It should be noted that at N → ∞ (where N is the number of particles in the cluster) this value of Df coincides with the fractal dimensionality of the WS cluster for three-dimensional space [132]. In contrast with the primary Witten-Sander model [131], in which WS cluster growth is unlimited (N → ∞), an interaction between WS clusters occurs in the modified simulation at multiple growth points [137],

84

G. V. Kozlov and G. E. Zaikov

and the condition of the process termination is obtained. That is why the conformity of quasi-equilibrium state formation conditions in cluster and WS models was considered [166]. Data from the literature for a series of amorphous and amorphous-crystalline polymers were considered [166]. For these polymers, the “seeding” density c0 = Ncl = 2νcl/F and macromolecular “hooking” network frequency, νh, were determined using Mh values from the literature [45, 53]. Figure 55 shows comparison of Ncl and νh values for 8 polymers under the strain and stress relaxation tests. Clearly quite good conformity of these parameters by both absolute values and the tendency of their variations was obtained. Quite broad dispersion is explained by corresponded deviation in Mh values from different literature sources, obtained for one and the same polymer (for example, for polyethylene Mh = 1,900 g/mol [53] and 1,390 g/mol [45], respectively). Nevertheless, Figure 55 indicates that the condition Ncl = νh allows identification of νl parameter as the “seeding” density [166].

Figure 55. Correlation between cluster density, Ncl, and macromolecular “hooking” network frequency, νh, for 8 amorphous and amorphous-crystalline polymers. The continuous line marks 1 : 1 ratio [166]

The simulation [137] assumes the presence of such parameter as the diffusion length, ξ, depended on the local environing of every “seeding”. Fractal propagation of WS cluster lasts until the condition ξ = Rc is reached [137]. Parameters ξ and Rc are bound to the concentration of free particles, c, as follows [137]: d −d + 2

ξ 2 = c −1 Rc f

.

(100)

Cluster Model as the Model of Irreversible Aggregation

85

Substituting the above condition of WS cluster termination into equation (100), the criterion (88) is obtained that gives concentration of free particles, c, at the moment of WS cluster termination, when it reaches radius Rc (hereinafter, cWS), or as in the framework of the WS model the quasi-equilibrium state is reached, because in this case, too, the structure invariance is determined by the balance of tendencies: diffusive propagation is limited by interaction of neighboring WS clusters [166]. In accordance with the relation (88) the use of dimensional Rc values induces cSW dependence on dimensionality of the length, selected for Rc. That is why for normalizing factor the lower scale of the fractal behavior (bl = 5 Å) was chosen [166], and dimensionless parameter (Rc/bl) was used in the equation (88). Selection of another bl value will change quantitative estimations of cSW insignificantly and is negligible for tendencies in their variations. In the framework of the cluster model (Figure 3), the ability to be added to the local order zone is inherent to the only segments, present in the packless matrix. As a consequence, in terms of the WS model these very segments represent free particles. That is why in the framework of the cluster model under reaching a quasi-equilibrium state, the concentration of the free particles, ccr, will equal the relative part of the packless matrix,

ϕ cr p.m. , in this state. This parameter was

calculated as follows. First, Df corresponded to the quasi-equilibrium state [41] was determined from the equation (42); sequentially, ϕcl and as (1 -

ϕ cr p.m. as (1 - ϕcl) (or

ϕ clmax ) for amorphous-crystalline polymers, equation (80)), which equals

ccr (see above) for the quasi-equilibrium state were determined from equation (7) [166]. Figure 56 gives comparison of cWS and ccr for 12 amorphous and amorphouscrystalline polymers. Clearly correspondence of these parameters indicating, in its turn, the conformity between interpretations of quasi-equilibrium states of the polymer structure in the cluster and WS models is observed. Somewhat overestimated cWS values over ccr are induced by arbitrary choice of bl value. Briefly resuming results of the present Chapter, note that the cluster model of the polymer amorphous state conforms both qualitatively and quantitatively to the modern physical concepts, which can be applied to description of the polymer structure. Applications of one or another alternative of the combined models allows significant expansion of the analytical abilities of the structure description and obtaining of principally new ideas on it.

86

G. V. Kozlov and G. E. Zaikov

Figure 56. Correlation between concentrations of free particles, cWS, and statistical segments in the packless matrix, ccr, for quasi-equilibrium states for 12 amorphous and amorphous-crystalline polymers. Dashed line marks 1 : 1 ratio [166]

REFERENCES [1] [2] [3] [4] [5] [6]

[7] [8] [9]

[10] [11] [12] [13] [14]

Feder J., Fractals, New York, Plenum Press, 1988, 254 p. Ivanova V.S., Balankin A.S., Bunin I.Zh., and Oksogoev A.A., Synergism And Fractals In The Material Science, 1994, Moscow, Nauka, 383 p. (Rus) Novokov V.U and Kozlov G.V., Uspekhi Khimii, 2000, vol. 69(4), pp. 378 393. (Rus) Novokov V.U and Kozlov G.V., Uspekhi Khimii, 2000, vol. 69(6), pp. 572 599. (Rus) Kozlov G.V. and Novikov V.U., Synergism And Fractal Analysis Of Polymer Networks, 1998, Moscow, Klassika, 112 p. (Rus) Novikov V.U. and Kozlov G.V., Analysis of Polymer Destruction In The Framework Of The Concept Of Fractals, 2001, Moscow, Izd. MGOU, 136 p. (Rus) Fractals And Local Order In Polymer Materials, Ed. G.V. Kozlov and G.E. Zaikov, 2001, New York, Nova Science Publishers. Inc., 190 p. Shogenov V.N. and Kozlov G.V., Fractal Clusters In Physicochemistry Of Polymers, 2002, Nalchik, Poligrafservis i T., 268 p. (Rus) Kozlov G.V. and Zaikov G.E., In Coll.: Fractals And Local Order In Polymer Materials, Ed. G.V. Kozlov and G.E. Zaikov, 2001, New York, Nova Science Publishers, Inc., pp. 55 - 64. Gladyishev G.P. and Gladyishev D.P., On Physicochemical Theory Of Bilogical Evolution (Preprint), 1993, Moscpw, Olimp, 24 p. (Rus) Gladyishev G.P. and Gladyishev D.P., Zh. Fiz. Khim., 1994, vol. 68(5), pp. 790 - 792. (Rus) Hornbogen E., Int. Mater. Rev., 1989, vol. 34(6), pp. 277 - 296. Bessendorf M.H., Int. J. Eng. Sci., 1987, vol. 25(6), pp. 667 - 672. Zemlyanov M.G., Malinovsky V.K., Novikov V.N., Parshin P.P., and Sokolov A.P., Zh. Eksper. Teor. Fiz., 1992, vol. 101(1), pp. 284 - 293. (Rus)

88

G. V. Kozlov and G. E. Zaikov

[15] Kozlov G.V., Ozden S., Krysov V.A., and Zaikov G.E., In Coll.: Fractals And Local Order In Polymeric Materials, Ed. G.V. Kozlov and G.E. Zaikov, 2001, New York, Nova Science Publishers, Inc., pp. 83 - 88. [16] Kozlov G.V., Ozden S., and Dolbin I.V., Russian Polymer News, 2002, vol. 7(2), pp. 35 - 38. [17] Bagryansky V.A., Malinovsky V.K., Novikov V.N., Pushchaeva L.M., and Sokolov A.P., Fizika Tverdogo Tela, 1988, vol. 30(8), pp. 2360 – 2366. (Rus) [18] Balankin A.S., Synergism of Deformable Body, 1991, Moscow, MO SSSR, 404 p. (Rus) [19] Kozlov G.V., Belousov V.N., and Mikitaev A.K., High Pressure Physics and Technology, 1998, vol. 8(1), pp. 64 - 70. (Rus) [20] Flory P.J., Brit. Polymer J., 1976, vol. 8(1), pp. 1 - 10. [21] Balankin A.S., Bugrimov A.L., Kozlov G.V., Mikitaev A.K., and Sanditov D.S., Doklady AN, 1992, vol. 326(3), pp. 463 - 466. (Rus) [22] Sokolov I.M., Uspekhi Fizicheskikh Nauk, 1986, vol. 150(2), pp. 221 - 256. (Rus) [23] Song H.-H. and Roe R.-J., Macromolecules, 1987, vol. 20(11), pp. 2723 2732. [24] Rammal R. and Toulouse G., J. Physiq. Lettr., 1983, vol. 44(1), pp. L13 L22. [25] Balankin A.S., Pis’ma V ZhTF, 1991, vol. 17(6), pp. 84 - 89. (Rus) [26] Novikov V.U., Kozlov G.V., and Boronin D.V., Materialovedenie, 1999, No. 3, pp. 25 – 28. (Rus) [27] Meakin P., Phys. Rev. Lett., 1983, vol. 51(13), pp. 1119 - 1122. [28] Kolb M., Botet R., and Jullien R., Phys. Rev. Lett., 1983, vol. 51(13), pp. 1123 - 1126. [29] Family F., Phys. Rev. Lett., 1983, vol. 51(23), pp. 2112 - 2115. [30] Irzhak V.I., Rozenberg B.A., and Enikolopyan N.S., Polymer Networks: Synthesis, Structure, Properties, 1978, Moscow, Nauka, 248 p. (Rus) [31] Kozlov G.V., Beloshenko V.A., Stroganov I.V., and Lipatov Yu.S., Doklady NAN Ukrainy, 1995, No. 10, pp. 117 - 118. (Rus) [32] Kozlov G.V., Burya A.I., and Zaikov G.E., Inzhenerno-Fizicheskii Zhurnal, 2003, vol. 77, No. 1 (in press). (Rus) [33] Katz A.J. and Tompson A.H., Phys. Rev. Lett., 1985, vol. 54(12), pp. 1325 1328. [34] Kozlov G.V. and Novikov V.U., Uspekhi Fizicheskikh Nauk, 2001, vol. 171(7), pp. 717 - 764. (Rus)

References

89

[35] Kozlov G.V., Beloshenko V.A., Varyukhin V.N., and Lipatov Yu.S., Polymer, 1999, vol. 40(4), pp. 1045 - 1051. [36] Beloshenko V.A. and Kozlov G.V., Mekhanika Kompozitnyikh Materialov, 1994, vol. 30(4),pp. 451 - 454. (Rus) [37] Kozlov G.V., Belousov V.N., Serdyuk V.D., and Kuzhetsov E.N., High Pressure Physics and Technology, 1995, vol. 5(3), pp. 59 - 64. (Rus) [38] Smirnov B.M., Uspekhi Fizicheskikh Nauk, 1986, vol. 149(2), pp. 177 219. (Rus) [39] Kozlov G.V., Beigelzimer Ya.E., Gazaev M.A., Novikov V.U., and Mikitaev A.K., Fractal Physics Of The Polymer Amorphous State, Manuscript deposited to VINITI RAS, Moscow, December 05, 1995, No. 3221-V95. (Rus) [40] Flory P.J., J. Chem. Phys., 1977, vol. 66(12), pp. 5720 - 5729. [41] Kozlov G.V., Aloev V.Z., and Lipatov Yu.S., Doklady NAN Ukrainy, 2001, No. 3, pp. 150 - 154. (Rus) [42] Kozlov G.V., Beloshenko V.A., Gazaev M.A., and Varyukhin V.N., High Pressure Physics and Technology, 1995, vol. 5(1), pp. 74 - 80. (Rus) [43] Careri G., Ordine E Disordine Nella Materia, Laterza, 1982, 228 p. [44] Ivanova V.S., Synergism. Strength And Destruction Of Metal Materials, 1992, Moscow, Mir, 160 p. (Rus) [45] Wu S., J. Polymer Sci., Part B, Polymer Phys., 1989, vol. 27(4), pp. 723 741. [46] Wu S., J. Appl. Polymer Sci., 1992, vol. 46(4), pp. 619 - 624. [47] Boyer R.F., Macromolecules, 1992, vol. 25(20), pp. 5326 - 5330. [48] Boyer R.F. and Miller R.L., Macromolecules, 1977, vol. 10(5), pp. 1167 1169. [49] Balankin A.S., Pis’ma V ZhTF, 1990, vol. 16(7), pp. 14 - 20. (Rus) [50] Aliguliev R.M., Khiteeva D.M., and Oganyan V.A., Vysokomol. Soedin., 1988, vol. B30(4), pp. 268 - 272. (Rus) [51] Aliguliev R.M., Khiteeva D.M., Oganyan V.A., and Nuriev R.A., Doklady AN AzSSR, 1989, vol. 45(5), pp. 28 - 31. (Rus) [52] Perepechko I.I. and Maksimov A.V., Vysokomol. Soedin., 1989, vol. B31(1), pp. 54 - 57. (Rus) [53] Aharoni S.M., Macromolecules, 1983, vol. 16(9), pp. 1722 - 1728. [54] Novikov V., Gazaev M., and Kozlov G., Proc. Second Symposium “Advances in Structured and Heterogeneous Continua”, August 14 - 16, 1995, Moscow, Russia, p. 45. [55] Kozlov G.V., Gazaev M.A., Novikov V.U., and Mikitaev A.K., Behavior Of Dissipative Structures In Deformable Polymer Matrices, Manuscript

90

[56] [57] [58] [59]

[60] [61] [62] [63]

[64] [65] [66] [67] [68] [69] [70] [71] [72] [73]

G. V. Kozlov and G. E. Zaikov deposited to VINITI RAS, Moscow, November 03. 1995, No. 2944-V95. (Rus) Kozlov G.V., Beloshenko V.A., Novikov V.U., and Lipatov Yu.S., Ukrainsky Khimichesky Zhurnal, 2001, vol. 67(3), pp. 57 - 60. (Rus) Shogenov V.N., Belousov V.N., Potapov V.V., Kozlov G.V., and Prut E.V., Vysokomol. Soedin., 1991, vol. A33(1), pp. 155 - 160. (Rus) Kozlov G.V., Shustov G.B., and Temiraev K.B., Vestnik KBGU, Ser. Khimicheskie Nauki, 1997, No. 2, pp. 50 - 52. (Rus) Kozlov G.V. and Sanditov D.S., Anharmonic Effects And Physicomechanical Properties Of Polymers, 1994, Novosibirsk, Nauka, 261 p. (Rus) Budtov V.P., Physical Chemistry Of Polymer Solutions, 1992, SaintPetersburg, Khimia, 384 p. (Rus) Kozlov G.V., Temiraev K.B., and Shustov G.B., Plast. Massy, 1998, No. 9, pp. 27 - 29. (Rus) Kozlov G.V., Burmistr M.V., Korenyako V.A., and Zaikov G.E., Voprosy Khimii I Khimicheskoi Tekhnologii, 2002, No. 6, pp. 77 – 81. (Rus) Kozlov G.V., Beloshenko V.A., Gazaev M.A., and Novikov V.U., Mekhanika Kompozitnyikh Materialov, 1996, vol. 32(2), pp. 270 - 278. (Rus) Gazaev M.A., Kozlov G.V., Milman L.D., and Mikitaev A.K., High Pressure Physics and Technology, 1996, vol. 6(1), pp. 76 - 81. (Rus) Lyubchenko L.S. and Lyubchenko M.L., Khimicheskaya Fizika, 1997, vol. 16(8), pp. 24 - 51. (Rus) Kozlov G.V., Burya A.I., Sviridenok A.I., and Zaikov G.E., Doklady NAI Belarusi, 2003, vol. 47 (in press). Kozlov G.V., Gazaev M.A., Novikov V.U., and Mikitaev A.K., Pis’ma V ZhTF, 1996, vol. 22(16), pp. 31 - 38. (Rus) Kozlov G.V., Novikov V.U., Gazaev M.A., and Mikitaev A.K., InzhenernoFizicheskyi Zhurnal, 1998, vol. 71(2), pp. 241 - 247. (Rus) Porter D., Polymer, 1987, vol. 28(8), pp. 1652 - 1656. Donald A.M., Kramer E.J., and Bubeck R.A., J. Polymer Sci., Polymer Phys. Ed., 1982, vol. 20(7), pp. 1129 - 1141. Wu S., ”Benibana” Int. Symp. October 8-11, 1990, Yamagata, Japan, Abstract, Yamagata, Japan, 1990, pp. 130 - 137. Lipatov Yu.S. and Privalko V.P., J. Macromol. Sci.-Phys., 1973, vol. B7(3), pp. 431 - 444. Haward R.N. and Thackray G., Proc. Royal Soc. Lond., 1968, vol. A302(1471), pp. 453 - 472.

References

91

[74] Plummer C.J.G. and Donald A.M., Macromolecules, 1990, vol. 23(7), pp. 3929 - 3937. [75] Edwards S.F. and Vilgis T., Polymer, 1987, vol. 28(3), pp. 375 - 378. [76] Balankin A.S., Ivanova V.S., and Breusov V.P., Doklady AN, 1992, vol. 322(6), pp. 1080 - 1085. (Rus) [77] Kozlov G.V., Temiraev K.B., Shetov R.A., and Mikitaev A.K., Materialovedenie, 1999, No. 2, pp. 34 - 39. (Rus) [78] Kozlov G.V., Ozden S., and Zaikov G.E., In book: Fractal Analysis of Polymers: From Synthesis to Composites, Ed. Kozlov G., Zaikov G., and Novikov V., New York, Nova Science Publishers, Inc., 2003, p. 113-121. [79] Caush G., Destruction Of Polymers, 1981, Moscow, Mir, 440 p. (Rus) [80] Kozlov G.V., Belousov V.N., Sanditov D.S., and Mikitaev A.K., Izvestiya VUZov, Severo-Kavkazsky Region, Estestvennye Nauki, 1994, No. 1 – 2(86), pp. 54 - 58. (Rus) [81] Aharoni S.M., Macromolecules, 1985, vol. 18(12), pp. 2624 - 2630. [82] Hong S.-D., Chung S.Y., Fedords R.F., and Moacanin J., J. Polymer Sci.: Polymer Phys. Ed., 1983, vol. 21(9), pp. 1647 - 1660. [83] Sanditov D.S., Kozlov G.V., Belousov V.N., and Lipatov Yu.S., Ukrainian Polymer J., 1992, vol. 1(3-4), pp. 241 - 258. [84] Frenkel Ya.I., Kinetic Theory Of Liquids, 1945, Moscow-Leningrad, Izd. AN SSSR, 424 p. (Rus) [85] Ferry J.D., Viscoelastic Properties of Polymers, 3rd Ed., New York, Wiley and Sons, 1980, 522 p. [86] Sanditov D.S. and Bartenev G.M., Physical Properties of Non-Oriented Structures, 1982, Novosibirsk, Nauka, 256 p. (Rus) [87] Sanditov D.S. and Kozlov G.V., Vysokomol. Soedin., 1996, vol. A36(8), pp. 1389 - 1393. (Rus) [88] Sanditov D.S., Sangadiev S.Sh., and Kozlov G.V., Fizika I Khimia Stekla, 1998, vol. 24(6), pp. 758 - 766. (Rus) [89] Sanditov D.S., Kozlov G.V., Belousov V.N., and Lipatov Yu.S., Fizika I Khimia Stekla, 1994, vol. 20(1), pp. 3 - 13. (Rus) [90] Belousov V.N., Kozlov G.V., Mikitaev A.K., and Lipatov Yu.S., Doklady AN SSSR, 1990, vol. 313(3), pp. 630 - 633. (Rus) [91] Sanditov D.S. and Kozlov G.V., Fizika I Khimia Stekla, 1993, vol. 19(4), pp. 593 - 601. (Rus) [92] Kozlov G.V., Beloshenko V.A., and Lipskaya V.A., Ukrainsky Fizichesky Zhurnal, 1996, vol. 41(2), pp. 222 - 225. (Rus) [93] Belousov N.V., Beloshenko V.A., Kozlov G.V., and Lipatov Yu.S., Ukrainsky Khimichesky Zhurnal, 1996, vol. 62(1), pp. 1 - 4. (Rus)

92

G. V. Kozlov and G. E. Zaikov

[94] Lipatov Yu.S., Uspekhi Khimii, 1978, vol. 47(2), pp. 332 - 366. (Rus) [95] Sanchez I.C., J. Appl. Phys., 1974, vol. 45(10), pp. 4204 - 4215. [96] Beloshenko V.A., Kozlov G.V., and Varyukhin V.N., High Pressure Physics And Technology, 1994, vol. 4(2), pp. 70 -74. (Rus) [97] Sanditov D.S. and Kozlov G.V., Fizika I Khimia Stekla, 1995, vol. 21(6), pp. 547 - 576. (Rus) [98] Knopoff L. and Shapiro J.N., Phys. Rev. B, 1970, vol. 1(10), pp. 3893 3895. [99] Sharma B.K., Acoust. Lett., 1980, vol. 4(2), pp. 19 - 23. [100] Sharma B.K., Acoust Lett., 1980, vol. 4(1), pp. 11 - 14. [101] Olemsky A.I., Katsnelson A.A., and Umrikhin V.V., Fizika Tverdogo Tela, 1985, vol. 27(2), pp. 318 - 321. (Rus) [102] Kozlov G.V. and Mikitaev A.K., Vysokomol. Soedin., 1987, vol. B29(7), pp. 490 - 492. (Rus) [103] Kozlov G.V., Shetov R.A., and Mikitaev A.K., Doklady AN SSSR, 1986, vol. 290(4), pp. 885 - 888. (Rus) [104] Cohen M.H. and Grest G.S., Phys. Rev. B, 1979, vol. 20(3), pp. 1077 1098. [105] Chen H.S., J. Non-Cryst. Solids, 1981, vol. 46(3), pp. 289 - 305. [106] Manevich L.I., Oshmyan V.G., Gai M.I., Akopyan E.L., and Enikolopyan N.S., Doklady AN SSSR, 1986, vol. 289(1), pp. 128 - 131. (Rus) Margolina A. and Wu S., Polymer, 1988, vol. 29(12), pp. 2170 - 2173. [107] [108] Bridge B., J. Mater. Sci. Lett., 1989, vol. 8(2), pp. 102 - 103. [109] Patrikeev G.A., Doklady AN SSSR, 1968, vol. 183(9), pp. 636 - 639. (Rus) [110] Patrikeev G.A., Mekhanika Polimerov, 1971, No. 2, pp. 221 - 231. (Rus) [111] Kozlov G.V., Sanditov D.S., Milman L.D., and Serdyuk V.D., Izvestiya VUZov. Severo-Kavkazskyi Region, Estestvennye Nauki, 1993, No. 3 – 4(83-84), pp. 88 - 92. (Rus) [112] Prevorsek D.C. and De Bona B.T., J. Macromol. Sci.-Phys., 1981, vol. B19(4), pp. 605 - 622. [113] Shustov G.B., Belousov V.N., Kozlov G.V., and Mikitaev A.K., Carcass Coherency And Mechanical Properties Of Extruded Amorphous Polymers, Manuscript disposed to VINITI RAS, Moscow, February 26, 1997, No. 626-V97. (Rus) [114] Kozlov G.V., Aloev V.Z., Bazheva R.Ch., and Zaikov G.E., In Coll.: IV AllRussian Sci.-Tech. Conf. “New Chemical Technologies: Production and Application”, Penza, PGU, 2002, pp. 59 – 61. (Rus) [115] Shklovsky B.I. and Efros A.L., Uspekhi Fizicheskikh Nauk, 1975, vol. 117(3), pp. 401 - 436. (Rus)

References

93

[116] Family F., J. Stat. Phys., 1984, vol. 36(5/6), pp. 881 - 896. [117] Kozlov G.V. and Dolbin I.V., Mater. Intern. Conf. “Physics of Electronic Materials”, Kaluga, Russia, Oct. 1-4, 2002, p. 134 - 135. [118] Kozlov G.V., Beloshenko V.A., and Lipatov Yu.S., Ukrainsky Khimichesky Zhurnal, 1998, vol. 64(3), pp. 56 - 59. (Rus) [119] Bobryishev A.N., Kozomazol V.N., Babin L.O., and Solomatov V.I., Synergism Of Composite Materials, 1994, Lipetsk, NPO ORIUS, 153 p. (Rus) [120] Kozlov G.V., Serdyuk V.D., and Dolbin I.V., Materialovedenie, 2000, No. 12, pp. 2 - 5. (Rus) [121] Beloshenko V.A., Kozlov G.V., and Lipatov Yu.S., Fizika Tverdogo Tela, 1994, vol. 36(10), pp. 2903 - 2906. (Rus) [122] Bartenev G.M. and Frenkel S.Ya., Physics Of Polymers, 1990, Leningrad, Khimia, 432 p. (Rus) [123] Kozlov G.V., Beloshenko V.A., Varyukhin V.N., and Novikov V.U., Zhurnal Fizicheskikh Issledovanii, 1997, vol. 1(2), pp. 204 - 207. (Rus) [124] Aloev V.Z., Kozlov G.V., and Beloshenko V.A., Izvestiya KBNTs RAN, 2000, No. 1(4), pp. 108 - 113. (Rus) [125] Berstein V.A. and Egorov V.M., Differential Scanning Calorimetry In Physicochemistry Of Polymers, 1990, Leningrad, Khimia, 256 p. (Rus) [126] Bittrich H.-J., Acta Polymerica, 1982, vol. 33(12), p. 741. [127] Kozlov G.V., Burya A.I., Sanditov D.S., Serdyuk V.D., and Lipatov Yu.S., Materialy, Tekhnologii, Instrumenty, 1999, vol. 4(2), pp. 51 - 54. (Rus) [128] Kozlov G.V. and Lipatov Yu.S., Vysokomol. Soedin., 2003, vol. B45(4), pp. 660 - 664. (Rus) [129] Kozlov G.V., Sanditov D.S., and Lipatov Yu.S., In Coll.: Fractals And Local Order In Polymeric Materials, Ed. G.V. Kozlov and G.E. Zaikov, New York, Nova Science Publishers, Inc., 2001, pp. 65 - 82. [130] Adam G. and Gibbs J.H., J. Chem. Phys., 1965, vol. 43(1), pp. 139 - 146. [131] Witten T.A. and Sander L.M., Phys. Rev. Lett., 1981, vol. 47(19), pp. 1400 1403. [132] Meakin P., Phys. Rev. A, 1983, vol. 27(3), pp. 1495 - 1507. [133] Kokorevich A.G., Gravitis Ya.A., and Ozon’-Kalnin V.G., Khimia Drevesiny, 1989, No. 1, pp. 3 – 24. (Rus) [134] Kozlov G.V., Beloshenko V.A., and Varyukhin V.N., Ukrainsky Fizichesky Zhurnal, 1998, vol. 43(3), pp. 322 - 323. (Rus) [135] Botet R., Jullien R., and Kolb M., Phys. Rev. A, 1984, vol. 30(4), pp. 2150 2152. [136] Brady R.M. and Ball R.C., Nature, 1984, vol. 309(5965), pp. 225 - 229.

94

G. V. Kozlov and G. E. Zaikov

[137] Witten T.A. and Meakin P., Phys. Rev. B, 1983, vol. 28(10), pp. 5632 5642. [138] Mosolov A.B. and Dinariev O.Yu., Problemy Prochnosti, 1988, No. 1, pp. 3 - 7. (Rus) [139] Witten T.A. and Sander L.M., Phys. Rev. A, 1983, vol. 27(9), pp. 5686 5697. [140] Meakin P. and Witten T.A., Phys. Rev. A, 1983, vol. 28(5), pp. 2985 - 2988. [141] Kozlov G.V., Shogenov V.N., and Mikitaev A.K., Inzhenerno-Fizicheski Zhurnal, 1998, vol. 71(6), pp. 1012 - 1015. (Rus) [142] Litt M.H., Koch P.J., and Tobolsky A.V., J. Macromol. Sci.-Phys., 1967, vol. B1(3), pp. 587 - 594. [143] Wunderlich B. Macromolecular Physics, Volume 1, New York – London, Academic Press, 1973, 623 p. [144] Burya A.I., Shogenov V.N., Kozlov G.V., and Arlamova N.T., Pridneprovsky Nauchny Vestnik, 1998, No. 83, pp. 9 - 16. (Rus) [145] Kozlov G.V., Beloshenko V.A., and Gazaev M.A., Ukrainski Fizicheski Zhurnal, 1996, vol. 41(11-12), pp. 1110 - 1113. (Rus) [146] Mashukov N.I., Gladyishev G.P., and Kozlov G.V., Vysokomol. Soedin., 1991, vol. A33(12), pp. 2538 - 2546. (Rus) [147] Afaunov V.V., Shogenov V.N., Mashukov N.I., and Kozlov G.V., Elektr. Zhurnal “Issledovano V Rossii”, 1999, 33. http://zhurnal mipt.rssi.ru/articles /1999/033.pdt. (Rus) [148] Graessley W.W. and Edwards S.F., Polymer, 1981, vol. 22(10), pp. 1329 1334. [149] Bessonov M.I., Koton M.M., Kudryavtsev V.V., and Laius L.A., Polyimides – The Class of Thermoresistant Polymers, 1983, Leningrad, Nauka, 302 p. (Rus) [150] Willbourn A.H., Polymer, 1976, vol. 17(10), pp. 965 - 976. [151] Mikitaev A.K., Kozlov G.V., and Shogenov V.N., Plast. Massy, 1983, No. 2, pp. 32 - 33. (Rus) [152] Koton M.M., Artemieva V.N., Kukarkina N.V., Kuznetsov Yu.P., and Dergacheva E.N., Vysokomol. Soedin., 1987, vol. B29(8), pp. 571 - 575. (Rus) [153] Kozlov G.V., Temiraev K.B., and Afaunova Z.I., The Effect of Intermolecular Interaction Energy On Structure Of Heterochain Polyesters, Manuscript deposited to VINITI RAS, Moscow, June 15, 1999, No. 1918V99. (Rus) [154] Kozlov G.V., Temiraev K.B., and Bedanokov A.Yu., Vestnik Adyigeiskogo Universiteta, 1999, No. 3, pp. 79 - 82. (Rus)

References

95

[155] Kalinichev E.L. and Sakovtseva M.B., Properties And Processing Of Thermoplasts, 1983, Leningrad, Khimia, 288 p. (Rus) [156] Vasnev V.A. and Kuchanov S.I., Uspekhi Khimii, 1973, vol. 42(12), pp. 2194 - 2220. (Rus) [157] Privalko V.P. and Lipatov Yu.S., Vysokomol. Soedin., 1971, vol. A13(12), pp. 2733 - 2738. (Rus) [158] Lee W.A. and Sewell J.H., J. Appl. Polymer Sci., 1968, vol. 12(6), pp. 1397 - 1409. [159] Meakin P., J. Chem. Phys., 1983, vol. 79(5), pp. 2426 - 2429. [160] Kozlov G.V., Burya A.I., Sviridenok A.I., and Zaikov G.E., Doklady NAI Belarusi, 2003, vol. 47 (in press). (Rus) [161] Jullien R. and Kolb M., J. Phys. A, 1984, vol. 17(12), pp. L639 - L643. [162] Kozlov G.V., Doklady Adyigeiskoi (Cherkesskoi) Mezhdunarodnoi AN, 2001, vol. 6(1), pp. 83 – 87. (Rus) [163] Kozlov G.V., Beloshenko V.A., Gazaev M.A., and Lipatov Yu.S., Vysokomol. Soedin., 1996, vol. B38(8), pp. 1423 - 1426. (Rus) [164] Kozlov G.V., Beloshenko V.A., and Varyukhin V.N., Prikladnaya Mekhanika I Tekhnicheskaya Fizika, 1996, vol. 37(3), pp. 115 - 119. (Rus) [165] Kozlov G.V., Beloshenko V.A., and Varyukhin V.N., Ukrainski Fizicheski Zhurnal, 1996, vol. 41(2), pp. 218 - 221. (Rus) [166] Kozlov G.V., Afaunova Z.I., and Zaikov G.E., Elektron. Zh. “Made In Russia”, 2003, Iss. 42, pp. 489 – 501; http: // Zhurnal.apl.relarn.ru/articles/ 2003/042.pdf. (Rus)

INDEX A access, 69 accuracy, 13, 70 Adams, 60 adhesion, 63, 64, 81 adjustment, 78, 80 agent, 12, 66 aggregates, 64 aggregation, 63, 64, 65, 66, 67, 81 aging, 7, 12, 52, 54 aging process, 12 alternative, 72, 85 alternatives, 7, 70 amine, 7, 52 amorphous, 1, 3, 4, 8, 14, 15, 16, 17, 19, 20, 24, 25, 26, 27, 28, 29, 33, 36, 37, 38, 41, 45, 47, 48, 49, 50, 51, 52, 53, 56, 59, 60, 64, 65, 67, 69, 70, 71, 73, 74, 77, 78, 79, 80, 84, 85, 86 amorphous polymer, 17, 19, 37, 38, 41, 47, 48, 50, 52, 53, 59, 60, 67, 74, 77, 78, 79, 80 amorphous polymers, 17, 19, 37, 38, 47, 48, 52, 59, 67 amorphous-crystalline polymers, 25, 29, 47, 49, 51, 56, 84, 85, 86 angstroms, 2, 14 anharmonicity, 41, 45 annealing, 59 annihilation, 35, 36

application, 6, 7, 11, 12, 13, 14, 27, 37, 41, 45, 47, 64, 70, 77, 78 aromatic, 74 assessment, 20, 29, 30, 42, 44, 48, 57, 70, 72, 82, 83 asymptotic, 23 atom, 35 atoms, 14, 35, 36 autocorrelation, 79 averaging, 24

B balanced state, 59 behavior, 3, 4, 6, 14, 25, 38, 53, 54, 55, 68, 85 binding, 5, 23, 56 block-copolymer, 74 blocks, 74, 75 bonds, 13, 26, 37, 78 Brownian motion, 63

C candidates, 71 capacity, 41 CEC, 7 chain molecules, 13 chain rigidity, 27, 31, 33, 76, 77

98

Index

chemical, 7, 10, 11, 14, 15, 16, 17, 38, 53, 55, 74, 82, 83 chemical cross-links, 17, 74 classes, 13, 26, 68 classical, 50, 52 classified, 51 cluster functionality, 36, 51 cluster model, 3, 4, 6, 10, 14, 17, 20, 33, 35, 37, 38, 41, 42, 45, 50, 52, 53, 56, 59, 60, 64, 65, 73, 77, 85 cluster network, 10, 17, 27, 45, 47, 48, 49, 53, 54, 55, 69, 82 cluster WS, 68 cluster-cluster, 65 clusters, 1, 2, 4, 7, 8, 10, 12, 17, 18, 20, 23, 24, 25, 26, 27, 28, 32, 35, 36, 48, 49, 50, 53, 54, 55, 56, 63, 65, 67, 69, 71, 77, 78, 81, 82, 83, 85 coherence, 49 cohesion, 74 coil, 21 collisions, 81 competition, 6 complement, 6, 12 components, 38, 41, 53, 55, 64, 78 composite, 72, 93 composites, 71, 72, 73 composition, 74 compressibility, 6 compression, 18 computer, 6, 63 Computer simulation, 64 concentration, 7, 51, 65, 70, 71, 72, 73, 74, 75, 76, 84, 85 concordance, 25 configuration, 4, 52, 54 conformational, 56 conformity, 15, 22, 27, 31, 33, 56, 57, 66, 70, 71, 73, 80, 84, 85 Congress, iv construction, 14 construction materials, 14 copolymer, 74, 75 copolymers, 75, 77

correlation, 5, 8, 9, 20, 21, 23, 26, 29, 31, 42, 48, 50, 51, 56, 66, 67, 68, 72, 76, 77, 78, 79, 82 correlations, 6, 27, 38, 59, 67, 69, 74, 76 covalent, 26, 78 covalent bond, 26, 78 critical behavior, 50 critical value, 36, 51, 82 cross-linked, 6, 16, 83 cross-linked polymer, 16, 83 cross-linked polymers, 16, 83 cross-linking, 7, 8, 12, 52, 81 crystal, 7 crystal growth, 7 crystalline, 15, 16, 17, 20, 25, 26, 27, 28, 29, 47, 49, 51, 56, 69, 71, 79, 84, 85, 86 crystallinity, 56, 74 crystallites, 7 crystals, 7 curing, 66

D Debye, 41, 42, 43, 44 decomposition, 1, 14, 36 deduction, 11 defects, 24, 68 deformability, 28 deformation, 17, 20, 24, 37, 80 degradation, 2, 29, 55 degradation process, 2 degree, 7, 56, 57, 74, 78 degrees of freedom, 36 delivery, 66 density, 2, 3, 42, 68, 69, 71, 72, 73, 74, 75, 76, 77, 78, 79, 84 destruction, 29 detachment, 35, 36, 37, 65 deviation, 22, 51, 60, 72, 80, 84 diaminodiphenylmethane, 25 dichloranhydride, 74 Differential Scanning Calorimetry, 93 diffraction, 22 diffusion, 63, 67, 81, 84

Index dimensionality, 2, 4, 6, 7, 10, 11, 12, 20, 21, 22, 23, 25, 29, 53, 54, 55, 56, 57, 64, 65, 68, 74, 79, 80, 81, 82, 83, 85 dislocations, 24 dispersion, 15, 76, 84 disposition, 75 dissipative structure, 14 dissipative structures, 14 dissociation, 37 distribution, 24, 27, 68 domains, 71, 72, 74, 76 double logarithmic coordinates, 3, 42, 43, 50, 51, 59, 68, 69

E elastic deformation, 17, 37 elasticity, 38, 45, 48, 49 elasticity modulus, 45, 48, 49 electronic, iv electrostatic, iv energy, 14, 17, 18, 19, 20, 21, 23, 29, 35, 36, 37, 42, 74, 75, 76, 77 energy density, 74, 75, 76, 77 energy transfer, 24 entanglement, 10, 14, 16, 17, 27, 31, 49, 69 entanglement network, 27, 31 entanglements, 14, 15, 16, 17, 27, 28, 29, 31, 47, 48, 70 EP, 4, 7, 8, 11, 12, 18, 22, 38, 51, 52, 53, 54, 55, 66, 81, 83 EP-1, 4, 7, 12, 18, 38, 51, 52, 53, 54, 55, 66 EP-2, 4, 7, 12, 18, 38, 51, 52, 53, 54, 55, 66, 81, 83 EP-3, 52, 53, 54, 55, 81, 83 epoxy, 7, 12, 24, 25, 38, 51, 52, 53, 54, 55, 82 epoxy polymer, 7, 24, 25, 38, 52, 53, 54, 55, 82 epoxy polymers, 7, 24, 25, 38, 52, 53, 54, 55, 82 equality, 28, 29, 47, 55, 69 equilibrium, 1, 2, 4, 6, 7, 12, 13, 14, 20, 22, 24, 52, 54, 55, 57, 59, 60, 61, 83, 85, 86 equilibrium state, 54, 55, 57, 59, 60, 61, 83, 85, 86

99

ester, 30 ethylene, 58 Euclidean, 2, 6, 22, 53, 65 Euclidean object, 6, 65 Euclidean objects, 6 Euclidean space, 2, 53 evolution, 14, 17 expert, iv extrapolation, 38, 55, 76 extrusion, 22

F February, 92 film, 22 films, 22 fixation, 28, 32, 33 flexibility, 16, 21, 27, 75 flow, 17, 18, 20, 23, 24, 38 fluctuation free volume, 35, 36, 37, 38, 65 fluctuations, 60 forecasting, 6, 74 fractal, 1, 2, 4, 5, 6, 10, 11, 12, 13, 21, 22, 23, 24, 25, 27, 29, 32, 33, 53, 54, 55, 56, 57, 58, 64, 65, 66, 68, 69, 70, 72, 73, 79, 80, 81, 82, 83, 85 fractal analysis, 1, 4, 6, 12, 13, 27, 32, 33 fractal dimension, 2, 5, 7, 10, 11, 12, 21, 22, 24, 25, 29, 53, 54, 55, 56, 57, 58, 65, 66, 68, 70, 72, 73, 79, 80, 81, 82, 83 fractal dimensionality, 2, 7, 10, 11, 12, 21, 22, 24, 25, 29, 53, 54, 55, 56, 57, 65, 68, 79, 80, 81, 82, 83 fractal objects, 1 fractal properties, 2, 69 fractal structure, 1, 6, 7 fractality, 1, 2, 3, 4, 5, 6, 12, 23, 52 fractals, 4, 6, 24 fracture, 1, 29 fragmentation, 24 free volume, 35, 36, 37, 38, 57, 58, 65, 77 freedom, 36 freezing, 63, 70 frequency, 7, 8, 12, 17, 27, 31, 33, 42, 43, 45, 48, 69, 71, 72, 74, 81, 82, 83, 84

100

Index

fulfillment, 1, 43 future, 12, 63

G gel, 6, 8, 11, 12, 23, 63, 65 gel formation, 7, 8, 11, 12, 23, 65 generation, 35, 37, 67 Gibbs, 1, 2, 6, 60, 93 glass, 22, 35, 36, 38, 50, 52, 58, 60, 74, 75, 76 glass transition, 35, 36, 38, 50, 52, 58, 60, 74, 75, 76 glass transition temperature, 36, 38, 50, 74, 75, 76 glasses, 35, 37, 41 glassy polymers, 6, 12, 36, 37, 41, 51, 67, 70 glassy state, 7, 11, 12, 27, 28, 32, 33, 41, 49, 56, 82 graph, 50 groups, 14 growth, 7, 55, 66, 70, 77, 78, 82, 83

H Hausdorff dimension, 6 HDPE, 36, 48, 49, 57, 69, 70, 71, 72, 73, 77 heat, 36, 41, 42, 54, 60 heat aging, 54 heat capacity, 41 homogeneous, 4, 6 hypothesis, 64

I identification, 69, 75, 84 independence, 43 indices, 4, 7, 52, 53, 54, 55, 65, 66 inequality, 50 infinite, 47, 50, 63 injection, 71 injury, iv intensity, 75, 78 interaction, 36, 37, 41, 42, 54, 70, 74, 78, 83, 85, 94

interactions, 52, 54, 64, 75 interdependence, 76 intermolecular, 37, 74, 75, 77, 78 intermolecular interaction, 74, 75, 78 intermolecular interactions, 75 interphase, 71 interpretation, 15, 17, 18, 28, 53, 70 interval, 8, 33, 43, 48, 79 isotropic, 14

J Japan, 90

K kinetic equations, 7

L lattice, 41, 79 laws, 50 light, 17 limitations, 28 linear, 2, 3, 14, 15, 16, 18, 22, 24, 25, 26, 31, 37, 38, 43, 44, 47, 48, 50, 51, 59, 60, 66, 68, 69, 76, 79, 82 linear defects, 24 linear dependence, 26, 76 linear function, 38 linear polymers, 14, 15, 22, 38 links, 17, 74 liquids, 35, 41 literature, 15, 23, 27, 31, 48, 84 local order, 1, 4, 5, 6, 7, 10, 12, 14, 23, 24, 25, 36, 41, 51, 54, 55, 57, 59, 65, 66, 69, 70, 71, 73, 77, 78, 79, 81, 83, 85 localization, 17, 18, 19, 20, 21 logarithmic coordinates, 3, 42, 43, 50, 51, 59, 68, 69 London, 94 low temperatures, 48

Index

M macromolecular coil, 21 macromolecular entanglements, 27, 47, 48 macromolecules, 8, 14, 33, 47, 48, 71, 82 magnetic, iv, 71 magnetic field, 71 magnetic fields, 71 mass, 42 mathematical, 4, 47 Matrices, 89 matrix, 17, 19, 22, 35, 37, 38, 53, 54, 55, 57, 66, 69, 77, 78, 85, 86 maximal local, 10 mechanical, iv, 14, 17, 20, 29, 47, 49 mechanical energy, 29 mechanical properties, 14, 47, 49 mechanical stress, 17 mechanical stresses, 17 media, 23 melt, 71 mercury, 41 metals, 24 methyl methacrylate, 30, 58 microcavity, 35, 36, 37, 65 migration, 35 mobility, 28, 29, 32, 52, 54, 56, 82 models, 4, 27, 28, 47, 52, 64, 65, 70, 74, 84, 85 modulus, 17, 18, 21, 45, 48, 49 molecular mass, 11, 48 molecular mobility, 28, 29, 32, 52, 54, 56, 82 molecular structure, 13 molecules, 7, 13, 41 Monte-Carlo, 63 Moscow, 87, 88, 89, 90, 91, 92, 94 motion, 36, 63, 78 multifractal, 6 multiplication, 66

N natural, 13, 47, 52, 71

101

network, 6, 10, 11, 12, 14, 17, 23, 27, 31, 33, 38, 45, 47, 48, 49, 53, 54, 55, 65, 66, 69, 71, 72, 82, 84 networks, 7, 22, 38, 47 New York, iii, iv, 87, 88, 91, 93, 94 nucleation, 7, 8, 9

O oligomer, 12, 66 organization, 6, 24, 25, 26 orientation, 41, 45, 52, 54, 55, 58, 81 oriented polymers, 20 oscillations, 41, 42

P PAr, 1, 2, 22, 36, 37, 38, 42, 43, 44, 45, 48, 49, 50, 51, 67, 68, 70, 71, 74 parameter, 6, 13, 18, 19, 21, 23, 27, 28, 29, 41, 42, 44, 48, 51, 52, 53, 55, 56, 65, 67, 68, 71, 72, 79, 80, 84, 85 particle-cluster, 63 particles, 63, 64, 65, 66, 69, 71, 72, 77, 78, 79, 81, 83, 84, 85, 86 PC, 1, 2, 22, 32, 33, 36, 37, 38, 48, 49, 50, 51, 57, 59, 60, 67, 68, 69, 70, 71, 77, 79, 80, 81 percolation, 4, 47, 50, 51, 52, 53, 54, 55, 59 percolation cluster, 4, 50, 51, 52, 53, 55 percolation clusters, 4, 55 percolation theory, 4, 47, 51 periodicity, 1, 3 phenolphthalein, 74 physical aging, 7, 12 physicochemistry, 1 physics, 1, 12, 13, 14, 41, 64 plasticity, 38 PMMA, 50, 51, 57, 60, 61 Poisson, 5, 32 polyamide, 75 polyarylate, 22, 74 polyesters, 74 polyethylene, 22, 84 polyethylenes, 48, 49

102

Index

polymer, 1, 2, 3, 4, 5, 6, 8, 10, 11, 12, 13, 14, 15, 16, 17, 19, 20, 21, 22, 23, 25, 26, 27, 28, 29, 32, 33, 36, 38, 41, 45, 47, 49, 51, 52, 53, 54, 55, 56, 57, 58, 59, 60, 63, 64, 65, 66, 69, 70, 71, 73, 74, 76, 77, 78, 79, 80, 81, 82, 83, 84, 85 polymer amorphous state, 3, 4, 8, 14, 25, 33, 38, 45, 52, 64, 69, 70, 73, 85 polymer amorphous state structure, 4, 25, 33, 38, 45, 64, 69, 70, 71, 73 polymer density, 69, 78 polymer network structures, 65 polymer networks, 7, 11, 12, 14, 15, 16, 17, 20, 25, 26, 27, 28, 38, 51, 55, 69, 81 polymer properties, 13, 27, 74, 77 polymer structure, 2, 3, 4, 5, 6, 10, 12, 21, 22, 25, 39, 50, 52, 53, 54, 55, 56, 57, 58, 59, 60, 71, 74, 77, 78, 83, 85 polymers, 1, 4, 6, 7, 11, 12, 13, 14, 15, 16, 17, 19, 20, 22, 23, 24, 25, 26, 27, 28, 29, 30, 31, 35, 36, 37, 38, 41, 43, 47, 48, 49, 51, 52, 53, 54, 55, 56, 57, 59, 60, 67, 68, 69, 70, 71, 74, 75, 82, 83, 84, 85, 86 polyvinylchloride, 75 potential energy, 42 power, 68, 70 preparation, iv, 22 pressure, 7, 42 probability, 24, 25, 26, 27, 47, 49, 50, 63, 79 probability distribution, 24 process, 18, 24, 52, 63, 64, 84 propagation, 63, 65, 66, 69, 71, 81, 84, 85 propane, 74 properties, 7, 11, 12, 13, 22, 23, 28, 35, 38, 47, 66, 71, 72, 75 property, iv, 17, 23 proportionality, 15, 36, 82 PSP, 36 PVC, 36

Q quantitative estimation, 85 quasi-equilibrium, 52, 54, 55, 57, 59, 60, 61, 83, 85, 86

quasi-equilibrium state, 54, 55, 57, 59, 60, 61, 83, 85, 86

R radius, 68, 70, 79, 85 random, 24, 35, 36, 37, 63 random walk, 63 range, 3, 6, 8, 14, 27, 32, 50, 52, 69, 72 RAS, 89, 90, 92, 94 redistribution, 78 regular, 75 regulation, 55 relaxation, 84 rheology, 27 rigidity, 6, 13, 27, 31, 33, 47, 49, 56, 75, 76, 77 rubber, 27, 55 rubbers, 29, 30 rubbery state, 29, 32, 82 Russia, 89, 93, 95 Russian, 88, 92

S sample, 22, 47, 65 scaling, 50, 65, 66, 79 science, 1 seeding, 70, 71, 72, 73, 84 Self, 53 self-assembly, 1 self-organization, 6 self-similarity, 8, 12, 14, 15, 16, 18, 20, 21, 29 series, 28, 37, 44, 52, 53, 55, 68, 70, 82, 84 services, iv shape, 2, 75 shear, 6, 17, 18 short-range, 37 sign, 69 signs, 69 similarity, 8, 12, 14, 15, 16, 18, 20, 21, 24, 29, 53 simulation, 6, 52, 63, 64, 70, 77, 78, 81, 83, 84

Index simulations, 70 solid phase, 1, 36 solid polymers, 4, 35, 49 solution, 13, 22 spatial, 14, 17, 18, 20 spectrum, 6 stability, 17 stages, 24, 69 steric, 64, 81, 83 strain, 83, 84 strength, 47 stress, 17, 80, 84 structural changes, 17, 72 structural characteristics, 7, 20, 52 structure formation, 1, 6, 47, 71, 74, 77 substitution, 5, 57 sulfur, 25 supermolecular structure, 6, 11, 21 superposition, 10 suppression, 54 symmetry, 6 systematic, 19 systems, 6, 11, 13, 25, 26, 64, 66

T temperature, 5, 28, 32, 35, 36, 37, 38, 41, 42, 43, 44, 45, 47, 48, 49, 50, 51, 57, 58, 59, 60, 67, 68, 69, 70, 74, 75, 76, 80, 81 temperature dependence, 5, 32, 35, 36, 41, 42, 45, 58 tensile, 22 theoretical, 1, 22, 30, 31, 50, 51, 58, 60, 70, 80, 82, 83 theory, 4, 9, 22, 35, 37, 41, 47, 51, 58, 60 thermal, 52, 53, 55, 59, 60 thermal cluster, 52, 53, 55, 59, 60 thermodynamic, 1, 6, 57, 58, 59, 60 thermodynamic equilibrium, 57, 60 thermodynamics, 14, 20 three-dimensional, 10, 22, 23, 50, 51, 53, 83 three-dimensional space, 10, 22, 83 threshold, 4, 47, 50 time, 3, 7, 8, 22, 66, 69 topological, 13, 28, 32, 33, 55

103

topology, 15, 27 transfer, 24 transformation, 24 transition, 1, 2, 6, 15, 28, 32, 35, 36, 52, 57, 58, 60, 63, 65, 69, 70, 74, 76, 82 transition temperature, 74 translational, 6 turbulence, 23, 24 turbulent, 23 turbulent flows, 23

U uncertainty, 13 uniform, 18 universality, 53, 64, 65, 66, 69

V valence, 13, 31, 32, 56, 57 values, 11, 15, 20, 22, 23, 27, 30, 31, 32, 43, 45, 48, 51, 52, 53, 55, 56, 66, 69, 72, 75, 78, 80, 81, 83, 84, 85 variable, 38 variables, 42 variation, 1, 4, 15, 23, 37, 39, 42, 52, 64, 68, 72, 78, 79 Viscoelastic, 91 viscosity, 23, 35, 36

W walking, 63 water, 41 WS model, 64, 65, 70, 72, 73, 74, 77, 78, 80, 84, 85

X X-ray, 22 X-ray diffraction, 22

104

Index

Y

yield, 17, 80

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close